Preface Welding: The Permanent Bond Between Two Solid Bodies What a long story welding is! Seeing the light of day at the end of the 19thcentury in the mind of scientists, it passed quickly into the hands of technicians, firstof all with the oxyacetylene technique, then with arc welding and resistance weldingtechniques. Other processes (we will not quote them all in this introduction) thenfollowed and the 20th century ended with laser welding which had its origins in the1980s. However, it must be said that only since the 1950s has welding been the mainmeans of assembly, as riveting was the most used method up to that point. In fact, after abandoning this method to some extent, scientists renewed theirinvolvement in the 1930s. In France, at the time, Albert Portevin set out Les basesscientifiques de la soudure autogène and a higher education teaching programmebegan in 1931 at L’Institut de soudure. In the 1930s welding was implicated inbridge failures, notably in Germany and Belgium, then during World War II camethe failure of Liberty ships constructed in great numbers thanks to the technique ofwelding. Other later catastrophic failures affected pressure vessels. It is in thiscontext that in 1948 L’Institut international de la soudure (IIS/IIW) was founded. Itmet the need for international collaboration, in particular with regard to safety andresearch, expressed by different national bodies and by the whole welding world,from scientists to users. Today in 2008, the IIS/IIW holds its 61st annual meeting: 16commissions, with sub-commissions and study groups, cover the whole field ofwelding, from design to performance and safety, including teaching and research.This demonstrates the importance of this collaboration and the richness of itscontribution.
xiv Metallurgy and Mechanics of Welding Welding can be regarded, like the language of Aesop, as the best and worst ofthings. Indeed, it makes it possible to bond almost all materials, from metals toplastics, with continuity; however, this does not imply homogenity. The processesand hence possibilities are very numerous depending on the types of assemblies tobe made, the properties required and evident economic constraints to be respected.At the same time welding can be regarded as the weak link of the majority ofconstructions as it is often called into question when problems arise. In the examplescited above (bridges, Liberty ships, pressure vessels) it is the welding that is calledinto question each time – often it must be added linked to a parent metal whoseresistance to a sudden failure is insufficient. The phenomena that occur during welding are both numerous and complex. Inparticular, the influence of extremely rapid thermal cycles and at high temperatureon the physical, metallurgical and mechanical properties of welded materials alwaysrequires a better understanding. In order to produce this work, the multiplicity of knowledge, scientific as well astechnical, to be put in practice has led us to have recourse to a range of authors toshare the task. The disadvantage is of course a certain disparity between the variouschapters, as well as the risk of some repetitions. On the other hand, its richness isderived from this very fact as this work brings together the contributions ofnumerous French specialists well known in their specific field. It presents an entityas complete as possible on the knowledge available today on welding, without ofcourse claiming to be exhaustive (for example, the welding of the plastics is outsideits scope). In a first part of 7 chapters, which deals with metallurgy and mechanics ofwelding, Chapters 1 and 2 present all the processes of welding, from the traditionalprocesses with and without filler, with and without mechanical action, to the recentprocesses with high energy, electron beam and laser. Chapter 3 deals with the wholeof the thermal, metallurgical and mechanical phenomena, which occur in the heataffected zone (HAZ) of the base material. Here the transformation phases with allthe consequences they have on the structures and their properties are presented, aswell as the phenomena of cracking, in particular cold cracking, which is a recurringtheme of this work. Chapter 4 is similar but deals with the question of molten metal in the weld, withother phenomena of cracking that are called into play.
Preface xv The different types of filler products are then dealt with in Chapter 5 dependingon the process used. The progress made in the manufacture of these products inorder to improve the properties of the weld and resistance to cracking is explained. Chapters 6 and 7 illustrate the problems of failure in service of weldedconstructions, the former dealing with resistance to fatigue, with solutions suggestedboth for materials and for the execution of the welds, the latter dealing with brittlefailure, with, after setting out the methods of evaluation of the toughness and theevolution of the harmfulness of defects, proposals relating to the composition of theparent material, the quality of the filler metal and the importance of weldingconditions. The second part, Chapters 8 to 14, focuses on the applications of welding forvarious materials and in various industries. First of all, Chapter 8 is devoted to the welding of thin sheets, both bare andcoated, mainly used in the automotive market with the appropriate processes ofwelding. The importance of new steels with a very low percentage of carbon isunderlined. The subject of Chapter 9 is the welding of steel mechanical components in theautomotive industry, with less traditional processes calling upon a minimum ofmolten metal. The welding of steel structures is the subject of Chapter 10. The steels used andthe techniques of welding with the precautions required in order to avoid defects arepresented. Chapter 11 concerns the welding of pressure vessels. It deals with examples oflarge components such as pressurized water reactors (PWRs) in the French nuclearindustry and analyzes the various processes of welding and coatings used accordingto the parts of the vessel. The majority of the preceding chapters refer to welding carbon and low-alloysteels, so Chapters 12 and 13 are devoted to other types of alloys. First of all, thewelding of stainless steels is presented in detail, and for various families(martensitic, ferritic, austenitic and austeno-ferritic) with the concomitant problemsof cracking and embrittlement, as well as the remedies and advice suggestedaccording to the processes selected. Then, the welding of aluminum alloys is tackledwith the various welding techniques used, the problems encountered and the rules torespect in order to obtain welds of good quality.
xvi Metallurgy and Mechanics of Welding Chapter 14 is devoted to standardization developments in welding dealing withthe general organization of quality and standards for non-destructive testing. We extend our thanks to all those authors who have agreed to contribute to thiswork and especially those who work in the industry and who have been willing intheir free time to contribute to this collection of the know-how and current researchin the different fields of welding. Régis BLONDEAU
Chapter 1 Traditional Welding Processes1.1. Introduction To avoid any misunderstandings, the definitions of the terms which appear inthis text are those proposed in the document entitled “Terms and definitions used inwelding and related techniques” published by the “Publications of AutogeneousWelding and the International Council of the French Language” [COL 96]. It has been specified in the preface to this book that welding makes it possible toreconstitute metallic continuity between the components to be assembled. Thisreconstitution involves the re-establishment of the interatomic metal bonding forceswhich requires at the same time a connection of the nodes of the crystal lattices andthe absence of any foreign body likely to constitute a screen. This chapter will successively cover the physical conditions necessary to createthe metallic bond and the industrial processes which make it possible to establishthis bond.1.2. Conditions to create metallic bonding Creating the metal bond consists, theoretically, of bringing the surfaces to belinked closer so that the surface atoms are at a distance of the order of the internodaldistances of their own crystalline system.Chapter written by Guy MURRY and Dominique KAPLAN.
2 Metallurgy and Mechanics of Welding This operation, which would assume at the beginning that surfaces arechemically clean and in a specular state of polish, is not practically feasible. To mitigate this industrial impossibility, the surfaces to be joined will have to beactivated with a view to eliminating the foreign bodies and elements likely toobstruct the creation of the bond.1.2.1. Activation of surfaces The most effective surface activation is fusion which can simultaneously ensuretheir cleaning. The metallic bond is created by solidification. Different procedurescan be employed: a) the two parts to be assembled undergo a surface fusion and thus contribute tothe formation of a molten metal pool (possibly with the addition of a filler) whichsolidifies without mechanical action; b) the two parts to be assembled undergo a surface fusion but an externalmechanical action expels the molten metal and creates the assembly by placing thesurfaces in contact at the solidus temperature; c) the two parts to be assembled undergo a localized fusion and take part in theformation of a captive molten metal core which during its solidification iscompacted by the action of an external effort of compression. The activation of surfaces can also be obtained by heating without fusion. Ingeneral it is then supplemented by a mechanical action which enables, moreover,cleaning and improvement in contact of the surfaces to be assembled. It is possibleto distinguish between: a) the case where the heating and the cleaning of surfaces to be assembled aresimultaneously carried out by mechanical friction (which implies the assembly ofaxisymmetric parts) and is followed, after stopping the latter, by a crushing(“forging”) by axial compression; and b) the case where the heating is carried out by external heating and the closecontact is ensured by an effort perpendicular to the joint plane. Finally, activation can result from a mechanical action without total heating ofthe parts to be assembled. This mechanical action causes a plasticization of the outerlayer of each surface and generates a very localized heating which finally allows theestablishment of the metallic bond. This process simultaneously requires a relativedisplacement of the surfaces to be assembled, parallel to the mating plane, coupledwith a compressive force perpendicular to this same plane. It is necessary to carry
Traditional Welding Processes 3out a careful surface preparation and/or to make sure that relative displacements ofthe latter cause the rejection of the products which pollute them.1.2.2. Elimination of obstacles to bond creation Obstacles to the creation of the metallic bond can be of various kinds: – geometrical surface irregularities, – pollution of the surface (oxides, grease, moisture, etc.), – chemical elements brought in by the surrounding air. Surface irregularities are likely to disrupt the creation of metallic bonds in all thecases where there is not surface fusion of the parts to be assembled. It will then benecessary to carry out a surface preparation by mechanical means (grinding,machining, etc.). All pollution of surfaces to be assembled will have to be eliminated bymechanical action (sanding, grinding) or by chemical means (solvents, scouring,drying, etc.). It is necessary to neutralize the possible effects of chemical elements brought inby the surrounding air. Welding operations generally being carried out inatmospheric conditions, it is especially oxygen, nitrogen and hydrogen (carried inthe air’s humidity) which can be harmful. Oxygen can react with the elements volatilized by the arc and in this waycontribute to the creation of welding fumes. Furthermore, it can especially dissolvein the molten metal and, during solidification, contribute to the formation of: – metallic oxides which constitute inclusions in solidified metal; – porosities in the molten metal due to the drop in solubility which accompaniescooling and solidification. This formation of porosities can be aggravated by areaction developing with an element contained in the metal and leading to theformation of a gas compound (for example, formation and release of CO during steelwelding without protection against the atmosphere). Protection against oxygen in the air can be ensured by the interposition of aneutral gas, a molten slag or by fixing in the form of oxides by the addition ofoxygen hungry elements (silicon especially). In the vicinity of the molten metal, thesurface of the parent metal raised to a high temperature can also react with oxygenand be covered with oxides, which is a further justification for using protectivemeans, including at the back of the weld.
4 Metallurgy and Mechanics of Welding Nitrogen can dissolve in the molten metal and contribute to: – either the formation of porosities in the molten metal due to the drop insolubility which accompanies cooling and solidification; – or the formation of metal nitrides which, according to the conditions in whichthey appear, constitute inclusions or precipitates more or less hardening andweakening in nature; – or for the part which remains in solid solution, a process of weakening byageing. Protection against nitrogen can be ensured by interposing a neutral gas or amolten slag. Hydrogen dissolves in the molten metal and its concentration can reach highlevels, even reaching saturation if precautions are not taken to limit its presence.Hydrogen, the solubility of which decreases when the temperature drops, can thencontribute to the formation: – of porosities during solidification; – of cracks, in a solid state, when, oversaturated, it gathers in the form of gasmolecules on the structural defects of a not very ductile metal. Protection against hydrogen primarily consists of limiting its introduction intothe molten metal by lowering the atomic or ionic hydrogen content of the plasmaarc. To do this it is necessary to minimize the water content of the surrounding air(no welding in a damp atmosphere), to interpose a gas low in hydrogen between thesurrounding air and the arc, to eliminate compounds supplying water (hydroxides,condensation, greases, basic non-dried coatings, fluxes, etc.) and other sources ofhydrogen (cellulose or rutile coatings and grease).1.2.3. How can we classify the various welding processes? At this stage we are led to adopt a system of grading the welding processesaccording to the modes of action and means of protection against the atmosphere(see Table 1.1).
Traditional Welding Processes 5 Activation Complementary action Protection none imperative fusion compression not essential heating compression possible friction compression none Table 1.1. Classing the welding processes according to modes of action and means of protection against the atmosphere Actually, the various welding processes are above all classified according tomore practical criteria, which are: – the energy source applied: flame, electric arc, plasma, Joule effect, spark,induction, friction, explosion, etc.; – the means of protecting the hot metal: gas or slag.1.3. Industrial welding processes Industrial welding processes are set out here according to the criteria definedabove, namely: – processes utilizing the fusion without mechanical action; – processes utilizing the fusion combined with mechanical action; – processes utilizing heating without fusion but with a mechanical action; – processes utilizing a mechanical action without heating. A classification akin to industrial practices will be presented at the end of thischapter.1.3.1. Processes using local fusion of the parts without mechanical action For welding processes operating without voluntary mechanical action, the localfusion of the parts to be assembled can be described by distinguishing the mode ofheating used and the means of protecting the molten metal against the chemicalaction of the surrounding air. Thus, it is possible to list: – flame or gas welding; – plasma welding;
6 Metallurgy and Mechanics of Welding – arc welding; – vertical electroslag welding; – aluminothermic welding. It should be noted that, in all these processes, the molten metal weld pool iscontained in a crucible formed by the shape of the parts to be assembled adjacent inthe mating plane (sometimes the complete closure of the “crucible” is ensured byspecific tools, e.g. slat, slides, mold). In this way a non-molten section of the parts,in the vicinity of the molten metal, is brought up to temperatures, according to itsdistance from the latter, between the temperature of the solidus of the metal and theinitial temperature of the parts. The fraction of this volume (nearest to the moltenmetal), of which the structure and therefore the properties change because of thisheating, is called the heat affected zone (HAZ).22.214.171.124. Flame welding Figure 1.1. Fusion of parent metals and filler metals obtained with a blowtorch The fusion of the parent metals and the filler is obtained by heating with ablowtorch (Figure 1.1) which enables us, by combustion of a gas (acetylenegenerally, hydrogen, propane) with a comburent (which is generally oxygen), tohave an effective flame (of a fuel rating, with acetylene, about 100 to 300 W/cm2 ona spot of heating [RYK 74], the diameter of which is about 5 to 10 cm). This flame comprises two zones, each with a specific role: – a cone at the immediate exit of the blowtorch nozzle whose surface constitutesthe site of primary combustion (this, if acetylene is used, releases hydrogen andcarbon monoxide). At the tip of the cone the temperature is very high (usingacetylene, it exceeds 3,000°C) and the atmosphere is reducing; – a plume where combustion is completed. According to the adjustment of theconsumption ratio, namely the ratio r = volume of oxygen to volume of acetylene,this plume can be oxidizing, neutral or reducing (and thus carburizing for steels). Inwelding a neutral flame is used corresponding to 1 r 1.2. The adjustment ofblowtorch power is made by regulating the flow of acetylene which is governed by
Traditional Welding Processes 7the nozzle diameter. Four nozzle sizes exist which give acetylene flows rangingfrom 10 by 63 l/h to 1,000 by 4,000 l/h. The flow of oxygen is regulatedaccordingly. This choice of acetylene flow takes account of the metal being welded,its thickness, the type of joint and the position of welding. It is possible to add a filler metal which is generally the same composition as themetal being welded and comes in the form of rods (from 1.6 to 5 mm in diameter). Thus, the blowtorch, from the temperatures reached, allows the fusion of metalsand, by its atmosphere, ensures the molten metal is protected against any chemicalreaction with gases in the surrounding air. However, with metals that are very sensitive to oxidation (aluminum, stainlesssteel, copper alloys) it is necessary to use a flux (spread out over the edges requiringwelding or incorporated with the rod) to eliminate oxides formed on the surface.126.96.36.199. Plasma welding Figure 1.2. Plasma non-transferred arc welding Fusion is carried out by heating using a plasma jet. This plasma is generated bythe passage of a known plasma-producing gas (argon, with the possible addition ofhydrogen or helium) in an electric arc created in the annular space formed between acoaxial nozzle and a refractory electrode (Figure 1.2). Generally, in DC, therefractory electrode is negative to avoid its destruction by the bombardment ofelectrons. The recombination in the jet of ionized species in the arc releases greatenergy and as a result generates a very significant rise in temperature which exceeds
8 Metallurgy and Mechanics of Welding10,000°C. The specific power can vary from 500 to 10,000 W/cm2 on a heating spot[RYK 74] whose diameter varies from a few millimeters to a few centimeters). Aperipheral tube ensures the distribution of an inert gas (generally argon or argonmixture + hydrogen) for the protection of the molten metal. This procedure, called anon-transferred arc or blown arc, is reserved for the assembly of relatively thincomponents. Figure 1.3. Plasma transferred arc welding The transfer of heat and therefore thermal efficiency is improved by striking thearc between the refractory electrode and the parts to be assembled. The arc is thenmaintained by a pilot arc which is created between the nozzle and the refractoryelectrode (Figure 1.3). The name given is plasma transferred arc welding. It is theprocedure most commonly used in welding. It makes the assembly of thickerproducts possible (albeit with a variable limit depending on the nature of the basemetal, but in the order of a centimeter), often by using the keyhole procedure; theplasma jet crosses the joint by pushing the weld pool backwards where solidificationoccurs (the faces to be welded can thus be straight edged). In this way completepenetration is ensured and regularized. The use of a support at the back of the weldis generally not necessary because the molten zone is quite narrow (although thisdoes not obviate the need for gas protection at the back). However, this process isnot suitable for carrying out a filler pass. It is generally employed in flat welding andsometimes in horizontal/vertical welding. A filler can be introduced in the form ofwire. To increase the rate of deposit, it can be beneficial to use the hot-wiretechnique. However, the filler can also be introduced in the form of powder into theshielding gas jet (thus around the plasma jet).
Traditional Welding Processes 9 The synchronized generation of electric power pulses in the arc and in theplasma-producing gas flow makes it possible to weld in a vertical position. Such aprocedure requires computerized control of all the parameters.188.8.131.52. Arc welding The contribution of heat used to form the molten weld pool is assured here by anelectric arc operating in DC or AC. The specific power can vary here from 103 to 105W/cm2 on a heating spot [RYK 74] whose diameter varies from a few millimeters toa few centimeters. It must be possible for the arc to be generated easily and then remain stable. Tofacilitate its generation (which will allow us to avoid resorting to a too high startingvoltage compared to the arc’s voltage in permanent mode) as well as to stabilize it,we have recourse to easily ionizable chemical elements which are introduced intothe plasma arc. These elements can come from the fusible and volatile compoundsincluded in the solid products which will form the slag or from gases applied toprotect the molten metal. In addition, the power source must be adapted so that: – its non-load voltage is high enough to allow arc generation, – its normal operating voltage makes it possible to achieve arc lengthscompatible with the technology employed, – its voltage in the event of the arc’s extinction is sufficient to allow the arc to berestored. The choice of polarity, in either AC or DC, must take account of the differentphenomena which occur at the cathode and the anode. Indeed, electron emissiontakes place at the cathode and all the more so if the cathode is heated to a hightemperature. However, if its heating is partially due to the direct Joule effect and thebombardment by the positive ions, it is above all due to the contribution of heatcoming from the Joule effect which occurs in the cathode’s transition zone. This lastpoint explains why the required current depends on the diameter of the cathode; thegreater it is, the higher the current must be to maintain the cathode at a sufficienttemperature. Electrons bombard the anode and thus cause significant heating, increasedfurther by the Joule effect in the anode’s transition zone. If the arc uses DC, the choice of polarity depends especially on the process andthe metal being welded, given that the anodic zone is heated more than the cathodiczone. The AC current supply makes it possible to alternate the phenomena at the twoends of the arc.
10 Metallurgy and Mechanics of Welding When the filler comes from a consumable electrode, the transfer of this metal inthe arc can be achieved in three different ways according to the electric mode of thearc. At high currents, the transfer takes place by pulverization, i.e. in the form ofsmall droplets forcibly projected by the electric field towards the weld pool. At moderate currents the transfer takes place in the form of large droplets which,with little force applied to them, follow irregular trajectories before falling in themolten metal or, possibly in the form of projections to one side – which is generallya sign of a bad adjustment of the welding parameters. At the lowest currents thetransfer takes place by short-circuit. The magnetodynamic effect is insufficient (thecurrent is too low) to detach the droplet from the surface of the electrode; the dropletgrows bigger to the point that it comes into contact with the molten metal. The short-circuit then generates a current surge which detaches the droplet, which isincorporated in the molten metal. The products that ensure the protection of the molten metal can, according to theprocess, be: – fusible compounds which form a slag floating on top (and are likely to reactchemically with it to refine its composition); – often inert gases (argon, helium or mixtures sometimes with the addition ofhydrogen) with, sometimes, the addition of carbon dioxide (whose decomposition inthe arc will give protective carbon monoxide and oxygen which will be fixed byelements introduced with the filler products). In this context, many processes have been developed that can be classifiedaccording to the conditions in which the arc is struck (between the two parts to beassembled or these components and an electrode) and that can also be distinguishedaccording to the conditions in which the welding products are applied.
Traditional Welding Processes 11 Rotating Figure 1.4. Rotating arc welding on pipesa) The arc is struck between the two parts to be assembledArc welding with pressure created with a magnetic field The arc is struck and moves between surfaces to be joined under the effect of apermanent magnetic field judiciously directed and controlled. After surface fusion,the parts to be joined are forced together (there is thus the formation of a seam). Analternative to this process is applied to tubular structures (Figure 1.4) using two coilswhich surround the tube and create two antagonistic magnetic fields. The resultingfield is radial; it thus causes the rotation of the arc in the mating plane. This isrotating arc welding.Arc welding of studs The arc is formed between the end of the stud and the target zone of the support.After fusion of the stud end and creation of a molten pool on the surface of thesupport where the stud is to be fixed, the stud is plunged in the molten metal andmaintained in position until solidification is complete. The power supply and studdisplacement (contact, withdrawal for striking the arc, maintenance then lowering –Figure 1.5) are controlled automatically. The protection of the molten metal isgenerally ensured by the positioning of a refractory containment ring which ensuresalso the “molding” of the molten metal during its solidification. The power source
12 Metallurgy and Mechanics of Weldingcomes from DC or capacitor discharge; the current intensity of the arc is adjustedaccording to the diameter of the stud.b) The arc is struck between a fusible electrode and the components to be assembled Generally, this procedure allows, with each operation, the deposit of a certainquantity of molten metal, a quantity which varies with the type of process andenergy brought into play. It can prove insufficient to form a sufficient seam sectionbetween thick components; it is then necessary to carry out several operations i.e.several passes. Such a situation often requires an edge preparation to be performed,a preparation which ensures proper weld creation (access for the electrode, type ofassembly, position, penetration, possible prevention of deformations, etc.). Thesepreparations have shapes and dimensions which vary especially according to thenature of the base metal and the process employed. The principal varieties are: – straight edged (Figure 1.6a) for assemblies of limited thickness, possibly withspacing between the edges (distance increasing with the thickness). It may benecessary to carry out a pass on the reverse to ensure penetration but it is alsopossible to use a support at the back; Figure 1.5. Stud arc welding
Traditional Welding Processes 13 – V-shaped chamfer (Figure 1.6b) or Y-shaped (Figure 1.6c) with heel andpossible edge spacing. This type of preparation is not employed for thickcomponents because it gives rise to considerable distortion; – X-shaped (Figure 1.6d) with heel and possibly edge spacing. This type ofpreparation requires access to both sides but limits distortion; – asymmetric U-shaped (Figure 1.6e) or, better symmetric (Figure 1.6f) if thereis access to both sides (with heel and possibly edge spacing). This preparation makesit possible to reduce the quantity of molten metal necessary. Sometimes particular preparations such as half-V shaped, half-U shaped (knownalso as J), K-shaped, etc. are used. The processes which will be described are known as “semi-automatic” if theelectrode or the torch is handled by the welder and “automatic” if the latter ispositioned and guided by automated devices. Figure 1.6. Edge preparations
14 Metallurgy and Mechanics of Welding Figure 1.7. Coated electrode arc weldingCoated electrode arc welding The electrode consists of a metallic core (whose diameter varies from 1 to 10 mmand whose length can be up to 450 mm) which serves as the electrical conductor andsupplies the filler metal, as well as an adhesive coating made up of products whichcontribute to the formation of a protective slag and others that volatilize in the arcplasma to stabilize it and, possibly, of metal particles which help form the moltenweld pool (Figure 1.7). This coating can commonly be: – cellulosic: this creates little slag but its combustion releases CO2 andcontributes to the enrichment of the molten metal caused by dissolved hydrogen; – rutile: the basic component is titanium oxide; it contributes to thedesulphurization of the molten metal; the binding agents used release hydrogen; – basic (electrodes used in steel welding): the basic component is calciumcarbonate; it releases little hydrogen but it is hygroscopic and so requires that theelectrodes be correctly baked (300°C approximately) then protected (by maintainingthem at around 100°C for example) before use. Rutilo-basic mixed coatings (better desulfurization) or rutilo-cellulose (goodpenetration) are also proposed as well as coatings containing metal powders toincrease the quantity of metal added (high-output electrodes) or to introducealloying elements.
Traditional Welding Processes 15 Core fusion slightly precedes that of the coating; it forms a crater which directsthe transfer of the filler towards the molten metal. This transfer takes place in theform of large droplets (cellulosic or basic coatings) or by pulverization (rutilecoatings). In many cases, the arc can be DC in origin (the polarity is then selectedaccording to the nature of the base metal, the coating and the welding position) but itis sometimes possible to use an AC current (in particular for steel welding). Theintensity of the current is selected according to the diameter of the electrode; it isgenerally recommended by the manufacturer. Figure 1.8. Arc welding with powdered flux Welding is in practice possible in all positions, each one requiring particularadjustments and appropriate preparation.Arc welding with powdered flux The electrode is a solid wire (approximately 2 to 10 mm in diameter) whosesupply is guaranteed by an automatic device through a torch equipped with a contacttube ensuring the power supply. Upstream of the torch (compared to the direction ofthe welding process) a nozzle in which the arc will be struck distributes thepowdered flux, part of which will constitute the protective slag, whereas the rest,covering the weld area with a layer of non-molten flux which slows down cooling,will be recovered later on. The arc is not visible, so consequently this imposes aprecise piloting of the torch displacement.
16 Metallurgy and Mechanics of Welding This process (Figure 1.8) makes it possible to weld with high currents and a highoutput. However, in general, dilution is significant, about 2/3 and it increases withthe welding current. The arc is struck using DC when the welding intensity does not exceed 1,000 A;the polarity can be direct (the wire is negative) if deep penetration is required orinverse (the wire is positive) if, on the contrary, a high welding speed and areduction in dilution is desired. With elevated currents it is sometimes easier to useAC, which makes it possible to decrease the effects of magnetic arc blow. The Joule effect along the length of wire electrode, between the contact tube andthe arc, heats the filler metal (all the more depending on length and current) andfacilitates its fusion, thus increasing the quantity of filler metal in the weld pool. Fluxes used are mixtures of mineral compounds (generally silicon manganese orsilico-alumino-calcic compounds) delivered in the form of calibrated pellets. Thetwo principal manufacturing processes give them different properties: – so-called molten fluxes are manufactured from minerals by fusion, molded andthen crushed; they thus have a vitreous and/or crystallized structure and can beporous; – so-called agglomerated fluxes are manufactured starting from natural mineralproducts agglomerated or sintered (with a binder). These fluxes can adsorb or absorbwater and so it is necessary to take precautions to avoid any addition of hydrogen. In general, the manufacturers of welding products combine flux and filler metal.Each combination often makes it possible to confer their own specific properties onthe molten metal. This welding process, due to the method of flux application, enables only flatwelding (and possibly at an angle with a special support). It allows straight edgedbutt welding with edge spacing up to significant thicknesses (depending on the basemetal) but to weld very thick components it requires a preparation which account forthe possibility of making a pass(es) on the reverse side: – no access: V-shaped preparation with heel, spacing and support at the back ortulip-shaped preparation or U-shaped with heel; – access: X-shaped with heel and spacing or K-shaped preparation with heel. Furthermore, welding can be accelerated by associating two (or more) weldingheads each with its own power supply; the electrodes are generally placed in tandemat a distance of about 25 to 35 mm.
Traditional Welding Processes 17 Figure 1.9. MIG-MAG weldingGas shielded arc welding with a solid fusible wire The electrode is a solid wire (from approximately 0.5 to 2.4 mm in diameter)whose supply is ensured by an automatic device through a torch equipped with acontact tube ensuring the connection to the power supply. This torch comprises an annular gas delivery which will ensure the protection ofthe molten metal. This gas can be of two types (Figure 1.9). It can be inert and theprocess is then known as MIG (metal inert gas) welding. It can be argon (pure ormixed with helium) which ensures good arc stability and gives a good penetration,or helium mixed with argon; the proportion of argon must be high enough topreserve arc stability. It can be active and the process is then known as MAG (metalactive gas) welding. In this case it contains oxygen and, more often, CO2 mixed withneutral gases (argon mainly). The presence of oxygen (whether supplied or comingfrom the break up of CO2) brings a certain number of advantages: the arc is morestable, the weld pool more fluid, the transfer by pulverization can be establishedover a broader range of power supply conditions, the chamfers are filled better andvoids less likely. However, the risk of loss of elements transported in the arc leads tothe introduction of elements likely to combine with oxygen into the wire electrode. The power is generally supplied in DC and in inverse polarity (positive wireelectrode) in order to increase the speed of wire fusion and to stabilize the mode oftransfer, in the arc, of the molten metal. Two modes are mainly used: – the transfer by axial pulverization for the welding of thick products but limitedto butt and flat angle welding or gutter welding; – the transfer by short-circuit which involves little energy and allows welding ofthin products and all types of in situ welding.
18 Metallurgy and Mechanics of Welding Certain modern equipment makes it possible to superimpose pulses over thebasic current in order to cause the detachment of the drops at fixed frequency andthus to stabilize their size. It then becomes possible to control their transfer and toregulate their flow whatever the welding current. The term used is pulsed welding. Assemblies are made with all the preparation types already evoked but takingaccount of the need to allow sufficient access for the torch. This access can befacilitated by lengthening the wire electrode between the contact tube and the arc,with a resultant increase in the quantity of metal deposited in consequence of theheating by Joule effect in this length of wire and, generally, reduction in penetration.Welding can be carried out in all positions after adaptation of operationalparameters. Figure 1.10. Cored wire arc weldingCored wire arc welding This process (Figure 1.10) is derived from gas shielded solid wire arc welding bya simple replacement of the solid wire with a flux cored wire (diameter from 1 to 4mm). A cored wire consists of a tubular metal envelope filled with a powder (flux)whose composition and role are comparable with those of the coating on a coatedelectrode. According to the manufacturing process of cored wire, this can be closed(by drawing of a hollow cylindrical wire filled with flux) or formed by pleating orcrimping and thus more or less sealed (but it can again comprise two parallel fillingscontaining flux and a metal filler powder). As the fluxes are hygroscopic and themetal sheath more or less sealed, it is necessary to take the same precautions for useas for coated electrodes. However, cored wires without slag (and thus containing
Traditional Welding Processes 19metal powders) enable us, with an effective gas protection, to appreciably increasethe welding speed and the quantity of metal added. As in MIG or MAG welding, the supply of the wire is guaranteed by anautomatic device through a torch equipped with a contact tube ensuring the powerconnection. This torch makes an annular gas supply possible, which will ensureprotection of the molten metal. This gas is generally reactive (CO2, possibly mixedwith argon). The filled wire being more rigid than solid wire makes it possible to furtherincrease the length of the wire electrode between the contact tube and the arc andthus to facilitate access (it is necessary to avoid over lengthening this distance so asnot to separate the molten metal too much from the shielding gas). Assemblies are made with all the types of preparation already evoked by takingaccount of the improved accessibility given by the increased length of the wireelectrode between the contact tube and the arc. This makes it possible to reduce thechamfer openings. In addition, the good penetration makes it possible to increase theheight of the heels and to decrease the spacing between surfaces to be assembled.Welding is generally carried out on the horizontal and sometimes in other positions,in which case, a small diameter cored wire is used. Cored wires are also offered for welding without a shielding gas. Protection isthen assured by both the slag (of which the limited quantity is not sufficient toensure total protection) and by a dense atmosphere generated by specific productsintroduced into the flux. In addition, the metal sheath of the filled wire containselements likely to decrease the harmful effects of an incomplete protection(deoxidizers and denitrifying agents). Finally the welding parameters are adjusted toreduce the length of the arc. These cored wires make it possible to decrease the sizeof the welding torch, to facilitate access and thus limit the preparation required. Figure 1.11. TIG (tungsten inert gas) welding
20 Metallurgy and Mechanics of Weldingc) The arc is struck between a refractory electrode and the components to beassembled The non-consumable electrode consists of a tungsten tip (Figure 1.11) held in atorch equipped with an annular gas delivery which will ensure the protection ofmolten metal. This gas is neutral: argon (sometimes with the addition of hydrogen –up to approximately 30%) or helium. Argon gives good arc stability but heliumensures better thermal efficiency and thus deeper penetration. These considerationsmean that argon-helium mixtures (about 80% Ar and 20% He) are often used. Thisprocess is most commonly called TIG (tungsten inert gas) welding. It can benecessary, depending on the base metal, to set up a gas protection on the reverse sideusing a gas which can be either identical or different from that supplying the torch(nitrogen-hydrogen). The electrode (0.5 to 10 mm in diameter) can be pure tungsten or tungsten withan addition of zirconium oxide (0.3-0.5%) or thorium (1-2%). These additions makeit possible to increase the electrode emission capacity and thus to improve arcstability and help arc initiation. They also increase the electrode performance andthus the acceptable maximum current. The shape of the electrode point is asignificant parameter of TIG welding. The electrode is often pointed in DC mode,and hemispherical in AC. The power supply is generally DC with direct polarity (negative electrode) so asnot to subject the electrode to electron bombardment. In this way the energy impactis concentrated on the parts to be assembled and at the same time a narrow bead andgood penetration are achieved. The arc can also be established by AC (with asuitable power source) when an electronic bombardment is desired to clean the partsto be assembled. Arc initiation is often assisted using a pilot arc. A filler can be introduced directly into the molten metal pool either in the formof rods or in the form of wire using a mechanized reel, allowing, if necessary, thepre-heating of the wire to improve the deposit rate. Assemblies are produced using all the preparation types already evoked abovetaking account on the one hand of the limitation of the volume of molten metal and,on the other hand, of the need for taking particular care (cleanliness, dimensionalaccuracy especially with regard to the spacing of the parts – it can be useful to set upa support on the reverse side). Welding can be carried out in all positions afteradaptation of the operational parameters. An easier use of the TIG process and an increase in penetration can be obtainedby applying a fine layer of a reactive flux to the surface of the edges to beassembled.
Traditional Welding Processes 21 The composition of this flux (often formed of oxides and/or halides) must beselected according to the nature of the base metal. Figure 1.12. Vertical electroslag weldingVertical electroslag welding This process consists of forming a molten metal bath in a verticalparallelepipedal mold formed by the two sections to be assembled and two water-cooled copper shoes applied to the surface of the two parts (Figure 1.12). Thecontinuous supply of molten metal due to the filler fusion (consumable wireelectrode and possibly fusible wire guide) and the progressive solidification of themolten metal little by little consolidate the two parts. Above the molten weld pool, abath of slag (thickness 40 to 60 mm) ensures its protection. The permanent heatingis due to the Joule effect which develops partly in the electrode but especially in thismolten mineral pool. Welding progresses vertically upwards. It begins with thestriking of an arc between the wire electrode and an appendage which closes thebottom of the mold and on which a welding flux is deposited (which will form theslag). When the volume of molten metal is sufficient, the quantity of flux necessary toconstitute the slag layer is introduced; the arc then ceases. It is generally preferableto set up, in the edge prolongation to be assembled, two blocks of the same
22 Metallurgy and Mechanics of Weldingcomposition as the base metal and of the same thickness. The weld’s end point willbe after the molten metal has reached the level of these blocks so that the shrinkageat the end of solidification does not affect the weld per se (any surplus deposit thuscreated will be removed later on). According to the dimensions of the parts to beassembled, the side shoes can be moved upwards to follow the progression ofwelding. The heat affected zone is wide, because of the very significant heat generation.According to the thickness of the parts to be assembled several wire electrodes canbe used simultaneously. To carry out welds of considerable height, a fusible wireguide plunged in the slag and melting simultaneously the wire electrode(s) can beemployed; this fusible wire guide contributes to the molten metal weld pool. Theterm then employed is vertical electroslag welding with fusible wire guide. Theprocedure generally makes use of AC. This process allows butt welding and welding at an angle (by using adaptedshoes) of work pieces whose thickness is generally not less than 40 mm.Aluminothermic welding In this process the welding is carried out by running a metal in fusion (filler) intoa mold built around the two faces of the parts to be assembled, placed face to face, ata specified distance. These two faces are often pre-heated with a flame via holesprovided in the mold. The molten metal is created on the spot by aluminothermy, i.e.exothermic reaction between oxides (of the metal filler) and powdered aluminum.This operation is carried out in a crucible placed at the top of the mold. As themolten filler is run in, the surface of the parts to be assembled melts, precedingsolidification of the assembly. The protection of the molten metal is ensured by theslag which is formed during the aluminothermic reaction. Afterwards, it is necessaryto remove the mold and grind the assembled parts, so as to eliminate any excessdeposits.1.3.2. Processes using local fusion of components with mechanical action The contribution of heat used to form the molten weld pool is assured here by theJoule effect of a high intensity alternating current which crosses the mating plane. Itis the contact resistance between the two surfaces of the parts to be assembled whichmakes it possible to concentrate fusion in this plane. Several processes have been developed that we can classify according to the fatereserved for the molten metal; containment or expulsion. All require rather heavyand specific equipment.
Traditional Welding Processes 184.108.40.206. Resistance welding with containment of the molten metal This process combines the Joule effect and a mechanical pressure applied to theoutside of the assembly, perpendicular to it and right where the molten metal zoneis. This force has the aim of ensuring a good electrical contact between the parts tobe assembled, thereby confining the molten metal in the zone where it is formed andapplying pressure to it after its solidification in order to improve its compactness byavoiding shrinkage (an operation known as spot forging). Generally the electrodescarrying the current apply this effort. These considerations show that they areoverlapping assemblies of products of limited thickness. The containment of themolten metal within the joint avoids any contact with the air; the problem of itsprotection thus does not arise. The effectiveness of this process is related to the localization of the zone heatedby the Joule effect, which depends on the electric contact resistance between theparts; precautions must be taken so that, on the one hand, other resistances in seriesin the electric circuit are much lower and that, on the other hand, there is nopossibility of the welding current being diverted to one or more parallel circuits. The piloting of the welding current as well as that of the compression force arehandled by automatisms which can: – apply pressure before the passage of the current, to bring the two componentsinto close contact and to ensure the electrical contact, – adjust the current intensity and limit its duration (in general, of a few periods toa few tens of periods i.e. durations which are calculated in tenths of a second), – adjust the pressure during the passage of the current to prevent the surfacesseparating (due to dilation) and the consequent dispersion of the molten metal, – maintain or increase the effort to ensure the compactness of the volume ofmolten metal, – if required, run a reduced current as a post-heating. The electrodes are copper-based alloys. The addition of alloying elements (Cr,Zr, W, Cd, Co, Be, etc.) confers the necessary mechanical performance withoutoverly affecting their electric conductivity and thermal conductivity. Their contactsurface to be welded must be clean and uniform in shape.
24 Metallurgy and Mechanics of Welding Figure 1.13. Resistance spot welding In this way resistance spot welding, projection and roller seam welding can becarried out.Resistance spot welding In this process current supply and load application are carried out by cylindricalelectrodes with tips in the shape of a truncated cone cooled by internal watercirculation. Their contact surface is generally flat or slightly convex. They areinstalled on fixed machines or mobile tools; it is always desirable that the step-downcurrent transformer is placed as close as possible to the welding zone. The volume of molten metal has an ovoid form and is called a spot weld. Thewelding is discontinuous and a seal cannot be guaranteed. The final load applicationgenerally causes an indentation on the two faces of the joint; it is possible to avoidon one of the two faces by replacing the electrode with a copper plate through whichthe welding current passes. Figure 1.14. Projection welding
Traditional Welding Processes 25 It is possible, in certain cases, to carry out two spot welds simultaneously bycoupling two transformers (double spot in series with push-pull assembly), or withonly one transformer (provided that it is possible to control the currents).Resistance projection welding In this welding process (Figure 1.14), the passage of the current is localized byraised areas called projections created on one or both of the assembly surfaces.These bosses are stamped on thin flat sheets and machined in other cases. Thesupply of the current and the load application are applied, generally, using plates;during the heating and fusion the bosses collapse and the mobile plate must reactvery quickly to ensure the close contact of the parts to be assembled. If the powersupply is powerful, it is possible and economic to weld several bossessimultaneously. The wear of the plates and deformation of the components areminimal. The geometry of the projections must be precisely controlled.Roller resistance welding In roller resistance welding (Figure 1.15), the electrodes are replaced by copperor copper alloy discs called rollers. These rollers are driven to ensure theprogression of the components. Of course, they carry the electric current and applythe necessary load. The electric current, in general, is modulated as in spot welding but in arepetitive way and the welding consists of successive spots. It can be: – discontinuous if the successive spots do not overlap. It is possible to stop theroller rotation at each spot and to carry out spot compression, and the result isidentical to that of spot welding. It is also possible to work uninterrupted but in thiscase without forging (the effort applied remains constant), – continuous if the various points overlap, i.e. if the formation of each pointinvolves the partial remelting of the preceding spot. The welding then forms aperfect seal. It is possible, in roller welding, to carry out the seam welding of thin sheets usingthe force applied during welding; the extra thickness is then eradicated. It isnecessary, to achieve this, that the overlap does not exceed one and a half times thethickness and that the sheets to be assembled are gripped very tightly.
26 Metallurgy and Mechanics of Welding Figure 1.15. Roller resistance welding220.127.116.11. Resistance welding with expulsion of the molten metal These processes combine the Joule effect with applied mechanical pressure, afterheating, from outside of the assembly and perpendicular to it, over all its surface.This force has the aim of creating the bond by keeping in close contact the surfacesheated to their solidus temperature. A weld metal bulge is formed at the ends of theassembly, which must then be eliminated. As the heated zone is confined, theproblem of its protection is not relevant. Within this framework two rather differentprocesses are employed.Upset resistance butt welding The effort is applied in two stages: first of all for the cold joining of the parts inorder to allow the passage of the current through the surfaces to be assembled, then,after passage of the current, to ensure the weld bond; an excess, or weld bead, isformed which must be eliminated. The Joule effect is limited to the contact zonebetween the two parts and the heating must bring them up to the forgingtemperature. This process is a large-scale consumer of energy and requires careful preparationof the faces to be assembled (which must be parallel and perpendicular to the effortapplied). Therefore, flash welding is sometimes preferred. An alternative used for the longitudinal closure welding of cold formed sectionsutilizes high frequency (HF) induction heating. The HF current is applied by twocontacts rubbing on the weld edges, above the intended weld, where they are stillseparate.
Traditional Welding Processes 27 Due to the skin effect, the current works its way along the edges to the contactpoint, where it generates heat (eventually to the point of fusion) and allows the bondto be formed with the pressure of two rollers. This process can be implemented eachtime it is possible to create an induced current which crosses the mating plane.Flash welding The parts are brought closer only after the current is supplied so that the currentis first of all only transmitted by contact points created by the imperfections of theopposing surfaces; at these points the current density is very high. From thebeginning of fusion the liquid part is expelled in the form of small incandescentparticles; this is the flash. Gradually this flashing takes over the whole matingsurface. Once this result is achieved the contact pressure is increased to drive out themolten metal and the impurities which it contains and to ensure the connection; thecurrent is simultaneously shut off. An excess weld bead is formed in this last phase;it will have to be eliminated. A pre-heating of large section parts limits the electricoutput and the force required. It also decreases the loss of matter during flashing butincreases the volume of the bead and the duration of the operation. This process does not require a careful preparation of the faces to be assembled;flashing alone is sufficient. In general, it is not necessary to protect the molten zonefrom oxidation in as much as the force is applied straight after the flashing. This process allows end to end welding of variously shaped components andsections (from just a few mm² to more than 1,000 cm²).1.3.3. Processes using heating without fusion but with mechanical action Heating can be achieved from an external source (resistance or induction) or bymechanical action (friction). The applied forces must be carefully controlled. Theseprocesses thus require very specific equipment.Diffusion welding Diffusion welding is a process of solid state coalescence in which the parts to beassembled, put in contact under suitable pressure, are brought up to and maintainedat a sufficiently high temperature (but very slightly lower than the melting point) toallow atom diffusion through the mating plane. This, helped by localized plasticdeformations, can ensure metal continuity. The pressure can be: – perpendicular to the mating plane: it is then often recommended that to avoidmacroscopic deformation, it does not exceed the limits of elasticity of the metal atthe diffusion temperature,
28 Metallurgy and Mechanics of Welding – isostatic: the pressure is in this case not limited and the resorption of porositiesis greatly improved. The surfaces to be assembled must have undergone a careful preparation by finepolishing (to ensure the closest contact possible) and cleaning (to eliminate anypollution likely to obstruct the diffusion). It is possible to insert one or more non-fusible leaves (strip iron or deposit) between them. Precautions must be taken to avoid any hot reaction of these surfaces with theatmosphere (vacuum welding or in a neutral atmosphere). For a given preparation,the quality of the assembly depends on the pressure, the temperature and theduration of maintenance at temperature. It has been shown [LEF 92] that fast localized heating by induction under ajudiciously modulated axial load (so as to be at any temperature equal to thecorresponding limit of elasticity) makes it possible to achieve an assembly followinga maintenance at a temperature whose duration varies, depending on its level,between 1 and 60 seconds. The heating conditions make it possible, in addition, tocarry out a heat treatment within the framework of the thermal welding cycle. Thisprocedure is applicable to many metals.Friction welding Friction welding is a process of butt welding under pressure which involves arotation of the parts against each other (maximum circumferential speed of about150 m/min) and the application of an axial load in order to generate, by friction, heatat the interface (only one part is put in rotation; it must be circular and its diameter,if solid, can vary from a few mm to 150 mm approximately). When the requiredtemperature is reached, rotation is stopped and the axial load is simultaneouslyincreased to ensure welding by forging. The rotating part is turned by a servo motor or a flywheel. In the first casemovement stops due to disengaging and braking, in the second the stop follows theexhaustion of the flywheel’s kinetic energy (which was spun before the operation ata sufficient speed to ensure the required heating). The joint does not contain molten metal and this fact has two principalconsequences: – the joint has good mechanical properties; – it is possible to weld different metals (iron and aluminum for example). An excess bead is formed at the periphery of the joint; it must be eliminated. Thecleaning of the surfaces to be assembled is ensured by friction; this process thus
Traditional Welding Processes 29requires neither careful preparation of the surfaces nor their protection in the courseof the welding operation. If none of the two parts to be assembled can be rotated, it is possible tointercalate an adapter which can be rotated. A process which can be compared to friction welding is currently proposedunder the name friction stir welding. It employs a non-consumable rotary tool, ofsuitable shape, which penetrates the mating plane; friction causes significant heatingwhich lowers the elastic limit of the base metal. A significant plasticization developsand the tool movement (at a speed which would be approximately that used in arcwelding) causes a flow of matter running from the front to the back of the tool,where it ensures the bond between the two parts to be assembled. The properties ofsuch an assembly are interesting.Forge welding In this process the parts to be assembled are heated to a sufficient temperaturethen hammered to cause the connection by plastic deformation at the interface.Between the two faces to be assembled, it is necessary to employ a cleaning product(equivalent to a flux) which ensures the elimination of oxides by ejection duringhammering.1.3.4. Processes using mechanical action without heatingUltrasonic welding This is a process of lap welding under contact pressure, during which ultrasonicvibrations (20 to 100 kHz) are briefly applied so that the two faces to be assembledare set into motion against each other. A negligible volume of metal, on both sidesof the mating plane, is thus raised (by friction) to the recrystallization temperatureand ensures the bond as a result. The ultrasonic energy required is that much greater the thicker (generally notexceeding 2 mm) and harder the components are. It is possible to weld differentmetals.Explosive welding This welding process is used to produce assemblies by covering or cladding. Thecovering or cladding metal is violently projected against the base metal by theprogressive detonation of an explosive layer distributed on its outside face. Theshock wave, as it spreads, causes the ejection, in front of the contact zone, of a jet ofmetal which perfectly cleans the faces to be assembled and enables the creation of
30 Metallurgy and Mechanics of Weldingthe bond. However, for this to occur, it is necessary that, before welding, a gap isestablished between the two faces which have been chemically cleaned beforehand.Their surface (from a few cm² to several m²) can be flat, cylindrical – tubes – orcrooked. It is possible to assemble different metals.1.4. Bibliography[COL 96] COLLECTIF, Termes et définitions utilisés en soudage et techniques connexes, Publications de la Soudure Autogène, 1996.[LEF 92] LEFRANCOIS P., KERGOAT M., CRIQUI B., HOURCADE M., “L’assemblage de l’acier en quelques secondes grâce au soudage-diffusion-dynamique à l’état solide: cas du 27CD4 soudé à 1050°C”, Mémoires scientifiques de la Revue de Métallurgie, January 1992.[RYK 74] RYKALINE N.N., “Les sources d’énergie utilisées en soudagé”, Soudage et techniques connexes, December 1974.
Chapter 2 High Density Energy Beam Welding Processes: Electron Beam and Laser Beam Welding processes using high density energy beams result from the application,in the second half of the 20th century, of work conducted by physicists in the fieldsof x-rays and vacuum techniques for the process of electron beam welding andoptronics for laser beam welding. The possibility of concentrating these beams onpoints having a very small surface area led engineers to use this property to meltmaterials to achieve welds or cuts. Compared to traditional arc welding processes, these two processes arecharacterized by a very high energy density at the impact point on the work piece.Rykaline [RYK 74] gave a representation comparing for several processes the heatflows at the center of the heat sources and the diameters of these sources. We canobserve that the energy density measured at the focal point of a laser beam or anelectron beam is 10,000 times higher than that reached in an oxy-fuel flame (seeFigure 2.1).2.1. Welding properties using high density energy beams These result from the dimension of the focal points (lower than a millimeter ingeneral) used at the level of the parts to be welded. These properties are as follows: – single pass welding;Chapter written by Abdelkrim CHEHAÏBOU and Jean-Claude GOUSSAIN.
32 Metallurgy and Mechanics of Welding – welding without filler material when there is no gap between the parts to bejoined; – welding of thin parts (tenths of millimeters) by heat conduction; – welding of very thick parts (tenths of millimeters) by the formation of a vaporcapillary. In this last case, two modes of welding are observed: - complete penetration weld using a keyhole when the electron or photon beampasses through the whole thickness of the workpiece (see Figure 2.2), - partial penetration weld when the beam only melts part of the thickness of theworkpiece (see Figure 2.2); – very narrow welds (molten zone and heat affected zone) because of the veryhigh energy density; – welds inducing very low distortion, which makes these two processes aprecision mechanical solution, since it thus becomes possible to weld machinedparts or parts not requiring deformation correction after welding. Figure 2.3illustrates the deformation (transverse and longitudinal shrinkage) obtained duringthe welding of a 15 mm thick sheet of martensitic steel by GTAW, plasma arc,GMAW and electron beam; – welds with gas protection (laser) or under vacuum (electron beam), whichensures a good protection against the oxidation of the molten zones and heataffected zones and makes it possible to weld materials sensitive to this phenomenonsuch as titanium and zirconium. Figure 2.1. Rykaline’s diagram
High Density Energy Beam Welding Processes 33 Figure 2.2. Complete penetration and partial penetration welds (Institut de Soudure document) Figure 2.3. Comparison of the transverse and longitudinal shrinkage of a butt welded martensitic stainless steel assembly (Institut de Soudure document)2.2. Laser beam welding2.2.1. History Einstein surely did not suspect the technological revolution to which hisstimulated emission theory, established in 1917, would give rise. The technologicaladventure could only really start in 1954 when Professor Townes and his teamdeveloped the first stimulated emission amplifier and oscillator, which they baptized“MASER” (Microwave Amplifier by Stimulated Emission of Radiation). Thisdiscovery was followed by many others. In 1958, Schawlow and Townesdemonstrated the theoretical possibility of producing coherent light by stimulatedemission of radiation. The first laser source was a ruby laser produced by Maiman in1960. It was very quickly followed by the development of the first gas laser byJavan (helium-neon laser). Many mediums were then studied and used for the
34 Metallurgy and Mechanics of Weldingmanufacture of lasers: doped crystals, semiconductors, ionized gases, moleculargases, liquids, dyes. Laser is currently experiencing an extraordinary development. It is used in manyspheres of activity.2.2.2. Principle Laser is an acronym formed by the initial letters of Light Amplification byStimulated Emission of Radiation. An atom can pass from a fundamental state E1 to excited state E2 by theabsorption of a certain energy quantity (h ). This energy contribution can bemechanical or kinetic in origin. This atom will revert to its fundamental state by therestitution of this energy quantity, it is “the spontaneous emission” expressed by thefollowing relation: h E2 E1where h is Planck’s constant and the emerging photon frequency. These randomly emitted photons produce a light known as “incoherent”. There isno relationship of phase, direction and polarization between all these photons. If an incident photon causes a return to the fundamental state of the excited atom,there is “stimulated emission”. The two emerging photons are in phase, they havethe same direction and same polarization as the incident photon: there is lightamplification by stimulated emission of radiation. The excitation of the medium is called “pumping”. It allows the populationinversion between excited and non-excited atoms. Pumping requires an externalenergy source which can be assured by electrical discharge or radio frequency in thecase of gas lasers, and by lamps or laser diodes in the case of solid lasers. A laser source must thus be made up of three principal elements: – an active medium made up of particles (atoms, ions, molecules), – an energy source to carry out the pumping of the medium and thus to obtainthe population inversion, – a resonator cavity made up of two mirrors ensuring photon oscillation. If oneof the mirrors is partially reflective, it will allow some of the photons to escapewhich will constitute the coherent light beam.
High Density Energy Beam Welding Processes 35 The laser beam thus obtained will have certain characteristics of divergence,polarization and energy distribution which will define the quality of the laser beam.2.2.3. Various laser types18.104.22.168. CO2 laser sources Gas laser sources are most commonly used for working on materials. The activemedium consists of a gas mixture containing helium (50%), nitrogen (40%) and CO2(10%). Pumping is carried out by electrical discharge or more often by radiofrequency. The excited nitrogen molecules transfer their excitation to the moleculesof CO2. The radiation wavelength of 10.6 m thus obtained does not allow thetransport of the beam by optical fiber. Only transport by mirrors, a less flexiblesystem, is possible. In spite of the possibility of pulsing the beam, welding mainlyuses CO2 in a continuous mode of operation. The electrical efficiency of such lasersources is lower than 10%. The search for increasingly powerful laser sources with a better beam quality andbetter efficiency have led to the development of various technologies. Those differin the direction of gas circulation, the type of excitation and the shape of the cavity.We can distinguish five.Sealed laser sources These consist of a discharge tube containing the gas mixture. They are limited inpower ( 600 W) but deliver a very good quality beam. In the field of metallicmaterials, they are particularly well adapted to engraving and cutting thin sheets.However, their good beam quality also enables them to be used for the welding ofthin strip iron. Advantages of such sources rest in their low cost and the possibilityof installing them on mechanized systems.Slow axial flow laser sources These are the first CO2 laser sources to have been developed. The gas circulatesslowly in the tubes in the axis of the laser beam (10 m/s). The excitation of gas isensured by electrical discharge. These laser sources produce a very good qualitybeam but their power per unit of volume is limited to 0.5 W/cm3. The maximum power of these laser sources is low ( 1,000 W). They can be usedfor cutting and welding thin materials.Fast axial flow laser sources The gas moves at high speed in the beam’s axis ( 200 m/s) using pumps orturbines in the cavity made of glass tubes. The excited gas is then cooled by heat
36 Metallurgy and Mechanics of Weldingexchangers and progressively regenerated. The excitation can be obtained byelectrical discharge but the most recent sources use radio frequency. This mode ofexcitation has several advantages: – more homogenous excitation, – the electrodes placed externally suffer less and their maintenance does notrequire the opening of the cavity, – greater flexibility in use. The power obtained per unit of gas volume can reach 2 to 3 W/cm3 for anexcitation by electrical discharge and from 8 to 10 W/cm3 for excitation by radiofrequency. Increasingly compact laser sources are obtained by reducing the cavityshape. Sources of 20 kW are proposed in today’s industrial market. These are the laser sources most commonly used today. They equip cutting andwelding machines.Transverse flow laser sources The gas flow moves transversely across the axis of the laser beam thanks to oneor more turbines. They do not use glass tubes. The cavity consists of a sealed metalchamber. The power per unit of gas volume is about 2 to 3 W/cm3. The maximumpower reached is high (up to 45 kW). The laser beam obtained is of lower qualitythan for a fast axial flow laser. Such beams are mainly used for welding or surfacetreatments.So called SLAB laser sources The parallelepipedic cavity generates a rectangular beam configuration. Thebeam then passes into a spatial filter which makes it circular. The gas moves slowlyin the cavity. The excitation of gas is carried out by radio frequency. The poweravailable lies between 100 W and 6 kW. This technology makes it possible to obtaincompact sources of a higher efficiency. Gas consumption is low and the beamobtained is of very good quality (close to Gaussian beam TEM00).22.214.171.124. Neodymium YAG laser sources It is a solid-state laser whose active medium is yttrium aluminum garnetmonocrystal doped with neodymium ions (Nd3+). The wavelength of this laser,1.06 m, enables it to be transported by optical fiber. This low volume monocrystal(for example, a bar 150 mm in length and 9.52 mm diameter) is placed in areflective cavity. The excitation of the medium is ensured by xenon lamps or laserdiodes. The electrical efficiency of the laser depends on the pumping system, 1-3%
High Density Energy Beam Welding Processes 37for a lamp pumped system and in the order of 10% for laser diodes. The cooling ofthe system is ensured by water circulation in the cavity. Two modes of Nd:YAG laser operation should be noted: pulsed and continuous.Pulsed YAG laser sources Pulsed YAG laser sources generally consist of a pumping module that deliversan average power ranging between 300 and 500 W. These YAG lasers can reach upto 2 kW on average by adding, in series, additional amplifying modules to thispumping module. The pulsed operation mode is ensured by flash lamps whichproduce with each impulse an optical response of a defined frequency and pulselength. The mode of operation for these lasers is schematized in Figure 2.4. Figure 2.4. Pulsed YAG laser mode The characteristics of a pulsed YAG laser are related to its peak power, whichcan reach 50 kW. The relations between the various laser parameters are as follows: – peak power: Pc E W ; – average power: Pm E FW ; – pulse duration: (ms) ; – pulse energy: E(J) ; – pulse frequency: F(Hz) . High peak powers are reserved for drilling or cutting operations. For welding,the peak power must be limited and depends on the material and the thickness to bewelded. They should not exceed 4 kW. The use of a high peak power will causematerial spattering. For this reason, the average power of the sources intended forwelding should be limited to 500 W. Sources of greater power will be used only forhigh pulse frequencies. The penetration depth will in any event be limited to 1.5 mmfor a quality steel weld.
38 Metallurgy and Mechanics of WeldingContinuous YAG laser sources These were developed after pulsed YAG laser sources. The excitation of themedium is ensured by continuously lit xenon lamps. The average powers reachedare higher than in the case of the pulsed YAG laser sources: 4 to 5 kW. The essentialdifference between the pulsed mode and the continuous mode lies in the peak power.In the case of the continuous mode, the peak power is equal to the average power. Figure 2.5. Pumping chambers of a continuous lamp pumped rod YAG laser (4kW average beam power) (Trumpf document) The current developments are mainly directed towards increasing the power ofthese sources and of the pumping system (see Figure 2.5). The power increase isobtained by the increase in the number of pumping chambers (resonators andamplifiers). In the case of a conventional laser source with cylindrical bars andlamp-pumping, the maximum number of pumping chambers currently put in seriesis eight. This limitation is mainly due to beam degradation. The beam quality ofindustrial continuous YAG lasers around 25 mm.mrad enables a laser beam of morethan 4 kW to be carried in a 0.6 mm diameter optical fiber. The development of diode-pumped rod Nd:YAG laser sources in the year 2000has offered scope for progress (see Figure 2.6). The system of pumping by laserdiodes allows a better efficiency ( 10%) and a clear improvement in beam quality(15 mm.mrad).
High Density Energy Beam Welding Processes 39 Figure 2.6. 4.4kW YAG laser source using laser diode-pumped rods (Rofin Baasel document) The development of diode-pumped rod laser sources were a stage in thetechnological development of YAG laser sources but they have not been usedindustrially. They have encountered considerable technical problems linked to thereliability of the diode laser sources used for pumping. Today they have beenreplaced by new types of laser sources, diode-pumped disk laser sources and fiberlaser sources.Disk laser sources For diode-pumped disk laser sources, the active medium consists of small sizedYAG disks (see Figure 2.7). Laser sources up to 8 kW power beam are available forindustry today, with a very high beam quality (0.8 mm.mrad) and high degree ofefficiency. As opposed to the rod systems, the disk laser has no thermal lensing.This means that the beam quality is constant across the entire power range. Furtherdevelopments of more powerful laser sources are expected in the near future (16kW). The exceptional beam quality obtained using these laser sources allows thetransport of up to 8 kW beam power in a 0.2 mm diameter optical fiber.
40 Metallurgy and Mechanics of Welding Figure 2.7. Resonator diagram of a laser diode pumped disk source (Trumpf document)Fiber laser sources This new laser source has recently been developed for industrial applications. Itwas initially developed for the telecommunications industry in the early 1990s. Itsactive gain medium is an optical fiber doped with a rare element like Ytterbium.This type of laser source can produce a very high power output (over 20 kW) with avery good beam quality. The efficiency attained is around 25%.126.96.36.199. Semiconductor laser sources (or laser diodes) The stacking of a multitude of semiconductors makes it possible to obtain laserdiode systems from a few tens of watts to several kilowatts. The wavelengthsavailable are 0.808 and 0.940 m. The multiple beams emerging from these stacksare treated by sophisticated optical systems in order to be combined. The poorquality of beam produced is not conducive to optimal beam focalization. Therectangular and large-sized focal point generates power densities on the workpiecelower than 105 W/cm², which is insufficient for keyhole welding. These characteristics make it an excellent tool for the welding of syntheticmaterials, brazing, surface treatment or conduction welding. The particularadvantage of this technology lies in its high energy efficiency (>25%), thecompactness of the sources, the low operating costs (absence of lamps or lasing gas)and the low wavelengths (better absorption by metallic materials and possibletransport by optical fiber). The development of optical systems allowing for a betterfocusing of the laser beam is keenly awaited and will revolutionize the use of theselaser sources.
High Density Energy Beam Welding Processes 41 Figure 2.8. Diode laser source (Rofin Baasel document)2.2.4. Laser systems188.8.131.52. Laser beam transport The beam emitted by a laser source must be transported to the component to bewelded with minimal losses. The transport and focusing systems used depend on thelaser beam’s wavelength. Nd:YAG laser beams can be transported by optical fiberwhereas the CO2 laser can only be transported by mirrors. In this case, the opticalpathway must be confined and pressurized in order to avoid the mirror deteriorationand the possible degradation of beam quality. Figure 2.9. Insertion of a laser beam in an optical fiber; from HAV 96 The optical fiber must be as small in diameter as possible. The beam quality isthen essential. Pulsed YAG laser beams averaging from 400 to 500 W in power canbe inserted into a fiber 400 m in diameter, continuous YAG lasers pumped by 4 kWlamps use optical fibers 600 m in diameter and disk laser sources pumped by laser
42 Metallurgy and Mechanics of Weldingdiodes benefit from a reduction in the optical fiber diameter (an 8 kW beam using a200 m diameter optical fiber). The power losses are limited to less than 10% peroptical fiber. The mirrors most commonly used for CO2 laser beam transport can be made outof bare copper, gilded copper or covered in molybdenum. Gilded copper is valuedfor its very low absorption properties but it is fragile and expensive. Bare copperalso has low absorbance and is comparatively inexpensive, but tends to oxidize.Molybdenum covered copper is extremely resistant but its reflective properties arelower than the others. There is no precise rule for the choice of mirrors. It ishowever advisable to avoid using bare or gilded copper for focusing heads subjectedto projections and welding fumes. The pressurized optical transport can consist ofbare copper mirrors (less expensive), of gilded copper mirrors (good reflectivity) orof molybdenum covered mirrors (more resistant but more absorbent).184.108.40.206. Focusing The laser beam must be focused on the workpiece in order to obtain the powerdensity necessary to weld. YAG laser beams are generally focused using glasslenses. CO2 laser beams whose power is lower than or equal to 3 kW can be focusedusing selenium-zinc lenses or mirrors. Higher powered CO2 laser beams aregenerally focused using mirrors alone. These can be bare or gilded copper,molybdenum covered copper or solid molybdenum. Gilded copper is generallyavoided for the construction of optical focusing heads because of its fragility. The dimensions of the focused beam depend on the beam wavelength, its qualityand the focusing system used. The diameter of the focal point is related to theseparameters by the following equation: d M 2(4 f / D)with: – d: diameter of the focal point, – M2: factor of beam quality, – : wavelength, – F: focusing distance of the optical system, – D: diameter of the beam before focusing.
High Density Energy Beam Welding Processes 43 Figure 2.10. Laser beam focalization; from [HAV 96] In the case of YAG lasers, the focal point diameter depends primarily on theoptical fiber diameter, and on the collimation and focusing system (see Figure 2.11),which explains the importance of minimizing the optical fiber diameter: Figure 2.11. YAG laser beam focalization; from [HAV 96] Another important dimensional specification of the focal point is the field depthL. It is defined as being the zone in which the diameter of the beam increases nomore than 5%. It can be expressed in the following way:
44 Metallurgy and Mechanics of Welding While remaining within this tolerance of 5% of the focal point diameter, thevariation in the resulting power density does not exceed 10%. We will see hereafterthe importance of this criterion for the welding process.220.127.116.11. Beam and workpiece displacement system There exist various mechanized beam and/or workpiece displacement systems.These systems are conceived according to the type of laser source used, thedimension of the parts to be welded and economic considerations. Contrary to themarket of laser beam cutting, welding machines are often dedicated to anapplication. In order to reduce the costs, the manufacturers propose more and moremachines by catalog or machines made up of standardized sub-assemblies. Figure 2.12. Mixed three axis system (Balliu document) For the simplest components, machines with fixed optics are used. Thecomponents are moved under the focused beam. Only the focusing optics are movedvertically to adjust the position of the focal point or to allow the loading and theunloading of the part. For this type of simple application, the optical pathway doesnot justify the use of optical fibers.
High Density Energy Beam Welding Processes 45 For more complex trajectories, we may have to use robotized systems withseveral axes of motion. There are two types: Cartesian robots or polyarticulatedrobots. Cartesian robots are mainly used for the mirror displacement in the case ofCO2 lasers. They can incorporate up to five axes of motion. These precisionmechanical systems, are expensive and require a rigorous optical pathway design(see Figures 2.12 and 2.13). Figure 2.13. Five axis system with mobile optics (Trumpf document) The development of high power continuous YAG laser sources and of beamtransport by optical fibers has increased the use of polymorphic robots for weldingoperations. Their unquestionable advantage is the very competitive installation costcompared to the five axis Cartesian systems. The applications are currently mainlyfor the welding of automotive bodyshells (see Figure 2.14). These robots offer less positional precision than gantry robots, but thisdisadvantage can be compensated by the use of real-time trajectory monitoringsystems.
46 Metallurgy and Mechanics of Welding Figure 2.14. Six axis robot equipped with optical fibers for a YAG laser (Kuka document) These robots can be equipped with a remote welding system (see Figure 2.15).This technology makes welding possible at a considerable distance from theworkpiece. This remote process uses the latest high quality laser sources (disk laserand fiber laser sources).18.104.22.168. Peripheral systems Peripheral systems are the devices that monitor the correct functioning of thelaser system (power measurement, beam analysis, etc.), to supervise the welds beingmade (infrared thermography, plasma analysis) and facilitate robot operation (jointmonitoring systems).
High Density Energy Beam Welding Processes 47Figure 2.15. Six axis robot equipped with a remote laser welding system (Trumpf document)Power measurement Laser sources are equipped with an internal system of power measurement. Itgives an indication of the beam power emitted by the source. This power value doesnot take account of possible losses along the optical pathway. External measurementsystems are available to measure the beam power at the component site. Thesesystems do not allow the power measurement during welding, so they will becomplementary to internal measurement systems, which can give an indicationduring the welding process.Beam analysis In the case of laser beam welding, the focused beam constitutes the welding tool,hence the importance of understanding its characteristics perfectly. Empiricalmethods allow an evaluation of the position and diameter of the focusing zone. Thedifficulty in using these methods increases with the power of the laser beam. Devices have been developed in order to determine laser beam characteristics ina precise way. The operating principle of these devices is based on taking away ofpart of the beam and analyzing it using photodiodes. On average, beams up to 20 kWwith power densities 107 W/cm² can thus be analyzed.Weld monitoring One of the principal advantages of laser beam welding is its high speed. Thisadvantage can quickly become a disadvantage if a defective weld is not detected intime. This can lead to the rejection of a great quantity of parts. It is thus necessary tomonitor the welds on the production line in order to detect the defects as soon aspossible. Several methods are employed.
48 Metallurgy and Mechanics of Welding Infrared thermography – an infrared camera scans the back of the weld bead,very close to the weld pool. The anomalies noted in the temperature isotherms makeit possible to highlight the formation of a welding defect. This control techniqueindicates the presence of an anomaly but does not give information about the qualityof the weld. It can be used in addition to other monitoring techniques. Thistechnique, which is difficult to control, is not very well suited for production linemonitoring. Plasma analysis – this method consists of analyzing the emission of plasma andthe weld pool. The sampling of data is carried out at the level of the laser/materialinterface by optical fibers or optical components located in the optical pathway. Thesensors used are photodiodes whose fields of sensitivity can be located in the ultra-violet (emission of plasma), the visible range or infrared (emission of the weldpool). An analysis of the signal makes it possible to correlate the events detectedwith the appearance of weld defects. These devices make it possible to detect inreal-time the formation of defects and to set off an alarm at a predetermined level.Control by closed loop is at the development stage.Seam tracking system Seam tracking, initially developed for conventional welding, has been adapted tolaser welding. The laser triangulation technique makes it possible to carry outdetection of the joint position in a reliable way for an environment where normalvision is disturbed (fumes, projections, highly emissive plasma). The majority ofsystems use the projection of a laser line which is compared with a computerizedmodel [BOI 98]. Visualization by CCD camera is nowadays offered as a competitivealternative to laser triangulation.2.2.5. Implementation of laser beam weldingLaser/material interaction The laser beam is focused on the surface of the part so as to obtain a powerdensity in the range of 5.105 and 5.106 W/cm². Figure 2.16 shows that a powerdensity threshold exists for the creation of a vapor capillary or keyhole.
High Density Energy Beam Welding Processes 49 Figure 2.16. Penetration depth and absorption coefficient in relation to laser beam intensity; from [HER 86]The threshold of the power density is a function of the following factors:– the nature of the material to be welded,– the laser beam wavelength,– the shielding gas,– the workpiece surface quality.
50 Metallurgy and Mechanics of Welding The nature of the material plays a big role in the creation of the vapor capillary.Materials such as silver, gold, copper alloys and aluminum alloys are not easilyweldable by laser beam because of their low absorption coefficients. Figure 2.17 shows that, because of their wavelengths, YAG laser beams andlaser diode beams are absorbed better by metallic materials than a CO2 laser. Wewill see that the wavelength can be a selection criterion for the welding of materialswith a low absorption coefficient. Figure 2.17. Beam absorption in relation to wavelength; from [ROE 86] The low absorption coefficient of a material can be compensated by a highpower density. This high power density can be obtained by the use of a good qualitylaser beam, the choice of short focal length optics, the increase in laser power or, inthe case of a YAG laser, the use of a small diameter optical fiber. The choice of assistant gas is also paramount. A good control of the gas supplyand an appropriate choice in its composition have an important impact on thewelding process and weld quality.Shielding gas The majority of the fusion welding processes (except the electron beam) requirea shielding gas at the weld surface and if necessary at the back of the weld bead. Incertain cases, a shielding gas covering can be used.
High Density Energy Beam Welding Processes 51 We can distinguish three zones to be protected: the weld pool, the surface of theweld just after solidification while still sufficiently hot to oxidize, and the root of theweld bead. For the protection of the weld pool and vapor capillary, we can use: – a coaxial nozzle, – a lateral nozzle, – a plasma blowing system. The coaxial and lateral nozzles transport gas at atmospheric pressure and at a lowflow (15 to 30 l/min according to the power of the laser beam). They allow a goodprotection of the weld bead without disturbing the weld pool. The coaxial nozzle hasthe advantage of being usable for welding in all directions, which is not the case ofthe lateral nozzle. The use of a plasma jet is used in some particular cases. This consists of using asmall diameter tube ( 6 mm) tilted at an angle ranging between 35 and 45° inrelation to the surface of part with a high gas output. The gas jet, directed a fewmillimeters above the surface of the part, blows the gas plasma. This system is littleused, because it does not allow a good gas protection and tends to disturb the weld pool. The principal assistant gases used are the inert gases helium and argon or theactive gas, that is, nitrogen. In the case of laser beam welding, gas protection doesnot only have the role of protecting the weld pool from contamination, it also takespart in the interaction between laser and material. The choice of gas thus depends onmany factors: – ionizing potential of gases, – laser beam wavelength, – nature of the material to be welded. Gases subjected to a high density of power ionize more or less easily. Heliumwhose ionizing potential is high (24.46 eV) creates a not very intense and ratherpermeable plasma regardless of the laser beam’s wavelength. It can be used up topowers of 45 kW without particular problems. Argon and nitrogen, whose potentialfor ionization are lower (Ar: 15.68 eV and N2: 15.51 eV), create an intense plasmawhich hinders the interaction of beam and material. In the case of the CO2 laserbeam, the use of these gases will be limited to powers 5 kW. From the perspectiveof welding performance, helium ensures the deepest weld penetration compared tonitrogen and argon and the narrowest weld beads. The addition of helium to argonmakes it possible to limit the harmful influence of argon generated plasma.Commercial mixtures (helium/argon) are offered, especially for welding by laserbeam. These mixtures can be used for powers up to 10 kW.
52 Metallurgy and Mechanics of Welding In the case of the Nd:YAG laser, the choice of gas is not so important. The firstdata collected indicates that the use of argon or nitrogen with a Nd:YAG laser orfiber laser is possible with powers up to 10 kW. Argon and helium, being inert, can be used whatever the nature of the material tobe welded, which is not the case with nitrogen. The latter can cause metallurgicaltransformations in the materials to be welded. It is not to be used for weldingzirconium and titanium alloys, as it will form titanium nitrides and zirconiumnitrides which will weaken the assemblies. Nitrogen can also cause an increase inthe sensitivity to hot cracking of austenitic stainless steels because of its gammageneeffect (it leads to the formation of austenite as well as primary austenitesolidification). For these materials, its use will be subject to procedures that preventhot cracking. However, because it is soluble in stainless steels, nitrogen could beused with some advantage to avoid the formation of porosities in the molten zone[BAR 98]. Its use for welding non-alloyed and slightly alloyed steels does not pose aparticular problem if a high quality of welding is not required.2.3. Electron beam welding2.3.1. History [FRI 98] The earliest applications of the electron beam result from the work completed byK.-H. Steigerwald in Germany and by J.A. Stohr at the CEA (Atomic EnergyCommission) in France. For the latter, this work was justified for the welding ofcombustible material casings made of zirconium alloy, a material very sensitive tooxidation and for which there did not exist, at that time, a suitable welding process.The production of an electron beam required vacuum conditions which naturallygave protection against oxidation. Thus, welding was made possible and the first EBwelds were obtained using a focused electron beam produced by a Guinier cathodesystem. A patent was thus declared in 1956 and licenses granted to companies forthe construction of machines, which appeared on the market in 1960. The first machines had low power electron beam guns (a few kilowatts), whichlimited the thicknesses that could be welded to approximately ten millimeters. Veryquickly, the gun power that could be increased (30 kW in 1970), which made itpossible to consider the welding of very thick parts (40 to 50 mm) encountered inboiler manufacturing or heavy engineering. During the 1980s, new applications were sought, with more than 1,000 machinesbeing built in Western Europe between 1980 and the end of the 20th century.
High Density Energy Beam Welding Processes 532.3.2. Principle The process of EB welding uses the energy dissipated by electrons at themoment they strike the part to be welded.The electronic beam The electron is a particle characterized by its mass m = 9.1 10-31 kg and itsnegative electric charge e = 1.6 10-19 Coulomb. When this electron is placed in aspace where an electric field E and a voltage V exists, it is subjected to a force F =eE. Under the action of this force, the electron moves with a speed v and willacquire, by ignoring the relativity effect, kinetic energy: Ec 1 mv2 eV 2 If we consider n/t electrons emitted per unit of time, the power transported by theelectron beam will be: W 1 n mv2 ne V I V 2 t twith: – V: acceleration voltage of the electrons, – I: intensity of the beam.Specific power This is defined as the ratio between the power transported by the beam and theimpact area of the beam on the parts to be welded. In welding, this specific power isa few tens of kW/mm-2. In fact, all the power is not transformed at the point of impact because of lossesin the electron trajectory between the emission point and the point of impact on thepart. The first losses are due to collisions with the atmospheric molecules; they are allthe more significant the higher the air pressure is. The second losses are less important in quantity; they are due to re-emissionphenomena, the most important of which is x-ray emission. The energy quantity thusdissipated is low (~ 1%) but the consequences are important from the perspective ofsafety.
54 Metallurgy and Mechanics of Welding2.3.3. Equipment Three welding techniques appear according to the pressure value P close to theworkpiece: – P > 10-5 mbar: secondary vacuum welding, – P ~ 10-2 mbar: primary vacuum welding, – P ~ 1,000 mbar: welding without vacuum. The equipment used is obviously different but they all include: – an electron beam gun with its viewing system, – a welding chamber containing the parts to be welded and sometimes theelectron gun. This enclosure also contains the displacement systems for the parts andthe gun, – a pumping unit to obtain a reduced pressure into the gun and the chamber, – a power supply and numerically controlled command and control circuits.The electron gun Figure 2.18 illustrates the principles of a triode electron gun, which include: – a cathode made of a very emissive material: tungsten, tantalum or lanthiumhexaboride. This cathode is heated in vacuum conditions, either directly by anelectric current (direct heated electron gun), or indirectly by a primary electron beamresulting from a heated filament (indirect heated electron gun); – a non-magnetic Wehnelt surrounding the cathode and acting, on the one hand,on the shape of the equipotential surfaces and thus on the shape of the beam (theelectrons move perpendicularly to these surfaces) and, on the other hand, on theelectron acceleration where this plays the part of a grid in a triode;
High Density Energy Beam Welding Processes 55 Figure 2.18. Principle of a triode electron gun (Institut de Soudage document) – a copper anode carrying a positive charge compared to the Wehnelt creating theelectric field to accelerate the electrons. This anode is bored in its center with achannel which allows the electron beam to pass through. This convergesimmediately at the exit of the anode then diverges under the effect of mutuallyrepulsive electrons as they move apart; – a magnetic focusing coil with windings in the same axis of symmetry as thegun. It reconcentrates the divergent beam and concentrates it on a small point (abouta millimeter in diameter); – a set of magnetic deflection coils enabling the beam to move in relation to itsaxis (side sweepings, circular movement, etc.); – a system for accurately positioning the beam on the joint by an optical viewingsystem or a television camera system. According to the electrode geometry and in particular of those of the anode andWehnelt, the maximum current available I will be determined according to theacceleration voltage V by a characteristic of the gun called perveance p and expressed as:
56 Metallurgy and Mechanics of Welding I p V3/ 2 The gun powers vary according to the thicknesses which need to be welded.They range from 5 to 100 kW but most of the installations are equipped with gunsthat have a power ranging between 10 and 30 kW. With regard to the accelerationvoltages, here those lie between 45 kV and 150 or even 300 kV, depending on thetechnologies chosen by the manufacturers and the power required from the gun.The welding enclosure and displacement mechanisms The enclosure (vacuum chamber) contains the parts to be welded with their toolsand their workpiece displacement. It can also contain the electron gun with itsdisplacement system with one or more axes. Generally, this enclosure must be of alow volume compatible with that of the parts to be welded, but it should beunderstood that too large a volume involves a longer pumping time, which has adetrimental effect on the equipment productivity. Figure 2.19. 6 kW EBW machine; dimensions 0.6 m 0.6 m 0.9 m (Techméta document) In addition, these enclosures must be designed to resist atmospheric pressurewithout any deformation and their internal sides walls must be clean in order to limitthe effects of gas adsorption and thus reduce the pumping time.
High Density Energy Beam Welding Processes 57 The enclosure volumes used industrially vary between 0.5 m3 and more than1,000 m3 (see Figures 2.19 and 2.20). Figure 2.20. 50 kW EBW machine with internal gun; dimensions 8 m 5 m 5 m (Techméta document) In order to avoid building large-scale enclosures, it is desirable to create thevacuum locally, where the weld is to be made. This solution was adopted between1970 and 1980 for various applications, including the welding of connecting pipeson boilers or tubes on tubular exchanger plates. Although tempting a priori, thissolution has effectively been abandoned, because equipment with localized vacuumchambers was very expensive due to its application to only one type of part, and itdid not offer great flexibility in use. The systems for positioning and moving the parts are tables with one or two axesor turning gears for the welding of rotating parts. These mechanical axes arecontrolled numerically.
58 Metallurgy and Mechanics of WeldingVacuum creation systems For the machines in primary vacuum, the pumping unit consists of standardmechanical pumps (rotary vane pumps or Roots booster pumps). For those working in secondary vacuum, one or more oil diffusion pumps orturbomolecular pumps are added. The pumping unit’s delivery is a function of the enclosure volume to be pumped,the pumping time and degasification related to the nature and the thickness ofmaterial being welded. This last criterion is particularly important when weldingvery thick parts. This pumping delivery can reach levels from 2,000 to 5,000 m3.h-1for mechanical pumps and from 10,000 to 20,000 l.s-1 for oil or turbomolecularpumps.Non-vacuum machines or under reduced pressure [POW 00] The first industrial non-vacuum EB welding machine was used in the USAautomotive industry towards the end of the 1960s. The essential characteristic of thistype of equipment lies in the absence of a vacuum chamber, which is very importantfor mass production, e.g. automotive components like transmission components,torque converters and exhaust systems. Counterbalancing this advantage is thedisadvantage of having to use a very high acceleration voltage (150 kV) in order toobtain a sufficiently powerful beam on the work piece, in spite of passing through agaseous atmosphere of only a few millimeters. This high voltage generates strongX-ray emissions and it is thus necessary, in order to protect the operators working onthe machine, to create an enclosure ensuring containment of this radiation. Unlike in the USA, this type of process was little used in Europe. However, since1990, significant developments have led to new equipment which functions atatmospheric pressure or under reduced pressure (<1 mbar). There is thus a renewedinterest in this technology in two fields: thin sheet welding for the automotiveindustry (welding of aluminum panels) and welding of thick parts such as pipes forgas pipelines and containers for storage of radioactive elements.Implementation of EB welding Achieving a good quality weld requires the following parameters to bemonitored: – the power transported by the beam: it is the product of the electron accelerationvoltage and the beam intensity. The power will be selected according to thethickness of the parts to weld, the nature of material and its physical properties (forthe same thickness, we need more power to weld copper than steel) and weldingspeed;
High Density Energy Beam Welding Processes 59 – the welding speed: this should not only be selected according to gun power butit must be determined by the metallurgical weldability of material, i.e. its ability toform a defect-free weld (with no cracks for example); – the pressure in the enclosure: this parameter is linked to the equipment, whichis designed to work either in primary vacuum or in secondary vacuum. Somemachines are able to work either in primary vacuum or in secondary vacuum; in thiscase, the choice of the pressure will be dependent on the material to be welded andits reactivity with oxygen (zirconium alloys for example); – focus current: this very important parameter because it determines the specificpower and thus has an important effect on the geometry of the molten zone. Thisparameter varies according to the nature of material to be welded and its thickness.It is thus related to the acceleration voltage and the welding intensity; – beam deflection makes it possible, by movements imparted to the beam, tocarry out welds by limiting the movement of the component. It is possible forexample to perform a small diameter circular weld without any movement of theworkpiece or of the gun while making the beam describe a cone having for its axisthat of the workpiece; – beam vibration: depending on the signal imparted to the deflection coils, it ispossible to impart sweeping movements to the beam, (transverse or parallel to thewelding seam and circular or elliptic in shape). Two parameters, amplitude andfrequency, are added to the signal, which have a bearing on the width of sweepingand the stirring of molten metal. This beam vibration is used at an operational levelto widen the molten zone and thus to tolerate a gap between the components, toimprove the quality of the weld pool when welding in position. From a metallurgicalperspective, it can help reduce hot cracking observed with certain materials (nickelalloys for example) and aid degassing of the weld pool, thus limiting porosities; – the welding position: a flat welding position (beam axis is vertical) is used forwelding thicknesses from 15 to 20 mm with a complete penetration mode. Thislimitation is due to the loss of balance between the surface tension forces whichmaintain the molten metal on the edges of the capillary and gravitational force. Inpartial penetration mode, the maximum weldable thickness in flat position is about130 mm for steels. Beyond these limits, it is necessary to use the horizontal/verticalwelding position (beam axis is horizontal). In this case the thicknesses are dependenton the electron gun’s power. Vertical upwards welding and vertical downwardswelding can also be used on steel thicknesses from 60 to 80 mm. For the overheadwelding position, the maximum thickness is the same as that of the flat weldingposition.
60 Metallurgy and Mechanics of Welding2.3.4. Design and preparation of the parts In general, welding is carried out without filler, on straight joined edges. Figure2.21 illustrates some frequently used preparations. Figure 2.21. Examples of joint preparation (Institut de Soudure document) These few examples show that, to profit from all the advantages offered by theseprocesses, the choice of process will have to be made in the research department.The absence of a gap is sometimes difficult to achieve. Some gap betweencomponents can be tolerated; its value will vary with the thickness of the parts to bewelded but, for thicknesses lower than 15 mm, this gap is approximately 10% of thethickness. Above this, it is necessary to use a filler in order to avoid overly thinareas. This is frequently carried out by laser beam; in EB welding, implementation ismore delicate. Because of component machining, a thorough degreasing prior to welding and anelimination of oxides present close to the joint are required to obtain a quality weld. In EB welding, special attention must be paid to the remanent magnetism ofcomponents because of the risk of electron beam deviation and consequently of awelding defect like lack of fusion. This magnetism will thus have to be monitoredbefore welding and the parts can possibly undergo a demagnetization operation. It ishowever necessary to realize that this is a delicate operation and does not alwayslead to the anticipated result. In order to ensure a precise positioning of the photon or electron beam in relationto the joint, positioning and fastening assemblies are often required. These must beprecise and made of non-magnetic materials in the case of EBW.
High Density Energy Beam Welding Processes 612.4. Metallurgy of high density energy beam welding The principal features of high density energy density beam welding processescompared to conventional welding processes (arc welding) are: – the absence of filler wire in most cases, – high welding speeds which involve higher solidification and cooling rates, – a narrow molten zone and heat affected zone, – low heating and a limited deformation of the parts, – no direct contact between the energy source and the component. These features involve characteristics related to the behavior of the materials tobe welded. In order to study these characteristics, it is advisable to distinguish, onthe one hand, pulsed welding modes such as pulsed YAG laser beam welding and,on the other hand, continuous welding such EBW, CO2 laser and continuous YAGlaser processes. The thermal cycles obtained during pulsed welding are shorter thanthose obtained in continuous mode. In order to present the weldability problems of various metallic materials in acoherent way, we will distinguish [MUR 94]: – operative weldability: this relates to problems encountered at the time ofwelding, when the behavior of the metal or alloy to be welded prevents the weldbeing completed; – metallurgical weldability: during the welding process, one of the zones whichconstitute it (molten zone, bond area, or HAZ) can be altered because of theoperation itself, to the point of questioning the performance of the assembly underthe operating conditions envisaged. Operative and metallurgical weldabilities will be presented for the main metalalloys (steels, aluminum alloys, nickel alloys, titanium alloys, zirconium alloys andcopper alloys).2.4.1. Steels22.214.171.124. Operative weldability Steels generally offer a good operative weldability. In addition to the advantagelinked to the absence of a vacuum enclosure, the laser welding processes offer,compared to EB welding, the advantage of being insensitive to beam deviations,remanent magnetism in the case of ferritic steels or, in the case of heterogenous
62 Metallurgy and Mechanics of Weldingassemblies, the Peltier effect. Stainless steels must however be welded with gasprotection, catered for by using a gas carriage.126.96.36.199. Metallurgical weldabilityNon-alloyed or low-alloyed steels With regard to metallurgical weldability, apart from certain features of the highdensity energy beam processes evoked before (no contact with the parts, absence ofhydrogen, lower shrinkage stresses), these welding processes significantly limit thecold cracking phenomenon. Figure 2.22. Illustrations of CO2 laser welds in 25 CrMo4V steel (from [COL 97]). 25CrMo4V: 0.005% of sulfur, 0.015% of phosphorus (no cracking) 25CrMo4V 4: 0.031% of sulfur, 0.016% of phosphorus (cracking) On the other hand, work completed at the Institut de Soudure [COL 97]highlighted an increase in hot cracking due to the combined effects of the highwelding speed and presence of residual elements, sulfur and phosphorus in particular(see Figure 2.22). The ranges of chemical composition recommended by the current standards donot take account of the specificities of the high density energy beam weldingprocesses. A restriction in residual elements (sulfur, phosphorus) is essential in orderto limit the risks of hot cracking.
High Density Energy Beam Welding Processes 63Austenitic stainless steels Many prediction diagrams depicting the metallurgical structure of as-weldedalloys have been established and modified as welding processes have evolved. Interalia, the Schaeffler diagrams [SCH 49], Delong team diagrams [DEL 56] or Suutaladiagram [SUU 79] established for conventional welding processes are no longerapplicable for welding processes involving rapid cooling. For this reason, a studycarried out by the Institut de Soudure [CHE 93] looked at the influence of thermalconditions and steel composition on the liability of stainless steels to hot crackingwhen welded by a laser beam. It was shown that these hot cracking phenomena arenot very important during continuous welding mode but become highly significantduring pulsed welding. Figure 2.23. Prediction diagram of hot cracking during pulsed YAG laser beam welding of austenitic stainless steels; from [CHE 93] A new prediction diagram for hot cracking dependent on the sulfur, phosphorusand boron content of the alloy’s chemical composition in terms of equivalent Cr/Ni,and of the primary solidification mode (austenitic or ferritic) has been establishedfor the pulsed YAG laser and CO2 laser beam processes (see Figure 2.23). This diagram presents three distinct fields: two non-cracking domains and acracking domain. The alloys, of which the Cr/Ni equivalent is higher than 1.7, arenot very sensitive to hot cracking up to a high impurity content. They result from aferritic solidification mode followed by a solid state austenitic transformation. The
64 Metallurgy and Mechanics of Weldingsecond non-cracking domain corresponds to alloys whose Cr/Ni equivalent is lowerthan 1.58 but whose impurity content is low (S + P + B 200 ppm). The crackingdomain is defined by a Cr/Ni equivalent lower than 1.58 and an impurity content of(S + P + B) >200 ppm. Alloys whose Cr/Ni equivalent is between 1.58 and 1.70 arein a transitory zone where hot cracking depends on impurity content. Figure 2.24. Austenitic stainless steel pulsed YAG laser bead on plates; from [CHE 93a]. X2CrNi18-09 Cr/Ni eq. = 1.75% (S + P + B) = 0.0475% (figure on left) X2CrNiMo17-12-2 Cr/Ni eq. = 1.57% (S + P + B) =0.0481% (middle) X2CrNiMo17-12-2 Cr/Ni eq. = 1.523% (S + P + B) =0.0106% (figure on right) This work showed that external factors, such as the use of nitrogen (gammagene)as a shielding gas, can contribute significantly to the formation of cracks (see Figure2.25).Ferritic stainless steels The main issues encountered during the welding of ferritic stainless steels aregrain enlargement and nitride and chromium carbide precipitation which can causeintergranular corrosion. These phenomena are particularly prevalent during the useof welding processes using high linear energy. The high density energy beamwelding processes, with low heating and high cooling rate, limit these phenomenaand improve the welded joint’s mechanical strength in a significant way.
High Density Energy Beam Welding Processes 65 Figure 2.25. Comparison of beads on plates carried out with various shielding gases (from [CHE 93]). Bead on plate with helium (figure on left). Bead on plate with nitrogen (figure on right)Martensitic stainless steels Martensitic stainless steels can be sensitive to the cold cracking phenomenon.The factors which give rise to cold cracking are: – high percentage of carbon (>0.3%), – stresses caused by the welding process or unsuitable joint design, – high cooling rates, – the presence of hydrogen in solution.
66 Metallurgy and Mechanics of Welding Figure 2.26. CO2 laser beam lap weld of X2CrMoTi 18-2 ferritic stainless steel (Institut de Soudure document) Various arrangements make it possible to limit or avoid the cold cracking ofthese steels: – the use of an austenitic filler wire, – pre-heating and post-heating, – avoidance of hydrogen introduction. The high density energy beam welding processes have great advantagescompared with conventional processes. Having no contact with the part to bewelded, they limit hydrogen contamination, and with the molten zone being verynarrow, the stresses caused by shrinkage during solidification are significantlyreduced. Certain steels considered unweldable by arc processes have been weldedwithout filler wire and pre-heating. Precipitation hardening martensitic stainless steels lose their mechanicalproperties after welding if they are welded in an age hardened state. It is appropriate,if the design of the parts allows it, to weld in a hyperquenched state and to carry outthe ageing treatment after welding.Austenoferritic stainless steels (duplex or super-duplex) These steels owe their good mechanical characteristics and their good corrosionresistance to their microstructure made up of 50% of austenite and 50% of ferrite.The high cooling rate induced by welding causes an imbalance between ferrite andaustenite. The high cooling rate generated by the high density energy beam weldingprocesses involve the formation of an almost entirely ferritic structure in the moltenzone. The reduction in welding speeds and/or the introduction of nitrogen as a
High Density Energy Beam Welding Processes 67shielding gas increases the austenite content. Unfortunately, these techniques do notsuffice to obtain a duplex structure (see Figure 2.27). The high density energy beamprocesses will be usable only whenever the corrosion requirements are not atmaximum. Figure 2.27. CO2 laser butt welded joint of 3 mm thick austenoferritic stainless steel; X2CrNiMoN22-5-3 (Institut de Soudure document)2.4.2. Aluminum alloysOperative weldability The main issues of operative weldability for aluminum alloys relate to thepresence of the refractory oxide layer and their high conductivity. The oxide layerrequires the surface cleaning of the parts before welding, whatever the weldingprocess used. The laser welding of aluminum alloys is made more difficult becauseof their low absorption coefficient. In this case, a YAG laser has a slight advantagecompared to the CO2 laser because of its lower wavelength, which allows a betterradiation absorption. Electron beam welding has advantages for the welding of these alloys because itdoes not have the absorption problem of laser beams, while the weldable thicknessesare high (see Figure 2.28) and the weld beads are narrow. The thermal welding cycleis sufficiently short, which limits the problems caused by aluminum’s high thermalconductivity.
68 Metallurgy and Mechanics of Welding Figure 2.28. Electron beam weld of aluminum alloy 5754 (Institut de Soudure document)Metallurgical weldability In a similar way to austenitic stainless steels, aluminum alloys react differently tothe pulsed or continuous welding mode. The solidification speed obtained during pulsed YAG laser beam welding causesthe systematic appearance of hot cracking. Only pure aluminum and the 4000 seriesaluminum (Al, Si) can be welded without hot cracking. The 5000 (Al, Mg) and 6000(Al, Mg, Si) series aluminum alloys can be welded either in a heterogenousassembly with the 4047 aluminum alloy (or 4043) or by using this alloy as fillerwire. Continuous mode welding processes cause fewer hot cracking problems. Theymake it possible to weld 3000, 4000, 5000 and 6000 series aluminum alloys undergood conditions. The 6000 series can however present hot cracking phenomena forhigh welding speeds. For laser welding, the use of 4047 (or 4043) filler wire canavoid this hot cracking phenomenon. However, this can give rise to a liquationphenomenon.
High Density Energy Beam Welding Processes 69 Figure 2.29. CO2 laser beam weld of 5 mm thick aluminum alloy 6013; from [CHE 98] In the case of 2000 series aluminum alloys, only alloy 2219 is truly weldable.Aluminum alloy 2024 can be welded with caution at a low welding speed. Figure 2.30. CO2 laser beam weld of 5 mm thick aluminum alloy 2219; from [CHE 98] The 7000 series alloys must be welded with precaution, because they have astrong tendency to hot cracking. Aluminum alloy 7020 can be welded by electronbeam (see Figure 2.31). It is advisable in this case to take account of the restrainteffects caused by the design of parts.
70 Metallurgy and Mechanics of Welding Figure 2.31. 2 mm penetration depth in a aluminum alloy 7020 welded by electron beam (Institut de Soudure document)2.4.3. Nickel-based alloysOperative weldability Like stainless steels, nickel-based alloys do not pose any particular operativeweldability problem. It is however necessary in the case of laser welding to providean adequate shielding gas using a gas carriage.Metallurgical weldability Nickel-based alloys can be classified into two big groups: – non-heat-treated alloys: these offer good corrosion resistance. Such alloysoffer, in general, good weldability; – precipitation hardening alloys: these are used for their good mechanicalproperties at high temperature. They are sensitive to hot cracking. A post-weld heattreatment is often necessary (see Figure 2.32).
High Density Energy Beam Welding Processes 71 Figure 2.32. CO2 laser beam weld of 6 mm thick Inconel 718 (Institut de Soudure document)Figure 2.33. Electron beam weld of 100 mm thick titanium alloy TA5E (Institut de Soudure document)
72 Metallurgy and Mechanics of Welding2.4.4. Titanium-based alloysOperative weldability Titanium alloys respond well to laser beam or electron beam welding. They havea good fluidity which helps the formation of an aesthetic weld bead. The use ofexcessive energy densities will cause surface defects like undercuts (see Figure2.33). Figure 2.34. CO2 laser beam weld of 6 mm thick alloy TA6V (Institut de Soudure document) They have, however, a great sensitivity to oxygen and nitrogen. An effective gasshield is required during welding. Contamination by oxygen and nitrogen entailsparticle formation, which increases mechanical resistance to the detriment oftoughness and thus will weaken the structure. For this reason the vacuum electronbeam is an excellent alternative.Metallurgical weldability Certain alloys are sensitive to grain enlargement during welding. As for ferriticstainless steels, high density energy beam processes significantly limit thisphenomenon. The weld beads obtained by laser or electron beams have a betterductility than those obtained by arc welding. The alloys usually employed are notvery sensitive to hot cracking.
High Density Energy Beam Welding Processes 732.4.5. Zirconium-based alloysOperative weldability The behavior of zirconium alloys is similar to titanium-based alloys. They can beeasily contaminated by ambient air. Oxidation starts at 400 to 500°C. Surface andback gas shielding must be guaranteed. The electron beam is the favored process forthese alloys. A pulsed YAG laser beam can be used because of the limited heatingeffect. Figure 2.35. Pulsed YAG laser weld of 1 mm thick zirconium alloy Zy4 (Institut de Soudure document)Metallurgical weldability Certain alloys are commonly used because of their good metallurgicalweldability. This is the case for Zircaloy in the manufacture of casings for thenuclear industry. Zirconium alloys are sensitive to grain enlargement, hence thevalue in using high density energy processes.2.4.6. Copper-based alloysOperative weldability The great reflectivity and high thermal conductivity of copper alloys are majordisadvantages for laser beam welding. It acts just as a mirror. The pulsed YAG laser
74 Metallurgy and Mechanics of Weldingbeam, thanks to its high density of energy, can sometimes be used for welding verythin parts. On the other hand, the electron beam presents many advantages. It makesit possible to weld thick sections without pre-heating. The weld beads obtained arenarrow. Figure 2.36. Electron beam welding of a copper part (Institut de Soudure document)Metallurgical weldability Pure copper exists in different levels of purity: – Cu-a1: 99.90% pure, contains up to 0.1% of oxygen, – Cu-b: 99.90% deoxidized with phosphorus, – Cu-c1: 99.94% pure, – Cu-c2: 99.96% pure. Copper must be welded in deoxidized types Cu-c1 or Cu-c2. Whatever the originof the oxide, when it occurs as intergranular precipitates, it weakens the weld and itssurroundings. It can also cause the formation of porosities. The main copper alloys have a good metallurgical electron beam weldability. Ahot cracking phenomenon is possible for certain alloys such as cupro-aluminums,cupro-berylliums and certain brasses. It is absolutely essential to avoid the presenceof lead (alloys with improved workability) which increases the tendency to hotcracking.
High Density Energy Beam Welding Processes 752.5. Mechanical properties of welded joints High density energy beam welds have specific characteristics such as single passwelding, a narrow molten zone and the absence of filler wire. These characteristicswill have an influence on the traditional mechanical properties. With regard to the tensile test, the transverse rupture of tensile specimensgenerally occurs in the base metal. Only austenitic steels present a rupture close tothe fusion line but at a breaking load very close to that of the base material. Formaterials with structural hardening, the rupture occurs in the molten zone. Thetensile tests in the longitudinal direction are not carried out because of the difficultyin taking a test piece due to the narrowness of the molten zone. Figure 2.37. CO2 laser beam weld of 12 mm thick non-alloyed steel (Institut de Soudure document) Bend tests lead to good results. It should however be noted that in welds carriedout on alloyed steels, the hardness difference observed in the weld area causes adeformation during the transverse bending test on either side of the molten zone.Longitudinal bend testing is thus more useful since it forces all the zones to deformin the same manner. For the impact test, a crack deviation and the absence of rupture is oftenobserved in the test sample. This then raises the problem of the test’s validity. Palliative solutions have beendeveloped to try to evaluate the strength of these welds. Currently there is no
76 Metallurgy and Mechanics of Weldinguniversal agreement, and further work is necessary to find a new test that is easy tocarry out, inexpensive and gives valid results. The hardness test, which shows the various joint structures, are characterized bya lower value in the molten zone than in the heat affected zones (HAZ). This can beexplained by a different cooling rate and the loss of quenching elements from themolten zone, such as manganese in steels. In arc welding processes, the hardness testis often associated with cold cracking and the threshold criterion of maximumhardness of 350 Vickers. For the laser and EB processes, this threshold is exceededin the majority of cases. However, as the welding is performed in the absence ofhydrogen since it is in a vacuum or under gas protection, the risk of cold cracking isalmost zero, except for highly alloyed tempered steels or those with high levels ofcarbon. Fatigue resistance,is in general satisfactory, due to the presence of compressivestresses on the bead surfaces.2.6. The quality of the assemblies The quality of a weld is measured with respect to its conformity to specificationsimposed on the final assembly. It can be a question of its mechanical performance,water/air-tightness, or resistance to corrosion. Quality is tested overall using tests onthe complete assembly or on the test specimens produced under the same operatingconditions, and/or by observing this assembly in a very precise way, using both non-destructive and destructive tests. In the following section, we will present a non-exhaustive list of the possibledefects in HEDB welds, the control methods most commonly used and the principalstandards in operation.2.6.1. Weld defects Standard NF EN 26520 is a “classification of the defects in the fusion welds ofmetals with explanatory comments” and makes it possible to enumerate and classifythe defects according to their geometry, their position in the weld and their origin.HEDB processes, due to their particular features, give rise to the appearance ofspecial defects.Cracks Hot cracks are most frequently encountered because of high solidification speedsand, in most cases, the absence of filler wire addition. They are emerging or
High Density Energy Beam Welding Processes 77non-emerging and small in size. They are called hot cracks when they appear at theend of solidification on a molten pool. There are interdendritic or intergranularcracks, related to segregation phenomenon. The pulsed YAG laser beam weldingprocess has a tendency to produce such defects in austenitic stainless steels,aluminum alloys and some nickel base alloys. The cracks are known as cold cracks when they appear towards the end ofcooling, at around 150°C or less. These cracks are found in the molten zone or theheat affected zone. They are related to martensitic quench hardening, hydrogenembrittlement and internal stresses. Non-alloyed or low alloyed steels are sensitiveto cold cracking according to their percentage of carbon and alloying elements.Various formulae have been proposed to define a weldability limit for these steels.Such formulae, established for conventional welding processes, only account for thecomposition of steels in terms of carbon equivalence but disregard the coolingspeed. These formulae are not applicable in the case of HEDB processes because ofits high cooling speed, and also the fact that they do not introduce hydrogen and thatshrinkage stresses are limited. These cracks, encountered less frequently than hotcracks, are quite small.Cavities These are voluminal defects. They include shrinkage due to the shrinking ofmetal during solidification and often appear halfway down in the middle of themolten zone or in the craters at the weld end. Crater shrinkages are oftenaccompanied by microscopic hot cracks. They are often observed in a widening ofthe molten zone or bulge related to poorly focused laser or electron beam. They aremore often found in very thick components and when high levels of impurities,sulfur and phosphorus, are found in the alloy. They are aligned with the axis of themolten zone. Cavities also include the pores formed by gas trapped during solidification. Theyappear in the form of isolated pores or distributed along the weld zone. They arefrequent in partial penetration welds. They occur more frequently when weldingthick components and in cases of poor cleaning (aluminum alloys, titanium alloy). Inlaser and EB weld beads, their size can vary from a few tenths of a millimeter to amaximum of two millimeters, a result of the molten zone’s narrowness. They arelocated mostly half way down or at the weld root.Lack of fusion or penetration The lack of fusion is a lack of connection between the base metal and the weldzone. It is a flat defect. It can be related to a discrepancy between the beam and theweld seam. In the case of a heterogenous assembly, it is due to a significant
78 Metallurgy and Mechanics of Weldingdifference in conductibility between materials. It is not easily detectable bynon-destructive tests. Lack of penetration is a lack of fusion between the edges to be welded. It islocated at the weld root. It is often caused by insufficient beam power or adegradation in beam focus.Shape defects We can distinguish the following defects: – undercuts: in the case of arc welding processes, these are due to a verylocalized lack of metal. They form an acute line on the surface at the front or on thereverse sides at the weld zone and base metal limits. In HEDB processes, undercutsare often due to a hollowing out of the weld bead on both sides of the molten zone.They are produced by an excessive power density or excessive welding speed. Theyare often encountered during the welding of titanium alloys; – insufficient thickness: this is caused by a collapse of the molten metal in theweld zone. There can be various causes: - a lack of material due to an excessive gap between the parts to be welded, - when welding very thick parts in flat position (the limits are: 20 mm for EBwelding, 15 mm for laser beam welding), - an excessive power density; – misalignments: these are due to a shift in position between the two parts to bewelded. This shift can lead to lack of weld root fusion.Projections (splatters) Metal splatter during welding can be adherent or not. It can be caused byexcessive power density, the presence of organic materials on the surface of the partor in the seam, or an inadequate gas protection. The welding of nitrided or carbo-nitrided steels can cause these projections.2.6.2. Weld inspection methods For HEDB welds, non-destructive tests make the detection of small defectspossible. The welding speed requires the use of fast and inexpensive control testprocedures. Controls can be carried out off-line (visual, radiography, ultrasound,magnetoscopy, Foucault current, etc.) or on-line (plasma analysis, infraredthermography, visually using a camera, etc.). In mass production, off-line controlcannot be applied to all components, so on-line testing is preferred. Very often, an
High Density Energy Beam Welding Processes 79on-line control is accompanied by sampling. In this case, a destructive test will beapplied to a selection of parts. Destructive tests (clamped side stamping tests, metallography, etc.) are long andexpensive. However, they make it possible to detect certain welding defects (cracks,lack of penetration or bond) and do not prejudge the total quality of the assembly.2.6.3. Standardization and qualification of the welding operating mode EB welding has been the object of thorough standardization. Laser beamwelding, a more recent process, is still in the process of standardization. The mainwelding standards are common today with ranges of different thicknesses for thetwo processes. The principal welding standards in force are as follows: – EN ISO 13.919-1: Welding – Joints welded by laser beam and electron beam –Guide to the quality levels of defects – Part 1: Steel; – EN ISO 13.919-2: Welding – Joints welded by laser beam and electron beam –Guide to the quality levels of defects – Part 2: Aluminum alloys; – EN ISO 15.609-3: Description of welding procedures by electron beam; – EN ISO 15.609-4: Description of welding procedures by laser beam; – EN ISO 15.614-11: Welding procedure test for electron beam and laser beam.2.7. Economic aspects The main obstacle to the large scale development of HEDB processes is theoperational and capital cost of this equipment. The investor must be certain of thetechnical advantage of the process but more especially its economic benefit. It isdifficult to speak about costs for rapidly evolving processes. We will limit ourselvesto touching on laser components and their operational and capital costs in order togive the reader the principal elements of any calculation [SAY 99].2.7.1. Cost of an electron beam machine The cost of a machine will vary according to the following factors: – technology selected: vacuum or non-vacuum, – electron acceleration voltage, – gun power,
80 Metallurgy and Mechanics of Welding – enclosure volume, – displacement systems of the parts and the gun. It is difficult in these circumstances to estimate a price. To give some ideahowever, a machine equipped with a 30 kW gun and with a 1 m3 enclosure pumpedin secondary vacuum will cost about €600,000. With regard to operating costs, the consumable costs are primarily electricity,cathodes and filaments whose lifespans vary according to use but can reach severaldozen hours. The principal operating costs lie in maintaining the cleanliness of theenclosure and the gun, which has a very significant impact on the equipmentproductivity (a clean enclosure leads to reduced pumping times) and on the weldquality (a clean gun cuts the risk of beam interruption owing to lack of insulation).2.7.2. Cost of a laser beam machine The hourly use rate of a laser system is mainly made up of paying off the capitalcost, consumables, and the expenses of maintenance and labor. The most significantpart of the total hourly rate is paying off the capital investment.Depreciation Companies tend to envisage increasingly shorter depreciation periods (less than3 years). In the overall investment costs, it is necessary to take account of the lasersource, the robot, the peripheral systems, the tools, the installation and integrationexpenses of the system.Consumables These depend on the laser system chosen.The CO2 laser system The “lasing” gas: consumption depends on the source type and the laser power.For lasers with fast axial flow, the gas outputs are low, about 30 l/hr for helium.Laser sources known as SLAB offer the lowest gas consumption. Shielding gas: the gas flow rates are about 15 to 30 l/min. The most expensivegas is helium; it is also the most frequently used because of its high ionizationpotential. Electricity: CO2 lasers have an electrical efficiency output of about 5 to 10%.The cost depends on the power used. It is important to take into account theconsumption of the complete installation, cooler included.
High Density Energy Beam Welding Processes 81 Maintenance: this is estimated to be 5% of the annual capital investment. Optics: the cost of optics can increase significantly if the optical path is badlydesigned. It depends on the number of mirrors in the optical path, the type of mirrorsand the protective systems used in the focusing head. It also depends on theprocedure (clean parts, presence of oxides or oil) and on the operating environment.YAG laser system Lamps: the cost depends on the number of lamps employed and their lifespan.Lamps in continuous YAG lasers have an average lifespan of 1,000 hrs. The lifespanof the lamps depends on their use and can reach 2,000 hrs. For a pulsed YAG laser, the lifespan is given as a number of pulses. This canreach several million pulses. Shielding gas: argon is more easily usable than in the case of the CO2 laser. Thegas flow rates are comparable. Electricity: a YAG lamp pumped laser has a lower electrical output efficiencythan a CO2 laser, about 1 to 3%. A YAG laser diode-pumped laser offers a muchbetter output of about 10%. Electricity consumption depends of course on the powerof the laser. Fiber-optics: these should not deteriorate in normal use. It is however necessaryto envisage their eventual replacement or repair. Focusing optics: these are very seldom replaced because of their glass protection.They are less expensive than lenses made of zinc selenium or mirrors. Protective glass: it is necessary to envisage the regular replacement of protectiveglass, at a frequency which will depend on the application. Currently the choice of a laser system is made at four levels: 1) choice of pulsed or continuous mode: this choice is determined by the type ofapplication (material to be welded, thickness, distortion, etc) and by the productionspeed required; 2) choice of the laser type (YAG or CO2): flexibility (fiber or mirrors), thicknessto be welded (powers available), materials (wavelength); 3) YAG laser pumped by lamps or pumped by diode: this issue is often raisedbecause of the recent development of diode-pumped YAG lasers. The advantage ofthis laser is uncertainly its high quality beam. It is however necessary to make thecomparison between the operating costs of both systems. A diode-pumped YAG
82 Metallurgy and Mechanics of Weldinglaser does not require a change of lamps and its electrical output efficiency is higher.However, the high cost of laser diodes makes its capital cost much higher than thatof a conventional YAG laser, which considerably increases its utilization cost. Areduction in the cost of laser diodes is expected, and this should reverse the trend; 4) choices of the mechanized system: the choice of a polyarticulated robot or aCartesian robot will depend on the application and the choice of the laser type (YAGor CO2). It should be noted that the capital cost of a Cartesian robot is definitelyhigher than that of a polyarticulated robot.2.8. Safety [HEE 00] The use of lasers in industry is recent and the technology is evolving quickly,which explains the regulatory weaknesses both in Europe and in France. Theprincipal reference text is standard NF EN 60.825-1 “Safety of laser equipment –Part 1: Equipment classification, requirements and user guide”. Other specificstandards cover particular questions such as: standard NF EN 12.626 December1997 “Safety of machines. Laser machines. Safety regulations” and standards NFEN 207 “Laser safety glasses” and NF EN 208 “Safety glasses for laser adjustment”,December 1998. The principal risks when using a laser are to the eye. They derive from thephysical characteristics of the laser. Certain radiations, according to theirwavelengths, are transmitted to the retina and are focused by the crystalline lens.The power density received can be 5.106 times higher on the retina than on thecornea. The retina is particularly vulnerable to radiation from the visible or near-infrared spectrum (0.4 to 1.4 m). If the density of energy received by the retina isexcessive, it can cause an irreversible lesion. Standard NF EN 60.825 classesvarious lasers according to their risk. For EB welding machines, apart from the risks related to the presence of highvoltages, which is controlled via the safety measures taken by the manufacturer, theprincipal risk is that of the production of x-rays, as previously mentioned. Thereagain, the precautions taken by the manufacturer should be sufficient and are thesubject of special attention at the time of delivery of the machine. It is thusincumbent on the user not to modify the equipment, particularly the enclosurewithout checking that the biological shields are properly in place.
High Density Energy Beam Welding Processes 832.9. Examples of industrial applications2.9.1. Electron beam welding The industrial applications of EB welding are now well-known and encompassall the industrial sectors, from the automotive (transmission components) andaeronautical (manufacture of jet engines) to the manufacture of diverse parts orsensors (Figures 2.38-2.40). Figure 2.38. Copper electrical connection (Techméta document) Figure 2.39. Stainless steel turbine
84 Metallurgy and Mechanics of Welding2.9.2. Laser beam welding We can list, in the following table, some well-known industrial applications. Application Industry Type of laser Materials Thickness Welding of Non-alloyed steels Automotive CO2 0.7 to 2 mm blanks coated or not Continuous Coated non-alloyed Bodyshells Automotive 1.2 mm YAG steels Gear box pinions Automotive CO2 Non-alloyed steels 2 to 5 mmTubular radiators Equipment Pulsed YAG Non-alloyed steels 1 mm Pipings Aeronautic CO2 Titanium alloy 1 mm Continuous Stiffeners Aeronautic Aluminum alloy 1 to 4 mm YAG or CO2 Plate heat Food CO2 Stainless steels 1 to 2 mm exchanger Aluminum, titanium, Casing closures Electronics Pulsed YAG 1 mm nickel alloys Continuous Oil filters Automotive Aluminum alloy 1 mm YAG Cardiac Medicine Pulsed YAG Titanium alloys 0.5 mm pacemaker Iron and steel Non-alloyed or slightly Pipes CO2 5 to 16 mm industry alloyed Power-assisted Continuous Automotive Non-alloyed steels 2 mm steering YAG Pulsed YAG, Aluminum alloy, Airbag initiators Automotive continuous 0.5 mm stainless steels YAG or CO22.10. Development prospects The two processes are often presented in opposition. This does not appearrealistic, each process having specific advantages which will make it better adaptedto a particular industrial application.
High Density Energy Beam Welding Processes 85 Figure 2.40. Superconducting niobium cavity (Techméta document) Figure 2.41. Automobile blank welding in aluminum alloy, 1.25 mm thick, power used 7.5 kW, welding speed 18 m.min-1 (igm Steigerwald Strahltechnik document) Electron beam welding reached its zenith in the 1970s. The application fieldswere the nuclear, aeronautical and automotive industries. Its principal handicap isthe vacuum enclosure. However, a renewed interest is currently noted with thedevelopment of new non-vacuum welding machines dedicated to automotiveapplications (see Figure 2.41). It should however be noted that, for several years, the appearance of sufficientlypowerful laser sources has led, for certain applications, to the replacement of EBwelding by laser welding because of an increased productivity related to the absenceof pumping. The main instigator of developments in laser welding processes hasbeen the automotive industry. After the welding of mechanical components (gearbox pinions), the welding of thin sheet was developed. Steelmakers started by
86 Metallurgy and Mechanics of Weldingoffering tailored welded blanks and today manufacturers invest in the spot weldingof bodyshells on a continuous production line. Electron beam welding machines are no longer the focus of significantdevelopments, whereas laser systems are evolving rapidly. Laser CO2 sources aremore compact, and the beams are of higher quality. A significant effort is beingmade to reduce consumables. The most significant developments relate to YAGlaser sources and diode lasers. The power of continuous Nd-YAG laser sources with cylindrical rods istechnically limited to 5 kW, to obtain a beam quality compatible with transport byfiber-optics. The advent of laser diode pumped systems makes it possible to increasethe power with equivalent beam quality. The ongoing developments in continuousYAG disk lasers will bring further improvements in beam quality and thus anincrease in the power of these sources. Lasers using laser diodes also offer great promise, because of their high outputand their low wavelength. Their use in welding is related to the improvement in thebeam focus. Amidst development projects, peripheral systems are not to be ignored. Theserelate to joint monitoring systems and on-line test systems. To improve the productivity of the laser welding process, efforts to combine alaser beam with an electric arc are underway. This new welding process is calledhybrid laser welding. The advantages of this process are numerous: – increase in acceptable gap between parts, – increase in welding speeds at equivalent laser power, – improvement of the laser/material interaction (aluminum alloys), – improvement of the metallurgy of welding by a reduction in the solidificationspeed, cooling rate and by the filler wire addition (reduction in the sensitivity to hotcracking). This process is promising. It should extend the range of laser applications.2.11. Bibliography[BAR 98] BAROUILLET C., CHEHAÏBOU A., “Soudage par faisceau laser CO2 d’un acier inoxydable martensitique à durcissement direct – Influence de l’azote comme gaz de protection”, 6th CISFFEL, vol. 1, 1998.
High Density Energy Beam Welding Processes 87[BOI 98] BOILLOT J.P., “La vision laser à haute vitesse, un atout indispensable pour…”, 6th CISFFEL, vol. 1, 1998.[CHE 93] CHEHAÏBOU A., GOUSSAIN J.-C., BAROUILLET C., “Etude de la sensibilité à la fissuration à chaud des aciers inoxydables austénitiques soudé par faisceau laser”, 5th CISFFEL, vol. 1, 1993.[CHE 98] CHEHAÏBOU A., GOUSSAIN J.-C., KNISPEL D., “Soudage par faisceau laser CO2 de différentes nuances d’alliages d’aluminum”, 6th CISFFEL, vol. 1, 1998.[COL 97] COLLECTIF, Etude du soudage par faisceau laser des aciers de mécanicien dans le cas d’un emboîtement – Investigation pour cerner la limite des nuances soudables, Rapport Institut de soudure no. 31729 (study financed by Cetim), November 1997.[DEL 56] DELONG W., OSTROM G., SZUMACHOWSXI E., “Measurement and calculation of ferrite in stainless steel weld metal”, Welding Journal, vol. 35, no. 11, 1956.[FRI 98] FRITZ D., LAZARENKO O.K., IRIÉ H., ABE N., OHMINE M., “Forty years of electron beam welding and material processing”, 6th CISFFEL, vol. 1, 1998[HAV 96] HAVRILLA D., Laser welding design and process fundamentals and troubleshooting guideline, Document Rofin Sinar, May 1990, revised 19 April 1996.[HEE 00] HEE G., MEREAU P., DORNIER G., Les lasers, Document INRS ED 5009, 2000.[HER 86] HERZIGER G., “The influence of laser-induced plasma on laser materials processing”, in David Belforte and Morris Levitt (eds.), The Industrial Laser Handbook, Penwell, 1986.[MAI 84] MAILLET H., Le Laser – Principes et Techniques d’Application, Lavoisier, 1984.[MUR 94] MURRY G., “Soudage et soudabilité métallurgique des métaux”, Techniques de l’ingénieur, M 715, 1994.[POW 00] POWERS D., SCHUBERT G., “Electron beam welding: the useful tool for the automotive industry”, Welding Journal, p. 35-38, February 2000.[ROE 86] ROESSLER D.M., “An introduction to the laser processing of materials”, in David Belforte and Morris Levitt (eds.), The Industrial Laser Handbook, Penwell, 1986.[RYK 74] RYKALINE N. N., Les sources d’énergie utilisées en soudage, Assemblée annuelle de l’Institut international de la soudure, Doc. IIS/IIW-465-74, Budapest, 1974.[SAY 99] SAYEGH G., “Eléments à considérer dans l’évaluation économique d’un investissement laser”, LaserAP3, Sarlat, 1999.[SCH 49] SCHAEFFLER A.L., “Constitution diagram for stainless steel weld metal”, Metal Progress, vol. 56, no. 11, p. 680, 1949.[SUU 79] SUUTALA N., KUJANPAA V., TALAKO T., MOISO T., “Correlation between solidification cracking and microstructure in austenitic-ferritic stainless steel welds”, Welding Research Int., vol. 2, p. 55, 1979.
Chapter 3 Thermal, Metallurgical and Mechanical Phenomena in the Heat Affected Zone As a general rule, welding operations modify the metallurgical structures and thelocal properties of the assembled parts deeply. In certain extreme cases, they can beat the origin of defects such as cracks, porosities or local embrittlement.Consequently, it is important to thoroughly understand the influence of variousfactors such as the thermal welding cycles and the chemical composition of the partsto be assembled. In this chapter, we will successively examine: – particular thermal phenomena associated with the operations of welding; – the microstructural modifications and principal metallurgical consequencesassociated with these thermal phenomena; – the modifications of the mechanical properties in the zone adjacent to themolten metal, i.e. in the heat affected zone (HAZ).3.1. Thermal aspects related to welding In spite of their great diversity, the welding processes have localized heatconcentration as a common characteristic.Chapter written by Dominique KAPLAN and Guy MURRY.
90 Metallurgy and Mechanics of Welding A welding operation can thus be described as a short passage of a small amountof matter at a very high temperature followed by a cooling, primarily by conductionin the adjacent parts: cooler adjacent metal, clamping tools, electrodes (in the case ofspot welding). The thermal cycle at any point close to the welded zone thusrepresents the heat dissipation associated with the welding, and thus depends onvariables related to the process (quantity of effective heat applied), on the material(thermal conductivity) and the configuration of the assembly. This localized heatingcan be carried out without displacement of the heat source (in the case of resistanceor aluminothermic welding) or by displacement of the source relative to the part (ingeneral arc and laser welding). In the second case, if a constant rate of travel is considered, the thermalcharacteristics of a quasi-stationary mode, where the temperature redistributionaround the source adopts a stable form in relation to time, can be determined. A resolution of the simplified heat equation was proposed by Rosenthal[ROS 46] as early as 1935, followed up by Rykaline [RYK 61], Clyde and Adams[CLY 58]. The principal points are the following: if one imagines a specific heatsource q moving at a constant speed along an axis x, the differential heat equation iswritten, in a series of coordinates (x,y,z) (see Figure 3.1): ² ² ² x² y² z² t [3.1]with: – : temperature; – t: time; – : thermal diffusivity (m2 s-1) of material = /pC, with: - : thermal conductibility (J m-1°K-1s-1), - C: voluminal calorific capacity (J m-3°K-1). A system of mobile coordinates can be defined related to the source by posing: = x - vt. In stationary mode ( = 0), the preceding equation then becomes: t
Thermal, Metallurgical and Mechanical Phenomena 91 ² ² ² v [3.2] ² y² z² Figure 3.1. Definition of the system of co-ordinates where a heat source moves at a constant speed v Figure 3.2. Diagrammatic flow of heat in the case of welding “thick” (a) or “thin” products (b) Equation [3.2] can be solved by considering two distinct situations (see Figure 3.2). In the case of welding “thick”1 products, the dissipation of heat occurs primarilyradially compared to the source. At any point, the change in temperature accordingto time and the distance is expressed: r² q v 0 e 4 t [3.3] 2 t1 The notions of thin or thick products will be quantified more precisely later.
92 Metallurgy and Mechanics of Weldingwith: – r: outdistance point considered compared to the source of heat (r = ( ² y ² z ² ); – q: calorific contribution (J); – v: rate of travel of source (m/s). The q/v term indicates linear energy or thequantity of heat introduced per unit of length of the welded joint; – 0: initial temperature. In the case of welding thin products, the heat dissipation is negligible in depth.The isotherms are thus perpendicular to the surface of the parts. A simplifiedsolution of equation [3.2] is written: r² q v 0 e 4 t [3.4] d (4 Ct ) 1 2where d indicates the thickness of the welded parts. Portevin and Séférian [POR 34] put forward a pictorial image, a thermal solid, torepresent welding temperatures in spatial terms, expressed in equations such as [3.3]or [3.4]. Figure 3.3 presents the example of such a diagrammatic representation, axisOx indicating the welding direction (x indicating distance as well as time), axis Oythe distance to the axis of the welded joint, and the axis Oz the temperature. With a given distance from the axis (y1 fixed), the thermal cycle (t) is describedby the intersection of the thermal solid with the plane parallel to (xOz) in y1. In thesame way, at a given temperature 1, the form of the isotherm is described by theintersection of the thermal solid with a plane parallel to (xOy) in 1. It is preciselyby using this last representation that the differences in temperature distributionduring welding of thin or thick products can be appreciated (see Figure 3.4). It willthus be observed that the network of isotherms is much denser upstream of thepassage of the heat source, which translates to the fact that the rise in temperature(heating phase) is faster than the descent (cooling phase).
Thermal, Metallurgical and Mechanical Phenomena 93 Cross-section of isotherms at different distances y Figure 3.3. 3D representation of welding temperature distribution in the case of a mobile source; from [EAS 83] Because of the finite speed of heat propagation, all the fibers parallel with thewelding axis do not simultaneously reach their maximum temperature. The plot ofpoints corresponding to this maximum is the curve (m). Compared to the direction ofdisplacement of the source of heat, all the points upstream of this curve are in theheating phase, and behind, in the cooling phase. The cooling and heating rates arecorrespondingly greater as the linear energy (q/v) is weaker or the products arethicker and the conductibility greater. In the case of welding of thin products, the temperature distribution is morespread out in the longitudinal and transverse direction than in the case of thickmaterials. The difference derives from the possibility, in this last case, of heatdissipation throughout its depth. Compared to materials with lower conductibility (e.g. austeniticstainless steel, 0.02 Wmm-1°C-1), the welding of material such as aluminum( 0.23 Wmm -1°C-1) leads to a widened isothermic distribution, albeitless extended in the longitudinal direction of the source displacement.
94 Metallurgy and Mechanics of Welding Figure 3.4. Example of temperature distribution during the welding of (a) thin or (b) thick sheet steel assembled under identical conditions; from [EAS 85] At this stage, we must keep in mind that the analytical calculations presented reston many assumptions (specific heat source, thermal properties independent oftemperature, ignoring latent heat due to phase transformations and heat losses byconvection or radiation, etc.). Although new digital methods (see for example [GRO94, KOV 86, WEI 95, ZAC 93]) allow for a more complete consideration ofparameters, experience shows that this simplified approach makes it possible tosolve the great majority of problems with satisfactory precision. Figure 3.5. Diagrammatic representation of the thermal cycle in HAZ. 700 800 Definition of the parameters M, t 300 , t 500
Thermal, Metallurgical and Mechanical Phenomena 95 We will now reconsider the thermal cycle (t) applicable at any point of theHAZ. Whatever the type of welding process (fixed source or mobile), it typicallycomprises (see Figure 3.5): – a very fast heating phase, of which the mean velocity is typically from some102°C/s (arc welding), rising to 104°C/s for the HDE processes such as laser welding[DEV 89]; – a passage at a maximum temperature M. In general, the duration at thistemperature is very short, and is all the more reduced the higher M is; – a more or less fast cooling phase. To simplify matters, we generallycharacterize the intensity of this cooling by time passing between two giventemperatures: 800 - either between 800 and 500°C, the cooling parameter is then t 500 , 700 - or between 700 and 300°C ( t 300 ). The relationship between this parameterand the previous one generally lies between 2 and 4. The choice of these two criteria was guided in particular by the fact that themajority of metallurgical transformations occur in these two temperature ranges inthe case of carbon-manganese steels. Experience actually shows that the final metallurgical structure at any point ofthe HAZ depends almost entirely on the maximum temperature M reached at this 800point, and on the cooling parameter as defined by t 500 . Certain thermal aspectsconcerning these two parameters will now be more fully developed.3.1.1. Maximum temperature attained in the HAZ It was seen that expressions like [3.3] and [3.4] described the temperature changeaccording to time in the respective cases of welding thick or thin products. Themaximum temperature is reached at a time tM such that: = 0. t tM Moreover, in order to avoid the singularity ( M ) when (r 0), the limitingcondition is imposed: M = f, melting point, when r = R, radius of the molten metaldeposit.
96 Metallurgy and Mechanics of Welding We are then led to the following expressions: – maximum temperature attained in the case of thick sheet welding (two-dimensional flow of heat in a section perpendicular to the welding direction): 1 e C ( r 2 R ²) 1 [3.5] M 0 2q v f 0 – maximum temperature attained in the case of thin sheet welding(unidimensional flow of heat in a section perpendicular to the welding direction): 1 2 e Cdr 1 [3.6] M 0 q v f 0 Figure 3.6. Evolution of peak temperature according to the distance to the fusion line. Comparison of the analytically calculated temperatures and those recorded in experiments (submerged arc welding); from [DEV 87]
Thermal, Metallurgical and Mechanical Phenomena 97 Thus, the maximum temperature in the HAZ varies in approximately inverseproportion to the distance r to the fusion line (i.e. in thin materials) or to its square(i.e. thick materials). In the case of plates, the maximum temperature reached doesnot depend on the product thickness. In spite of their simplicity, these expressions generally give a good account ofthe maximum temperature evolution in the HAZ, as Figure 3.6 testifies. Thispresents a comparison of experimental data recorded by thermocouples of thermalcycles in the HAZ, with the results of an analytical calculation (welding of thickproducts in the case presented here).3.1.2. Cooling parameter in the HAZ With the maximum temperature, the cooling speed, quantified by the parameter 800 t , is the most significant determining factor for the metallurgical structure of 500the HAZ. Expressions [3.3] and [3.4] make it possible to calculate: – the cooling parameter associated with thin sheet welding: t 500 = (q / vd )² 800 1 1 [3.7] 4 C (500 0 )² (800 0 )²(temperatures expressed in °C); – the cooling parameter associated with thick sheet welding: t 500 = q / v 800 1 1 . [3.8] 2 (500 0) (800 0) Readings of thermal cycles taken for welded joints [DEF 75, MUR 67] show thatthe cooling parameter varies very little within the same welded joint. In this way, itcan be said that the various zones of a welded deposit can be characterized by a 800 700single cooling parameter value t 500 (or t 300 ). The continuing evolution of themicrostructure thus depends only on that of the maximum temperature reachedlocally, all the points undergoing a practically identical cooling rate. It now remains to link the cooling parameter to the welding conditions in a moreprecise way: if welded joints are produced, starting from products of variousthicknesses while varying the linear energy of welding, the variation of the coolingparameter associated with these conditions is presented in Figure 3.7.
98 Metallurgy and Mechanics of Welding Figure 3.7. Influence of the thickness and linear welding energy on the cooling parameters Beyond a certain thickness, the cooling parameter does not vary. This criticalthickness, called the thickness limit, is correspondingly higher the greater thewelding energy is. From the point of view of welding, a product will thus beregarded as “thick” for a given energy of welding, if its thickness is higher than thethickness limit. In reality, this concept of thickness limit represents the modification of the natureof heat dissipation in the welded joint: below the limit, the flow of heat is two-dimensional, with normal isotherms compared to the plane of the product. Beyondthis, the flow is three-dimensional and the isotherms take on a cylindrical form.There exists a zone of transition between these two modes, where the isothermalform is affected by radiation to the lower part of the component. In practice, it is important to define the welding linear energy (term q/v in thepreceding expressions) encountered in this phenomenon. This is the product: – of linear electrical energy Ee, defined from the welding parameters: forexample, in arc welding, carried out with a voltage U and current intensity I, the UIexpression can be written: Ee , E being frequently expressed in kJ/cm; v – of a thermal efficiency coefficient P, intrinsic to the welding process used,which characterizes the relationship between the energy actually transferred to thepart and electrical energy. Table 3.1 indicates generally accepted values.
Thermal, Metallurgical and Mechanical Phenomena 99 Welding process Thermal efficiency p Submerged arc welding 0.9 to 1 Welding with coated electrode 0.7 to 0.85 MIG welding 0.7 to 0.85 TIG welding 0.2 to 0.8 Electron beam welding 0.8 to 0.95 Laser 0.4 to 0.7 Table 3.1. Thermal efficiency coefficient of various welding processes; from [CHR 65, CON 87, DEV 85, GRO 94, ION 97, NIL 75] It will be noted that TIG welding’s efficiency is generally low and varies withmany factors: intensity, DC or AC, shielding gas, etc. In the same way, theefficiency of laser welding is very variable according to the reflectivity of the part:low for copper or polished aluminum parts, the efficiency (and thus the beampenetration) can be increased by depositing a fine layer of graphite or zincphosphate. The linear welding energy is also the product of a coefficient G relatedto the geometry of the deposit and assembly. By definition, a flat deposit(heat diffusion at an angle of 180°) will be expressed as: G = 1. A T-shapedassembly (diffusion of heat at 270°) will be characterized by the coefficient 180 2 G = . This approach can be generalized for more complex examples 270 3(preparation of X-shaped, V-shaped chamfers, etc.). UI The effective linear welding energy is then written: E = P G . v This value, as well as the thickness of the welded products, makes it possible todefine the thermal welding mode: in a remarkable study [BER 72] based on atheoretical and experimental approach, G. Bernard could specify the field of thickand thin products with respect to welding heat dissipation.
100 Metallurgy and Mechanics of Welding 800 Figure 3.8. Graph determining the cooling parameter t 500 according to the welding conditions; from [ATS 80]
Thermal, Metallurgical and Mechanical Phenomena 101 In the absence of pre-heating ( 0 = 20°C), a part will be regarded as thick based 800on the criterion t 500 if its thickness d (mm) is such that: d > 4.5 E 700E being expressed in kJ/cm. In the case of the criterion t 300 , this condition wouldbe written: d > 6.35 E From such criteria, it is then possible to calculate the t parameter valuesaccording to expression [3.7] or [3.8]. To enable rapid estimations, IRSID [ATS 80] developed a forecast graph of the 800value of t 500 starting from the various parameters in the case of arc welding (seeFigure 3.8). Thus, as an example, we can consider a TIG welded joint with an UIenergy of 15 kJ/cm on a T-shaped assembly. Starting with electrical energy v(point A), corrections related to the geometry of the assembly (point B) and to theefficiency of the process lead to an effective energy E (point C) of 5 kJ/cm. Underthese conditions, the welding of 8 mm thick materials will lead to a value of 800 t 500 of 4 seconds (D). Another example (MIG welding at 20 kJ/cm) shows how it is possible to takeaccount of the pre-heated temperature 0 (here 200°C) by a correction of thethickness and effective energy. As an indication, Table 3.2 gathers some typical values of cooling speedsobserved for various welding processes, in the range of thicknesses used in theseprocesses. Welding resistance TIG, LASER Flash Coated MIG, Submer- Electroslag process (spot, ERW, electrode MAG ged arc Electrogas roller…) plasma 800 t500 <1s <3s <5s 1-10 s 2-15 s 4-30 s 5-50 s 100-250 800 Table 3.2. Typical cooling speed values t 500 of various welding processes
102 Metallurgy and Mechanics of Welding3.2. Microstructural modifications in the HAZ: metallurgical consequences of thethermal cycles of welding3.2.1. Transformations in the HAZ during heating In a strict sense, the rapidity of the welding thermal cycles does not make itpossible to use the balance diagrams to forecast the true nature of the various phasesin the vicinity of the line of fusion. However, following the example of Easterling[EAS 83], this type of diagram is a suitable starting point to interpret themicrostructural modifications qualitatively. To serve as an example, structural steels,which are the most widely used in welding applications, will be considered byexamining the diagram (Fe-C) in parallel with the maximum temperatures reachedin a welded joint (see Figure 3.9). Figure 3.9. Presentation of the various constituent parts of a welded joint; from [EAS 83] Let us consider for example the case of welding a 0.15% steel. As we approachthe molten zone, the following zonal situations are to be found. The base metal has not undergone a transformation phase in the heating, i.e. ithas been heated to a temperature lower than the transformation point A1 (727°C). Onbalance, it is thus a microstructure made up of ferrite (solid solution carbon
Thermal, Metallurgical and Mechanical Phenomena 103insertion in iron, of a centered cubic structure) and of iron carbides Fe3C (orcementite) or more precisely of pearlite, a lamellar aggregate of ferrite andcementite. We have a subcritical zone, where a phase shift has not yet occurred. However,when the temperature reached is sufficiently high (for example >600°C), certainphenomena such as tempering, the spheroidizing of the cementite lamellae, therecrystallization in the case of welding of strain hardened products, ageing, etc., canpossibly occur [GRA 95]. We also have a partial transformation zone (or intercritical zone), between A1and A3 ( 830°C for the composition considered). In this field ferrite coexists with anewly formed phase, austenite , a solid insertion solution of cubic centered facestructure. It is starting from this zone ( > A1) that the heat affected zone begins. From temperature A3 up to approximately 1,495°C, the transformation intoaustenite is total. The new structure thus replaces and erases any trace of the formerferritic structure. It is within this zone that an austenitic grain enlargement occurs:this is of a very small size at temperatures slightly higher than A3, and can reach afew hundred microns for the highest temperatures. In this case, the term employed iscoarse grain zone (for example, when the austenitic grain size exceeds a few tens ofmicrons) and in general it is this zone which is the most likely to cause certainmetallurgical problems, as will be seen later. We have another zone partially in the liquid state, where a solid ferritic phase ( )and a liquid phase coexist. Very small in size (and thus difficult to observemicrographically), this zone constitutes the connection between the base metal andthe molten metal. On the balance diagram, this corresponds to the temperatureinterval between the beginning and the end of fusion (solidus-liquidus interval). Certain phenomena (local decarburization by enrichment of the liquid in thesolute, intergranular liquation by eutectic formation at low melting point in the caseof impurities, etc. [GRA 95, HAL 84]) can intervene in this bond zone. Finally, the molten metal often has a composition different from that of the basemetal, because of the volatilization of certain elements, reactions with thesurrounding medium, or of enrichment by external elements (filler material). Thefirst molten metal nuclei are solidified by epitaxy (crystallographic coherence) onthe grains of the HAZ. At this stage, it is necessary to note the following points: – the transformations and temperature ranges evoked above correspond to a stateof balance. In reality, the brevity of the thermal cycles means that phase
104 Metallurgy and Mechanics of Weldingtransformations and structural homogenity intervene at temperatures sometimesconsiderably higher than these balanced temperatures; – the particular case considered here (alloy Fe-0.15% C) presents a situationwhere phase shifts occur during heating. In the case of other materials (for example:aluminum alloys, copper, ferritic stainless steels, etc.), the thermal welding cycleintervenes in a single-phase area. A grain enlargement will then be found throughoutthe cycle, without possibility of refinement by phase shift; – starting from expression [3.5] or [3.6] and the knowledge of the phasetransformation temperatures, it is possible to predict the HAZ width in variousconditions of welding. The calculations, confirmed by observations of welded joints,show that this can vary from a few hundreds of microns (for example: low powerdensities in laser welding [ION 97] and resistance welding [CHA 74]) to 15 mm inelectroslag welding [DEB 82, HAR 80]. In addition to these microstructural modifications, welding operations have amarked influence on the precipitates possibly present in the base metal. Indeed, it isknown that modern steels draw their mechanical properties (resistance, ductility,toughness) from an optimized combination of hardening, by the nature of themicrostructure, the grain and precipitation refinement. This balance is significantlymodified by the thermal welding cycles. Generally, the dissolution of various particles (carbides, nitrides, sulfides,oxides) can be quantified, starting from the variation of their solubility product withthe temperature, described in this form (case of diluted solutions) [RIS 74]: M aN b aM + bN, a and b defining the stoichiometry of the initial compounds: Go B log [%M] a [%N] b = =A– RT T G 0 indicates the free energy of the reaction, T the absolute temperature, R theconstant of perfect gases (1,987 cal. K-1 mol-1). Table 3.3 and Figure 3.10 present thesolubility product of some compounds, from which the temperature at which theyare totally soluble can be calculated.
Thermal, Metallurgical and Mechanical Phenomena 105 Type of precipitate A– B T NbN 4.04 – 10230/T VN 3.02 – 7840/T AlN 1.79 – 7184/T TiN 4.35 – 14890/T TiC 5.33 – 10475/T NbC 2.26 – 6770/T MnS 2.93 – 9020/T Al2O3 20.43 – 125986/T SiO2 5.10 – 44801/T MnO –5.71 – 24262/T Ti2O3 16.18 – 104180/T Table 3.3. Expression of the solubility product of various compounds in austenite; concentrations in % by weight, T in °K The higher the temperature reached locally in the HAZ, the greater the likelihoodof precipitates decomposing. In decreasing order, the stability of these compounds isas follows: oxides, nitrides, sulfides, carbides. For common compositions of structural steels, decomposition of carbides in theHAZ will be observed around 1,100-1,150°C (VC, TiC) [HRI 95], nitrides around1,150 to 1,300°C, sulfides being generally dissociated around 1,100 to 1,200°C.Taking into account their very strong stability, oxide inclusions resulting from the steelmaking in the liquid state (alumina, silicates, etc.) are not affected by the weldingcycle. Being very few, and relatively large in size (for example: several tenths to a fewmicrons), these oxides generally do not play a role at the time of the heating phase inthe HAZ. It is not the same for nitrides or carbo-nitrides. Indeed, it is known that thesenumerous, fine and dispersed particles slow down the growth of austenitic grain sincethe joint displacement this achieves is accompanied by a local increase in enthalpy.
106 Metallurgy and Mechanics of Welding Figure 3.10. Solubility products of various compounds in austenite Maximum size of grains dmax , in the presence of a population of precipitates ofsize r and whose voluminal fraction is VF, can be expressed by the Zener relation 4r[ZEN 48]: d max . 3V f In general, an increased austenitic grain size in the HAZ leads thereafter to acoarser ferritic structure. To limit this phenomenon, it is possible to show that lowadditions of titanium (an element which forms, as was seen previously, very stablenitrides at high temperature) slow down the growth of the austenitic grain effectively(see Figure 3.11). It should however be stressed that this result is obtained only ifthese nitrides are relatively fine (a few tens of nanometers), i.e. primarily if they areformed after solidification during steelmaking and not in the form of coarserprecipitates (micrometric particles, formed in the molten metal).
Thermal, Metallurgical and Mechanical Phenomena 107 Figure 3.11. Influence of maximum temperature on the austenitic grain size in HAZ of steels containing various types of precipitates; from [KAN 76]3.2.2. Transformations in the HAZ during cooling In the case of structural steels, the microstructures observed in the HAZ ofwelded joints correspond to transformed products of austenite. It is in fact difficultto study these metallurgical transformations starting from traditional CCT diagrams(continuous cooling transformation). Indeed, these are generally established startingfrom austenitic treatments at a relatively low temperature (900-950°C) and for longdurations, i.e. a situation exactly opposite to that encountered in the HAZ. In orderto consider more representative conditions, the metallurgical phenomena startingfrom thermal heating and cooling cycles very close to those met in welding arestudied. These tests are generally carried out on specific thermal simulators (Gleebleand Smitweld simulators, etc.). For a given material (see Figure 3.12) andaustenitization conditions (temperature generally higher than 1,200°C, so as tosimulate the HAZ with coarse grains), the transformations of the austenite accordingto the cooling speed using the CCT diagram in welding conditions or more simply ofthe evolution of hardening the final microstructure with temperature can begathered.
108 Metallurgy and Mechanics of Welding Figure 3.12. (a) Example of CCT diagram in welding conditions ( M = 1,300°C); (b) corresponding graph (hardness-criterion of cooling t). Steel C = 0.18%, Mn = 1.4%, Si = 0.4% According to the cooling speed, various types of microstructures are liable to beformed. For very high speeds (lower than the critical quenching rate VCM, whichcorresponds to a plateau on the hardness-criterion cooling graph or HV- t),martensite appears. Having a tetragonal crystallographic structure, thissupersaturated solid solution of carbon in iron is formed by a shearing mechanismwithout atomic diffusion. Identical in composition to that of the mother austenite,martensite has a hardness HVM which depends virtually only on the percentage ofcarbon in the steel alone, according to the expression: HVM=283+930(%C)[IRS 77]2. At intermediate speeds, bainitic structures appear. Formed starting frommetastable austenite at temperatures too low for the carbon to be able to diffuse atthe grain boundaries, the bainite is characterized by the very fast growth of ferriteneedles by shearing and a precipitation of carbides. Without returning to thecomplex debate relating to the description of bainitic structures (see for example[BHA 97, HEH 72, HON 95, OHM 74]), we will simply recall that faster cooling2 Other similar expressions have been proposed: HVM = 293+812(%C) (Satoh),305+802(%C) (Duren) or HVM= 294+884[%C(1-0.3 (%C))²] (Yurioka), etc.
Thermal, Metallurgical and Mechanical Phenomena 109speeds lead to the formation of the harder lower bainite structures (carbideprecipitation in the shape of thin platelets within the ferrite laths), whereas slowerspeeds are associated with higher bainite formation (carbides rejected from theferrite lath joints, sometimes in the form of quasi-continuous cementite lamellae[CON 92]). In this last case, the local carbon content can be such that the formationof compounds between the laths occurs where martensite and austenite coexist (M-Acompounds), the latter being stabilized because the transformation temperature Msis lowered below room temperature [AND 65]. Slower cooling speeds in welding correspond to the precipitation of proeutectoïdferrite at the old austenitic grain boundaries and the evolution towards a ferrito-perlitic structure. It is also in this range of cooling speeds that some compounds(vanadium and niobium nitrides or carbo-nitrides, etc.), dissolved at the time of theheating phase, can re-precipitate in a more or less complete form. Various more or less complex formulae have been proposed in order to describethe evolution of HVmax hardness in the large grained HAZ of C-Mn steels accordingto their composition and the speed of cooling. We can for example quote that ofYurioka [YUR 87], applicable to steels of less than 0.3%C, 5%Ni, 1%Cr without B 800( t 500 expressed in s, content in %): HVmax= 206 + 442 C + (402 CEI – 90 CEII + 80) arctan (x) + 99 CEIIwith: Mo Mn Cr Ni Cu Si CEI = C 4 6 8 12 15 24 Mo Nb Mn Cr V Cu Ni Si CEII = C 2.5 3 5 10 18 24 x= CEIII = These expressions reveal the concept of carbon equivalent (CE, a function of thelevel of C, M, Mo, etc.), which will be subject of further discussion in connectionwith cold cracking. At this stage, it must be retained that it is a factor quantifying the
110 Metallurgy and Mechanics of Weldingcapacity for hardening. At a given cooling speed, limiting hardness amounts tolimiting the percentage of carbon equivalent. As has been previously stressed, the microstructure formed at any point of theHAZ depends on the temperature reached locally. Figure 3.13 illustrates, in the caseof a 32C1 steel, the influence of the temperature on the transformation of austenite. 700If cooling is sufficiently fast (for example, t300 <1 s), all the zones where thetemperature exceeds 1,000°C are martensitic. In the case of a slower cooling (for 700example, t300 5 s), the part of the HAZ heated to around 1,000°C has a bainiticstructure, whereas the coarse grained part of the HAZ (1,100 to 1,200°C) ismartensitic. This microstructural difference explains why the majority of themetallurgical problems (toughness, sensitivity to cracking in the presence ofhydrogen) occur primarily in the coarse grained part of the HAZ, heated to a highertemperature. Figure 3.13. Influence of maximum temperature in the HAZ on a CCT diagram in the welding of a steel 0.3% C, 0.8% Mn, 0.2% Si, 0.3% Cr3.2.3. Case of multipass welding Beyond a certain thickness, the product assembly generally involves a number ofsuccessive deposits (welding involving several passes, or multipass). Except in thelast deposit, all the points of the HAZ undergo, during this operation, a complexsuccession of reheating cycles [DEV 87]. In reality, if a point is located in the HAZ
Thermal, Metallurgical and Mechanical Phenomena 111in the immediate vicinity of given pass N, the progressive distance of the depositsmeans that their metallurgical influence quickly becomes negligible (maximumtemperature lower than 500°C) beyond pass N + 2. Moreover, it is understood thataustenitization at very high temperature erases the metallurgical influence of thepreceding cycles at lower temperature; therefore, the metallurgically effectivethermal history in a multipass HAZ can be summarized with some characteristiccombinations, comprising at most three thermal peaks. Thus, the three followingzones can be distinguished (see Figure 3.14). Figure 3.14. Diagrammatic illustration of the thermal cycles and the microstructures encountered in multipass welding; from [MAT 94] A zone with coarse grains is unaffected by the subsequent passes, because it isheated to a temperature lower than Ac1 (zone A in the figure, or SRCGHAZ:subcritically reheated coarse grain heat affected zone). In general, themicrostructure and the mechanical properties of this zone are relatively close tothose of a zone with coarse grains in a rough state (CGHAZ, zone D). A zone with coarse grains heated in the intercritical field, between Ac1 andAc3 (ICCGHAZ: intercritical reheated coarse grain heat affected zone, zone B).The transformation ( ) occurs in particular in the zones of easy diffusion, suchas the former austenitic grain boundaries, the zones richest in carbon (carbides, M-Acompounds) or the segregated zones. The austenite which is formed locally isincreasingly carbon enriched the lower the temperature is. With cooling, the
112 Metallurgy and Mechanics of Weldingaustenitic sites can be transformed into martensite or to austenite (M-A compounds)according to a mechanism described in the preceding section. As many studies havehighlighted the poor character of these compounds with respect to toughness [IKA80, LAM 99, MAT 94], it is generally considered that the zone heated in theintercritical field is, with the coarse grained zone, the zone of least toughness inmultipass welded joints. However, the brittleness of this zone all but disappears witha reheating to a sufficient tempering temperature (for example: 350-400°C) relatedto the deposit of a subsequent welding pass or a stress relieving heat treatment. When structural steels must provide guarantees of toughness in multipass weldedjoints, manufacturers and steelmakers particularly endeavor to minimize theproportion of local brittle zones (LBZ, coarse grain or intercritical zones [HRI 95,TOY 86]) in the vicinity of the molten metal by controling the conditions of weldingand the chemical composition. Finally, a zone with fine grains (FGHAZ, fine grain heat affected zone) isencountered, associated with a temperature peak slightly higher than Ac3. The veryfine microstructures associated with this type of treatment correspond to structuresresulting from normalization treatments and present excellent mechanical properties.A wise choice of welding conditions, so as to maximize this zone with fine grainsand to favor the transformation of M-A compounds, makes it possible to guaranteegood toughness properties of multipass joints [IKE 95, KAW nd, KOS 81, LIN 89]. To conclude, it should be noted that certain software, based on a thermal andmetallurgical modeling, have been developed in order to forecast the risk of brittlezones appearing in multipass HAZs and their effects on mechanical properties [DEV91, KAP 98, REE 94].3.2.4. Cold cracking The concept of weldability has often been confused with and reduced tosensitivity to cold cracking, which gives some indication of the importance of thisphenomenon. During arc welding, the molten metal is likely to dissolve hydrogen derived fromthe decomposition of water present (ambient air, moisture, etc.), or from that ofhydrogenated matter (greases, etc.) and possibly from hydrogen in the welding gas;the dissolved quantity can be high. Results published by Granjon [GRA 95] showthat, during structural steel welding, the quantity of diffusible hydrogen present in100 grams of molten metal can reach, on average: – 15 cm3 in welding with electrodes with a rutile coating,
Thermal, Metallurgical and Mechanical Phenomena 113 – 9 cm3 in welding with powdered flux, – 7 cm3 in welding with electrodes with a basic coating, – 4 cm3 in MIG welding. During solidification, cooling and any possible allotropic transformations, thesolubility of hydrogen decreases appreciably. This fact could be responsible for theformation of porosities during solidification and will generate thereafter a diffusionof gas towards the atmosphere and, if this is insufficient (fast cooling), asupersaturation of the solid metal with in situ formation of H2 molecules. The gasthus produced gathers in the spaces caused by structural defects and decohesionsbetween metal and inclusions. In these places, the gas pressure rises with thediffusion of hydrogen and can reach elevated levels, which generates considerablelocalized stresses likely to combine with shrinkage stresses. If the structural state ofthe metal is not sufficiently strong under these conditions, a crack is likely todevelop. This precise situation is encountered during the welding of structural steels likelyto undergo a ( ) transformation; it leads to cold cracking. Indeed, in a joint: – the transformation in molten metal (when it is susceptible to a ( )transformation, which is generally the case) starts before that of the HAZ because, ifit cools like the latter, it is lower in carbon and its Ms point is higher. Any hydrogencontained is thus released, partially towards the atmosphere and partially towards theHAZ (as long as the latter is in an austenitic state); – the ( ) transformation in the HAZ, by the effect of heat gradients and thedifferences in hardenability caused by the enlargement of the austenite grains,progresses from the coolest parts (close to the base metal) towards the limit of themolten metal. Consequently, hydrogen is trapped in the most overheated part of the HAZ,whereas its solubility decreases as a result of cooling and especially from thepassage to the state. If this part is transformed into martensite (not very plastic,even brittle), it can fissure under the action of stresses caused by the localizedhydrogen pressures and the shrinkage stresses. Thus, cold cracking will occur. To assess the risks of cold cracking, it is necessary to carry out tests for crackingunder the welding conditions considered. If it is easy to reproduce thermal cyclesand the hydrogen loading (it is sufficient to apply identical welding conditions), it ison the other hand very difficult to reconstitute the pattern of shrinkage stresses. Forthis the tests employed will be conventional. The most common and most significant
114 Metallurgy and Mechanics of Weldingis the implant test defined by French standards NF A 89-100 and NF A 03-185 andby the recommended procedure IIS/IIW-447-73. A notched cylindrical test-piece isimplanted in a thick plate. The test weld is carried out under the selected conditionsthen, upon the solidification of the molten metal, the implant is subjected to traction(see Figure 3.15). Figure 3.15. a) Example of implant with a circular notch; b) implant subjected to traction after deposit of a weld bead Micrographic sections taken after cooling and waiting time allow the detection ofpossible cracks. While simultaneously varying the welding conditions (energy andthickness of the support plate) and the load applied to the implant, we have thenecessary information to plot a cracking curve which distinguishes, within thetensile effort/cooling parameter coordinates, the fields where cracking occurs andwhere it is avoided (see Figure 3.16). Such a curve is characterized by the steel, thewelding process and the hydrogen content under consideration. This procedure hasmade it possible to qualify the metallurgical weldability of many steels with respectto the risk of cold cracking and to define minimal energies to employ when weldingthem without risk. It should however be noted that the influence of hydrogen contentis foremost; it is often enough to lower this to make cold cracking disappear, asshown in Figure 3.17 for a simple C-Mn steel. It is then this factor that the welderwill have to consider as a priority.
Thermal, Metallurgical and Mechanical Phenomena 115 Figure 3.16. Example of a cracking curve determined from the implant test However, if lowering the hydrogen content is impossible or insufficient, thewelder can still intervene by carrying out a careful pre-heating and possibly a post-heating. These two operations (which we should not regard as being heat treatments)consist of modifying the thermal evolution of a weld by heating up the parts whichconstitute the assembly at a higher temperature than room temperature (this is pre-heating) and possibly by maintaining this heat, after welding, for a given time (thisis post-heating). Figure 3.17. Influence of hydrogen content on cold cracking
116 Metallurgy and Mechanics of Welding These procedures: – slow down the joint cooling which is applied with a cooling medium – the basemetal – no longer at room temperature but maintained at the temperature of pre-heating. If the base metal is not too hardenable, this slowing down modifies the ( ) transformation by allowing a certain proportion of bainite to form before themartensitic transformation; the metal of the HAZ is less hardened and thus less hardbut especially less brittle. In addition, starting from the pre-heating temperature justas starting from the temperature of post-heating, the final cooling is very slow sinceit corresponds to all of the pre-heated and possibly post-heated area. The end of themartensitic transformation thus occurs very slowly in the presence of a hydrogenquantity which gradually decreases since it diffuses into the atmosphere, outside thejoint. The relatively long duration of post-heating and between the latter and theambient temperature constitute a tempering operation to which the already formedmartensite is subjected, causing a further decrease in its brittleness; – increase the HAZ depth and decrease the temperature gradients. The dilationgradients are in this way decreased and, consequently, the possibilities of shrinkageand thus significant stresses are reduced. All these effects have the same beneficial result; they decrease or eliminate therisk of cold cracking. To assess a priori the risk of cold cracking, on a practical level, a particularparameter called carbon equivalent (Ceq) has been used on a regular basis,calculated on the chemical composition of the parent metal. Many formulae havebeen proposed, the best known being that employed since 1940 by the InternationalInstitute of Welding [DEA 40]: Ceq (%) = C% + Mn%/6 + (Cr% + Mo%+V%)/5 + (Cu% + Ni%)/15 With a constant Ceq, metallurgical weldability would be constant and the lowerthe Ceq, the lower the risk of cold cracking. Such a method of assessing this riskdoes not appear very satisfactory, indeed: – Ceq does not take into account the hydrogen content of the molten metal, theimportance of which has just been discussed (certain formulae have been proposedwhich remedy this oversight); – Ceq does not take into account the cooling conditions, which are a determiningfactor concerning the proportion of martensite formed; – Ceq regrettably confuses the capacity for hardening (and thus the risking ofmartensite brittleness) which depends on the percentage of carbon and secondly
Thermal, Metallurgical and Mechanical Phenomena 117hardenability (and thus the risk of martensite formation) which depends on thecontent of alloying elements. Ceq can therefore only be used to make comparisons within very limited fields. Currently, some NF EN standards define limiting values for this Ceq. As anexample, and to highlight the improvements in weldability achieved thanks to thedevelopments in iron and steel processes, the maximum guaranteed value can becited for steels meeting standard NF EN 10113 and delivered in a normalized stateor after thermomechanical treatment in the form of flat products with a thicknessranging between 16 and 40 mm. Lastly, it is important to stress that the development of many iron and steelproducts during the last few decades has been guided mainly by the desire todecrease the sensitivity to cold cracking. Consequently, the concept of metallurgicalweldability has played a crucial role in the evolution of structural steel composition. Ceq maximum (%) of steels according to NF EN 10113 (16 < thickness mm 40) Part 2 Part 3 after normalization after thermomechanical rolling S275N Ceq <= 0.40% S275M Ceq <= 0.34% S355N Ceq <= 0.43% S355M Ceq <= 0.39% S420N Ceq <= 0.48% S420M Ceq <= 0.43%3.2.5. Lamellar tearing It will be noted later that welding leads to the formation of stresses andsignificant deformations. A possible consequence of this phenomenon is lamellartearing, which corresponds to a particular type of crack developing parallel to thebond zone of the welded joints and perpendicular to the grain of flat-rolled products(see Figure 3.18). Its appearance corresponds to an insufficient ductility of thewelded material in the direction of its thickness, caused by the presence ofinclusions aligned in the direction of rolling.
118 Metallurgy and Mechanics of Welding Figure 3.18. Cracking due to lamellar tearing Examination of the ruptures primarily reveals a characteristic step-like breakcorresponding to decohesion between the inclusions (essentially sulfides) lengthenedby rolling and the matrix. This type of cracking can be avoided: – by the joint design, avoiding procedures which lead to high levels of stress inthe short transverse direction as much as possible (geometry, preliminary buttering,limitation of the elastic limit for the molten metal, etc.); – by the choice of the metallurgical quality of the steel, which must have asufficient ductility in its thickness. This characteristic is checked on cylindricaltensile test-specimens taken in this direction, and on which striction (Z%) ismeasured after rupture. So we talk about “Z… steels” in connection with productswith guaranteed properties in their thickness, which are obtained by limitating theinclusion content (in particular expressed by the sulfur behavior) and/or controlingthe morphology of these inclusions (treatment in production by addition of calcium,rare earths (cerium, etc.) [OLE 81], etc.).3.3. Influence of the thermal cycles on the mechanical properties of the HAZ Important modifications in microstructures caused by welding are naturallyaccompanied by significant changes in the mechanical properties compared to thebase metal. These will be examined with regard to localized tensile, hardness ortoughness properties.
Thermal, Metallurgical and Mechanical Phenomena 1193.3.1. Modifications of the mechanical properties of hardness or traction in theHAZ The modifications of mechanical properties in the HAZ (mechanical resistance,or more simply hardness [GRU 81]) must obviously be understood in comparisonwith the base metal, whose properties can result from various combinations(thermomechanical composition/treatments). Thus, it is possible to enumerateamong the big groupings of structural steels, for example the C-Mn steels of ferrito-pearlitic structure obtained by normalization treatments, high strength steels (HSLA)combining refinement of the ferritic grain and fine hardening precipitation, steelswith high or very high strength (ferrito-bainitic, or bainitic with very low carbon(ULCB)), dual-phase steels (ferrite-martensite), quenched and tempered steels, etc. In general, the thermal cycles associated with the coarse grain zone lead to alocalized increase in hardness compared to that of the base metal, particularly in thecase of a fast cooling after welding. The purpose of this mechanical heterogenity isoften to displace the rupture site towards the base metal in the case of smooth tensileor bending tests across the welded joints. In the case of mechanical tests comprisinga notch located in the HAZ, the presence of the less hard adjoining base metalcontributes to the development of a plastic zone and to a rise in apparent toughness[DEV 86a]. In certain extreme cases (very large difference in hardness between thewelded zone and the base metal, very narrow welded zone, as in the case of weldsby laser or electron beam), a marked deviation of the rupture can be noted towardsthe least hard zones [DEV 86b, GOL 76]. More generally, this illustrates the possible difference between intrinsicmechanical behavior in a given zone and that obtained in the presence of theadjoining zones with different behavior patterns, possibly in the presence of amechanical defect. The whole of these rather complex questions, the interaction ofthe mechanical properties in the various parts of the welded joints, is known as thematching of welded joints (see for example [LON 94, TOY 92]). In certain cases (base metal with high yield strength obtained by thoroughthermomechanical treatment), the thermal cycles can involve the formation ofsoftened zones compared to the base metal. Softening appears at a temperaturecorresponding to Ac1 or Ac3 [DEV 83, ITO 00] and increases the higher the energyis (for example: aluminothermic welding of rails). Very often, the triaxiality of thestresses and the localized consolidation make it possible to avoid an excessiveconcentration of deformations within the softened zone. It is advisable to limit theamplitude of softening (difference in hardness between the base metal and the HAZ)as well as the width of the softened zone [DEV 84], so as to avoid rupture or apremature wear by concentration of the deformation in this zone. Finally, it shouldbe noted that the presence of this softened zone can sometimes be associated with a
120 Metallurgy and Mechanics of Weldingcracking due to localized hydrogen (stress oriented hydrogen induced cracking, orSOHIC) [TAK 95].3.3.2. Toughness properties of the HAZ The mechanical properties in the HAZ are the subject to increasingly severedemands from users and of construction codes, with the aim of guaranteeing theviability of the welded joints with respect to brittle fracture. The toughness of theHAZ can clearly be assessed by direct removal of notched samples from withinwelded joints. However, this method presents many difficulties (delicate positioningof the notch within very narrow zones with high microstructural gradients, residualstresses, etc.) which leads in practice to an excessive spread in the toughness results.This is why the tenacity of these zones is often assessed on the basis of experimentalon test-samples that have undergone simulated thermal treatments representative ofthose encountered in the HAZ. On the basis of such simulation tests, Figure 3.19 presents the influence of thecooling speed in the coarse grain HAZ on the transition temperature to the level 28Joules of impact strength. In parallel, it includes the corresponding evolution ofhardness in the HAZ. Figure 3.19. Influence of the cooling speed on impact strength and hardness in the coarse grain HAZ; steel C = 0.18%, Mn =1.4%, Si = 0.4%; from [BER 75] Looking at the fastest cooling speeds, three successive phases will be noted. An optimal toughness in the HAZ corresponding to the end of the martensitearea. The martensites obtained in welding are frequently self-tempered laths,characterized by the presence of carbide sticks aligned according to the direction of the slats. Indeed, in steels with a low percentage of carbon, the temperature
Thermal, Metallurgical and Mechanical Phenomena 121of the end of martensitic transformation M F is so high that it allows a certaintempering of martensite even during the welding cycle. The presence of lowerbainite in these predominately martensitic HAZs is rather frequent. The toughness ofthe HAZ structures obtained from these fast cooling speeds is thus similar to that oftempered martensites and the mixed martensite-bainite structures obtained bytraditional heat treatments [HEI 75, OHM 74]. An abrupt drop in toughness is then observed when the cooling speed decreases.This is related to the evolution of lower bainite towards the higher bainite, whoseslat sizes or bainitic packages offer less cleavage resistance. For the slowest cooling speeds (ferrite-carbide structures), a stabilization oftoughness is finally observed, possibly after a slight fall in the temperature oftransition. As already seen (see section 3.2.2), this cooling speed field correspondsto ferrite extension and certain authors [OTT 80] put forward a connection betweenthe degradation of toughness and the thickness of the ferrite proeutectoïd jointsappearing at the old austenitic grain boundaries. At this stage, it should be noted that simultaneous requirements concerningtoughness and resistance to cracking can sometimes appear contradictory: indeed,the guarantee of a minimum toughness can be dependent on the limitation of the 800cooling parameter (for example: t500 < t1 crit.). On the other hand, the desire toavoid cold cracking can result in the requirement for a minimum cooling speed, inorder to avoid too strong a martensitic proportion (generally 80%), that is to say: 800 t500 > t2 crit. It can thus be seen that the simultaneous respect of these two criteriacan lead to the concept of a metallurgical weldability field between the values t1 critand t2 crit. The influence of various elements present in C-Mn and micro-alloyed steels ontoughness in the coarse grain HAZ can be schematized as follows.
122 Metallurgy and Mechanics of Welding Figure 3.20. Influence of the percentage of carbon on the transition temperature TK28J in the HAZ structure (martensite + lower bainite); from [DEV 88] Carbon decreases the toughness of the HAZs equally in the case of fast and slowcooling speeds. Figure 3.20 thus shows the unfavorable influence of carbon on thetransition temperature of impact strength for HAZs of optimal microstructure(martensite-bainite), therefore cooled relatively quickly. 800 In the case of the slowest coolings (for example, when t 500 >100 s), carbonand nitrogen (the latter having an even more marked influence) have a detrimentalinfluence on toughness [DEV 88]. Nitrogen’s detrimental effect exists both inas-welded and stress relieved states. It is also interesting to limit silicon a certain extent, an element which leads tothe formation of M-A compounds decreasing the toughness of the coarse grain HAZand the reheated HAZ in the intercritical field [TAI 95]. Within certain limits (P < 20 × 103%), phosphorus seems to have rather littleinfluence on the HAZ toughness in the case of high energy welding, but has asignificantly detrimental effect in the case of welding at low energy levels, inparticular after stress relief [GRO 86]. As has been observed previously, controlled additions of titanium slow down thegrowth of the austenitic grain. This beneficial action on toughness is also reinforcedby the fixing of part of the free nitrogen. If moreover the aim is to avoid coarsenitride precipitation in the liquid state, the titanium and nitrogen content must besuch that the product of their activity remains lower than the product of solubility in
Thermal, Metallurgical and Mechanical Phenomena 123the liquid state. Various pieces of research have shown that effective additions oftitanium must be carried out in steels with a low nitrogen content (<5 × 10-3%) andmust be themselves fairly low (Ti 10 × 10-3%) [BAK 97, DEV 88, YAO 90]. Recently developed steels, comprising complex titanium oxides, also show verygood toughness properties in the HAZ. In this case, these thermally very stableoxides can be used as sites of ferritic germination with cooling in the HAZ, even athigh temperature (1,400°C, for example), and involve the formation of a fine,disorientated acicular ferrite structure. Boron is a very effective element with which to increase hardenability and tolimit the formation of proeutectoïd ferrite or Widmanstätten ferrite. It is howeveradvisable to limit the B content to 10-15 ppm to avoid an embrittlement byprecipitation of boro-carbides or the formation of M-A compounds [RAM 86]. The gammagene property of nickel significantly lowers the transformationtemperatures in cooling and refines the grain size. From a content of 0.3 to 0.5%, itimproves toughness in the HAZ as well as in the base metal. 800 In the case of slow cooling (for example when t500 >100 s) or at the time of alater tempering, the dispersoid elements such as niobium and vanadium canreprecipitate and lead to a certain embrittlement. For a given grade of steel, it shouldhowever be noted that this possibly unfavorable influence is largely compensated bythe fact that the presence of these elements is generally associated with a significantreduction in the percentage of carbon.3.3.3. Residual stresses associated with welding The origin of residual welding stresses is related on the localization of the heatsource and the variations of the mechanical properties of materials according to thetemperature. Two sources of residual stresses can be distinguished: – residual stresses, purely thermal in origin, result from the following fact:subjected to a rise in temperature , an element of the heated central zone shoulddilate to the degree , indicating the linear dilation coefficient of thematerial. Actually, this expansion is very limited since the neighboring cold partsplay a restraining role. The element is thus subjected to a compression from them.The flow limit being very weak at high temperature, all the deformations that appearcorrespond to plastic deformations. With cooling, the situation is reversed: theheated central zone cannot retract freely, and is put under pressure by theneighboring zones. After cooling, the heated zones (molten metal and HAZ) will besubjected to residual tensile stresses, the neighboring zones being, for reasons of
124 Metallurgy and Mechanics of Weldingbalance, in compression. In the molten metal, the stresses thus created can be veryhigh, in the order of material yield strength at room temperature. Figure 3.21presents a typical example of longitudinal distribution or transverse stresses(compared to the direction of welding) within a welded joint; – residual stresses associated with allotropic transformations on cooling: in thecase of construction steels, the transformation of austenite is always accompanied bya more or less marked expansion. If this occurs at relatively low temperature(temperable materials, fast cooling, etc.), the associated deformation will no longerbe plastic, but elastic. The expansion, opposed by the neighboring zones, results inthe formation of residual compressive stresses. Superimposed on the thermal stresses, these can decrease the level of tensilestresses, and even lead to compression stresses in the HAZ [MAS 80]. Figure 3.21. Typical example of longitudinal distribution and transverse residual stresses within a welded joint, from [MAC 77] The residual stresses resulting from welding are superimposed on the in-servicestresses, and for this reason play a role in various phenomena or properties: coldcracking, fatigue strength, rupture, stress corrosion, etc.
Thermal, Metallurgical and Mechanical Phenomena 1253.3.4. Influence of residual stress relieving heat treatments in the HAZ In certain cases, the residual stresses of welding can seriously reduce the serviceperformance of assemblies, and it is necessary to lower their level by stress relievingtreatment. The principle aspect of this operation consists of transforming the residualelastic stresses into plastic deformations. In general, this is carried out by a post-welding heat treatment at a temperature such that the elastic limit of material issufficiently reduced to obtain this transformation. This type of treatment thuscomprises: – a slow heating to a temperature where relief is sufficiently significant; – a maintenance at this temperature (for example: to around 530 to 630°C forC-Mn and micro-alloyed steels and, 670 to 710°C for Cr-Mo steels, etc.); – a sufficiently slow cooling so as not to introduce new residual stresses. We will restrict ourselves here to pointing out some general metallurgicalconsequences of this type of treatment, by recalling that the precise choice ofconditions depends on many factors (type of material, thickness, and of course anyregulations in place [BER 78]). In general, the tempering associated with the relief treatment has a beneficialeffect on quenched microstructures, although this is less favorable when the initialstructures in the HAZ are ferrite-carbide. A favorable effect caused by therestoration of possible strain hardened-aged zones during welding, or after coldworking should also be noted. As has been seen, the precipitation of micro-alloying elements (Nb, V) isgenerally incomplete during coolings in the HAZ. The complementary precipitationwhich can occur during the stress relieving heat treatment will generally have adetrimental influence on toughness. Thus, the metallurgical effect of the treatmentwill often result from a conflict between a mechanism of matrix softening(favorable) and a more or less significant precipitation (unfavorable). The tempering treatment can sometimes have a post-heating role, allowing thediffusion of hydrogen out of the welded joints, lowering the levels of hardness, andthus reducing the risk of cold cracking (see section 3.2.4). In the case of low alloyed steels, the additions of Mn, Cr, Ni can lead to a certaindeterioration of tenacity for a stress relief treatment followed by a slow cooling,contrary to the additions of Mo [BLO 80]. This phenomenon is more accentuated thecoarser the grain involved and the greater the temper. To avoid the problems ofreversible temper brittleness [BLO 88], it is important to limit the impurity content,
126 Metallurgy and Mechanics of Weldingwhich can be achieved by, for example, using the Bruscato parameter: X = (10P +4Sn + 5Sb + As)/100, lower than a value of 10 for demanding specifications [BER 97]. In certain cases (low alloy steels, alloys containing nickel, etc.), it is observedthat stress relief heat treatments lead to an intergranular cracking in the HAZ, knownas reheat cracking [DHO 87, DHO 92]. This phenomenon occurs in the presence of significant residual stresses,accentuated particularly by localized stresses caused by the geometry, in coarsegrain zones weakened by intergranular precipitations (AlN, Mo, Nb, V carbides) andsegregated impurities (S, P, As, Sn, Sb, etc.) within these same joints. Theappearance of such cracks is generally interpreted from a precipitation hardening ofthe grain interior during the post-welding treatment, which limits all stress relief orplastic deformation within the grains, by concentrating them on the less resistantgrain boundaries. The prevention of reheat cracking thus involves the adoption ofless sensitive materials, but also by use of suitable welding conditions: lowresistance molten metal, buttering, increased contribution of heat and/or pre-heating,use of the temper bead method, i.e. narrow passes to achieve a refinement of thepreceding ones, etc.3.4. Bibliography[AND 65] ANDREWS K.W., “Empirical formulae for the calculation of transformation temperature”, Journal of the Iron and Steel Institute, no. 7, July 1965.[ATS 80] ATS/OTUA, “Conseils pour le soudage des aciers de construction métallique et chaudronnée à limite d’élasticité garantie 420 N/mm²”, Cahiers de l’ATS/OTUA, 1980.[BAK 97] BAKER T.N., Titanium Technology in Microalloyed Steels, Institute of Materials Publications, 1997.[BER 72] BERNARD G., PRUDHOMME M., “Compléments à l’étude des phénomènes thermiques dans les joints soudés”, Revue de Métallurgie, July-August 1972.[BER 75] BERNARD G., “A view-point on the weldability of C-Mn and microalloyed structural steels”, Microalloying Symposium 75, Washington, October 1975.[BER 78] BERNARD G., Opportunité des traitements thermiques de relaxation dans les constructions soudées, Doc. IIS/IIW no. X.913-78, 1978.[BER 97] BERANGER G., HENRY G., LABBE G., SOULIGNAC P., Les aciers spéciaux, Lavoisier, 1997.[BHA 92] BHADESHIA H.K.D.H., Bainite in Steels, Institute of Materials, 1992.[BLO 80] BLONDEAU R., “Les aciers faiblement alliés soudables, influences des éléments d’addition”, Soudage et Techniques Connexes, January-February 1980.
Thermal, Metallurgical and Mechanical Phenomena 127[BLO 88] BLONDEAU R., “La fragilité de revenu réversible, facteurs et remèdes”, Traitement thermique, 220, 1988.[CHA 74] CHANDEL R.S., GARBER S., “Mechanical and metallurgical aspects of spot-welded joints in heat-treated low-carbon mild steel sheet”, Metals Technology, September 1974.[CHR 65] CHRISTENSEN N., DAVIES V. DE L., GJERMUNDSEN K., “Distribution of temperatures in arc welding”, British Welding Journal, February 1965.[CLY 58] CLYDE M., ADAMS C.M., “Cooling rates and peak temperatures in fusion welding”, Welding Research Supplement, May 1958.[CON 87] CONNOR L.P., Welding Handbook, volume 1, American Welding Society, 1987.[CON 92] CONSTANT A., HENRY G., CHARBONNIER J.C., Principes de base des traitements thermomécaniques et thermochimiques des aciers, PYC Edition, 1992.[DEA 40] DEARDEN J., ONEILL, “A guide to the selection and welding of low alloy structural steels”, Trans. Int. Welding, 1940.[DEB 82] DEBROY T., SZEKELY J., EAGAR T.W., “Temperatures profiles, the size of the Heat- Affected Zone and dilution in electroslag welding”, Materials Science and Engineering, no. 56, 1982.[DEF 75] DEFOURNY J., BRAGARD A., “Caractérisation des cycles de température en soudage bout à bout à l’arc submergé de tôles d’aciers au moyen de deux grandeurs du champ thermique”, Revue Belge de la Soudure, no. 3, Lastijdschrift, 1975.[DEV 83] DEVILLERS L., KAPLAN D., MOUSSY F., Soudabilité des aciers trempés et revenus obtenus par trempe directe, Final research report, CECA no. 7210 KA/308, 1983.[DEV 84] DEVILLERS L., KAPLAN D., MOUSSY F., Prévision et comportement de la zone adoucie des aciers trempés-revenus, IRSID Report no. RE 1137, September 1984.[DEV 85] DEVILLERS L., KAPLAN D., Propriétés d’emploi d’assemblages obtenus par faisceau d’électrons des tôles de forte épaisseur en acier de construction, Final research report CECA no. 7210 KA/310, IRSID Report RE 1252, December 1985.[DEV 86a] DEVILLERS L., KAPLAN D., MAAS E., “Aspects mécaniques de l’évaluation de la ténacité d’éprouvettes métallurgiquement hétérogènes”, Revue de Métallurgie, CIT, April 1986.[DEV 86b] DEVILLERS L., KAPLAN D., Interpretation of deviated fracture of electron beam steel welds in notch bending tests, IRSID Report no. RE 1319, 1986.[DEV 87] DEVILLERS L., KAPLAN D., JANSEN J.P., “Simulation thermique des zones affectées par la chaleur en soudage multipasse des aciers de construction”, Soudage et Techniques connexes, March-April 1987.[DEV 88] DEVILLERS L., KAPLAN D., JANSEN J.P., “Aspects thermiques et métallurgiques de la ténacité des ZAC”, Revue de Métallurgie, CIT, March 1988.[DEV 89] DEVILLERS L., KAPLAN D., Aspects métallurgiques de l’assemblage des tôles de faible épaisseur par LASER CO2, Final research report CECA no. 7210 KA/314, IRSID Report RCA 89333, October 1989.
128 Metallurgy and Mechanics of Welding[DEV 91] DEVILLERS L., KAPLAN D., TESTARD P., An approach for predicting microstrucrures and toughness properties in HAZ of multipass welds, IRSID Report 91316, March 1991.[DHO 87] DHOOGE A., VINCKIER A., “Reheat cracking – a review of recent studies”, Int. J. Pres. Ves. and Piping, 27, 1987.[DHO 92] DHOOGE A., VINCKIER A., “La fissuration au réchauffage- revue des études récentes (1984-1990)”, Le Soudage dans le Monde, vol. 30, no. 3-4, 1992.[EAS 83] EASTERLING K., Introduction to the Physical Metallurgy of Welding, Butterworths, 1983.[GOL 76] GOLDAK J., BIBBY M., “The toughness of EB welds in HSLA steels”, Welding of HSLA Structural Steels Conference, Rome, ASME Publications, 1976.[GRA 95] GRANJON H., Bases métallurgiques du soudage, Publications du soudage et ses applications, 2nd edition, 1995.[GRO 86] GRONG O., AKSELSEN O.M., “HAZ toughness of microalloyed steels for offshore”, Metal Construction, September 1986.[GRO 94] GRONG O., Metallurgical Modelling of Welding, Institute of Materials, 1994.[GRU 81] GRUMBACH M., Les essais de dureté, Collection IRSID-OTUA, 1981.[HAL 84] HALE G.E., NUTTING J., “Overheating of low-alloy steels”, International Metals Review, vol. 29, no. 4, 1984.[HEH 72] HEHEMANN R.F., KINSMAN K.R., AARONSON H.I., “A debate on the bainite reaction”, Metallurgical Transactions, vol. 3, May 1972.[HEI 75] HEISER F.A., DE FRIES R.S., “Temper embrittlement in steel for thick wall gun tubes”, Journal of Metals, January 1975.[HON 95] HONEYCOMBE R.W.K., BHADESHIA H.K.D.H., Steels, Microstructure and Properties, Edward Arnold, 1995.[HRI 95] HRIVNAK I., “Weldability of modern steel materials”, ISIJ International, vol. 35, 1995.[IKA 80] IKAWA H., OSHIGE H., TANOUE T., Effect of M-A constituent on HAZ toughness on a high strength steel, Document IIS-IIW, no. IX-1156-80, 1980.[IKE 95] IKEUCHI K., LIAO J., TANABE H., MATSUDA F., “Effect of temper-bead thermal cycle on toughness of weld ICCGHAZ of low alloy steel SQV-2A”, ISIJ International, vol. 35, 1995.[INO 98] INOUE K., ISIJ International, vol. 38, no. 9, 1998.[ION 97] ION J.C., “Modelling of LASER welding of Carbon-Manganese steels”, in H.C. Cerjak (ed.), Mathematical Modelling of Weld Phenomena 3, Institute of Materials, 1997.[IRS 77] IRSID, “Courbes dureté-paramètre de refroidissement en conditions de soudage”, collection established at the IRSID, 1977.
Thermal, Metallurgical and Mechanical Phenomena 129[ITO 00] ITO R., SHIGA C., KAWAGUCHI Y., HAYASHI T., SHINOHARA H., TORIZUKA S., Microstructural analysis of softening region on weld HAZ of ultra-fine grained steels, Document Institut International de la Soudure no. IX-1968-00, 2000.[KAN 76] KANAZAWA S., “Improvement of weld fusion zone toughness by fine TiN”, Transactions ISIJ, vol. 16, 1976.[KAP 98] KAPLAN D., STUREL T., “Couplage d’un modèle métallurgique de soudage et de critères locaux de rupture pour prévoir la ténacité des joints soudés multipasses”, 9èmes Journées AFIAP, Paris, October 1998.[KAW nd] KAWABATA F., AMANO K., TOYODA M., MINAMI F., Tempering effect by succeeding weld passes on multi-layered HAZ toughness, doc. Kawasaki Steel, no date.[KOS 81] KOSO M., MIURA M., OHMORI Y., “Microstructure and toughness of weld HAZ in 785 MNm-2 steel”, Metals Technology, December 1981.[KOU 86] KOU S., WANG Y.H., “Computer simulation of convection in moving arc weld pools”, Met. Trans. A, vol. 17A, December 1986.[LAM 99] LAMBERT A., DRILLET J., GOURGUES A.F., STUREL T., PINEAU A., Microstructure of M-A constituent in HAZs of HSLA steel welds in relation with toughness properties, IRSID report, no. 99 21, 1999.[LIN 89] LIN Y., ABKEN M.G., BOWKER J.T., “Mechanical and microstructural analysis of multi-pass welded HAZ”, Proceedings of Recent Trends in Welding Science and Technology, ASM International, Gatlinburg, 1989.[LON 94] LONGAYGUE X., KAPLAN D., MAURICKX T., “Etude paramétrique de l’influence des facteurs d’hétérogénéité mécanique sur le comportement en service des assemblages soudés”, Revue de Métallurgie, CIT, June 1994.[MAK 77] MACHERAUCH E., WOHLFAHRT H., “Different sources of residual stress as a result of welding”, in Residual Stresses in Welded Construction and their Effects, The Welding Institute Publications, London, 1977.[MAR 80] MARQUET F., DEFOURNY J., MARIQUE C., MATHY H., BRAGARD A., Recherches sur les connaissances de base en vue d’améliorer le soudage des aciers sous haut apport calorifique, Rapport final de recherche CECA no. 7210 LA/303, 1980.[MAS 80] MASUBUCHI K., Analysis of Welded Structures, Pergamon Press, 1980.[MAT 94] MATSUDA F., FUKADA Y., OKADA H., SHIGA C., IKEUCHI K., HORII Y., SHIWAKU T., SUZUKI S., Review of Mechanical and Metallurgical Investigations of M-A constituent in Japan, Doc. IIS-IIW no. IX-1782-94, 1994.[MIE 92] MIETTINEN J., “Mathematical simulation of interdendritic solidification of low- alloyed and stainless steels”, Acta Polytechnica Scandinavica, Chemical Technology and Metallurgy Series, no. 207, 1992.[MUR 67] MURRY G., PRUDHOMME M., CONSTANT A., “Etude des transformations dans la zone thermiquement affectée lors du soudage et son intérêt pour l’estimation de la dureté sous cordon”, Revue de Métallurgie, 64, no. 6, June 1967.
130 Metallurgy and Mechanics of Welding[NIL 75] NILES R.W., JACKSON C.E., “Weld thermal efficiency of the GTAW process”, Welding Journal, Welding Research Supplement, January 1975.[OHM 74] OHMORI Y., OHTANI H., KUNITAKE T., “Tempering of the bainite/martensite duplex structure in a low-carbon low-alloy steel”, Met. Sci., vol. 8, 1974.[OKA 92] OKAGUCHI S., ISIJ International, vol. 32, no. 3, 1992.[OLE 81] OLETTE M., GATELLIER C., “Action d’une addition de calcium, de magnésium ou des éléments des terres rares sur la propreté inclusionnaire des aciers”, Revue de Métallurgie, CIT, December 1981.[OTT 80] OTTERBERG R., SANDSTRÖM R., SANDBERG A., “Influence of Widmanstätten ferrite on mechanical properties of microalloyed steels”, Metals Technology, October 1980.[POR 34] PORTEVIN A., SEFERIAN D., XIe Congrès de l’Acétylène et de la Soudure Autogène, Rome, vol.3, 1934.[RAM 86] RAMBERG M., AKSELSEN O.M., GRONG O., “Embrittlement phenomena in the intercritical HAZ of boron-containing steels”, Advances in Welding Science and Technology, Publications de l’ASM, Gatlinburg, 1986.[REE 94] REED R.C., BHADESHIA H.K.D.H., “A simple model for multipass steel welds”, Acta Metall. Mater., vol. 42, no. 11, 1994.[RIS 74] RIST A., ANCEY-MORET M.F., GATTELLIER C., RIBOUD P.V., “Equilibres thermodynamiques dans l’élaboration de la fonte et de l’acier”, Techniques de l’Ingénieur, M 1733, 1974.[ROS 46] ROSENTHAL D., “The theory of moving sources of heat and its applications to metals treatments”, Transactions ASME, vol. 68, 849, 1946.[RYK 61] RYKALINE N.N., “Calcul des processus thermiques de soudage”, Soudage et techniques connexes, no. 1-2, 1961.[TAI 95] TAILLARD R., VERRIER P., MAURICKX T., FOCT J., “Effect of silicon on CGHAZ toughness and microstructure of microalloyed steels”, Met. Trans. A, vol. 26, February 1995.[TAK 95] TAKAHASHI A., OGAWA H., “Influence of softened heat-affected zone on stress oriented hydrogen induced cracking of a high strength line pipe steel”, ISIJ International, vol. 35, 1995.[TOY 86] TOYODA M., Fracture toughness evaluation of steel welds (Review), Osaka University Document, July 1986.[TOY 92] TOYODA M. (ed.), Proceedings of the Workshop Mismatching and its Control, Osaka University, Tokyo, July 1992.[WEI 95] WEISS D., SCHMIDT J., FRANZ U., “A model of temperature distribution and weld pool deformation during arc welding”, Mathematical Modelling of Weld Phenomena 2, Institute of Materials, 1995.[YAO 90] YAO S., KOÇAK M., Influence of titanium on HAZ microstucture and toughness of offshore steel welds: literature review – part 1, Report GKSS, no. 90/E/39, 1990.
Thermal, Metallurgical and Mechanical Phenomena 131[YUR 87] YURIOKA N., OKUMURA M., KASUYA T., COTTON H.J.U., “Prediction of HAZ hardness of transformable steels”, Metal Construction, April 1987.[ZAC 93] ZACHARIA T., DAVID S.A., “Heat and fluid flow in welding”, Mathematical Modelling of Weld Phenomena, Institute of Materials, 1993.[ZEN 48] ZENER C., Transactions ASME, no. 45, 1948.
Chapter 4 Molten Metal4.1. Metallurgical reminders Broadly speaking, the mechanical characteristics of a steel result from itsstructure and its chemical composition. For a given structure, the chemicalcomposition influences the mechanical properties due to the effect of the elements insolid solution. Figure 4.1. Increase in the tensile strength of iron due to the effect of various elements in solid solution; from [GAR 75] Figure 4.1 shows that this effect is modest since an atomic addition of 1% ofchromium or molybdenum modify the fracture strength of the ferrite by only 6 or70 Mpa respectively.Chapter written by Christian BONNET.
134 Metallurgy and Mechanics of Welding As for the structure of steel, it depends on the heat treatment but also on thechemical composition which determines its hardenability. Thus, two steels ofdifferent chemical composition will not lead to the same structure for the same heattreatment and will thus have different mechanical properties. Figure 4.2. Continuous cooling transformation (CCT) diagrams; from [COL 74]
Molten Metal 135 The CCT diagrams of steels XC48 and 50CD4 show very clearly that thestructural influence is infinitely higher than the effect of the solid solution ofalloying elements. Indeed, the two steels with similar carbon percentage havesimilar hardnesses when they are in the same structural state (hardness: 210/220 Hvin the ferrite + pearlite state; 60/62 HRc in a martensitic state) but have extremelydifferent characteristics when they are subjected to the same heat treatment. Thus,for the cooling speed highlighted in Figure 4.2, steel 50CD4 has a primarilymartensitic structure which confers a hardness of 60 HRc, while steel XC48 has aferrite + pearlite structure whose hardness is only 23 HRc. These metallurgical principles are very broad and thus also apply to the weldingmetallurgy. Thus, we will have to examine any welding operation from a thermal aswell as a chemical point of view.4.2. Molten metal4.2.1. Thermal aspect The thermal aspect has already been covered in Chapter 3. The approach usedthen applies to any point in the molten metal and it is thus possible to determine withthe cooling conditions of each pass of an assembly with sufficient precision,provided that the welding energy, the type of joint, the process, the thickness/esconcerned, the pre-heating temperature and/or the inter-pass temperature are known. Figure 4.3. Bypass submerged arc weld The effect of variations in the operating conditions on the thermal cycle isgenerally underestimated by the majority of the welders. By means of the IRSIDgraph for example (see Figure 3.8), it can be seen that minor modifications of theelectric parameters or temperature between passes can significantly modify thethermal welding cycle and, consequently, the mechanical properties of the weldedjoint (see Table 4.1). Such variations can be employed by a welder to improve wetting or to save timeduring the execution of a small-size homologation sample which will lead to a much
136 Metallurgy and Mechanics of Weldinghigher temperature between passes than will be the case in real constructionconditions. Influence of welding energy 1st pass Example 1 Variati Example 2 onWelding parameters 600 A; 28 V; 50 cm/min 660 A; 30 V; 40 cm/minWelding energy 20.16 kJ/cm 47.3% 29.7 kJ/cm t 800/500 11 s 263% 40 s Influence of temperature between passes 2nd pass Example 3 Variati Example 4 onWelding parameters 600 A; 28 V; 50 cm/min 600 A; 28 V; 50 cm/minTemperature 20°C 130°C 150°CWelding energy 20.16 kJ/cm - 20.16 kJ/cm t 800/500 11 s 82% 20 s Table 4.1. Evaluation of the thermal cycle based on the IRSID graph; from [COL 77]4.2.2. Chemical aspectConstitution of the molten metal The chemical composition of molten metal results from the metal mixture addedby the welding product and the base metal. The proportion of base metal in a weldbead is characterized by the dilution ratio (see Figure 4.4). Surface (B) Dilution ratio = Surface (A + B) A B Figure 4.4. Influence of the base metal on the composition of the molten metal
Molten Metal 137 According to the process, the type of joint and the welding procedure, theproportion of base metal is more or less important and in the case of a multipassjoint, it varies from one pass to another. However, the products of welding arebalanced chemically so that their deposits “outside dilution” acquire the necessarymechanical properties under the cooling conditions corresponding to the mosttraditional thermal welding cycles. It should be understood that each time a weldingmaterial undergoes cooling transformation phases, the analysis of the metal addedby the welding product which makes it possible to obtain the same mechanicalproperties is different from that of the base metal, because the cooling conditionsduring the manufacture of the latter are very different from those which areassociated with welding. Thus, by dilution effect, the molten metal has anintermediate analysis between that of the added metal and that of the base metal andthis analysis can vary from one pass to another in multipass welding. This is why themajority of the operating mode procedures require a check on the properties atvarious levels in the welded joint and, in particular, in the root zone where thedilution ration is the highest and consequently where the lowest impact strengthvalues will often be found. In spite of these qualifications, the manufacturers are notspared unpleasant surprises while checking the properties of the assemblies duringproduction if they have recourse to materials of various sources. This results fromthe fact that the qualification of the operating procedure takes the standardizeddesignation of the base metal into account and that in the majority of cases, this isbased on the product’s mechanical properties. Thus, according to the differentmanufacturing techniques available to them, the various steelmakers will usesignificantly variable analyzes to comply to the same standardized designation as theanalyzes of three steels used indifferently by the same manufacturer show (see Table4.2). If they are welded with the same filler product, these steels, althoughconforming to the required standard, will lead to very different analyses andmechanical properties of the molten metal in the zones where there is a high dilutionrate. % C Si Mn P S Cu NiNF EN 10028: 0.08 0.9P295GH 0.20 <0.4 1.5 <0.030 <0.025 <0.30 <0.30Steel 1 0.20 0.23 1.02 0.014 0.008 - -Steel 2 0.13 0.28 0.99 0.013 0.010 0.29 -Steel 3 0.12 0.40 1.34 0.018 0.008 0.24 0.12 Table 4.2. Examples of analytical variations in steels complying to the same standardized designation
138 Metallurgy and Mechanics of WeldingAnalytical characteristics of the deposited metal The deposited metal comes from the fusion of the filler product in theatmosphere of the arc. The welding processes with a refractory electrode (TIG,plasma) generally takes place in an inert atmosphere to avoid rapid deterioration ofthe tungsten electrode. When these processes are employed, the analysis of thedeposited metal is then very close to that of the filler; it differs only in thevolatilization of various elements present, which are a function of their respectivevapor tensions. Thus, a slight reduction will be noted in the manganese content inthe deposited metal compared to the filler. On the other hand, for all the other processes the arc atmosphere is deliberatelymore or less oxidizing because a light oxidation of the base metal’s surface aidselectron emission and, thus the stability of the arc. This being the case, oxido-reduction reactions occur, mainly in the metal drops which transfer in the arc, so thatthe analysis of the deposited metal deviates notably from that of the filler. It is easyto take these chemical exchanges into account at the time the welding product isformulated, so as to adjust the alloying elements to obtain the content desired in theadded metal but one will never be able, with these processes, to lower the oxygencontent of the deposited metal to the level of that of the base metal (see Table 4.3).Oxygen being practically insoluble in the majority of metals, it will be found in theform of inclusions finely dispersed in the weld. In the case of steels, we will see laterthat under certain conditions these inclusions can play a key role at the time of theaustenite transformation of the molten metal. Molten metal Steel TIG/Plasma MAG SMAW/ SAW Solid wire Filled wire O ppm 15-40 20-60 250-550 300-1,100 280-1,100 Table 4.3. Ranges of oxygen content variations in steel welds according to the processes and the types of welding products In welding with a coated electrode (SMAW), there is another element whosecontent in the molten metal cannot be kept as low as we could wish: nitrogen.Indeed, although coatings of the coated electrodes always contain componentswhich break up during fusion and generate at the level of arc gases in order toprotect the metal droplets from the ambient air, the protection thus obtained is neverperfect and we cannot avoid a certain amount of contamination. Because the processis manual, it is clear that the extent of this contamination depends on dexterity on thewelder but, whatever it is, it is very difficult to have less than 100 ppm of nitrogen inthe deposited metal, particularly in all-positional welding.
Molten Metal 1394.2.3. Microstructures in ferritic steel welds: relationship with impact strengthcharacteristics As in the HAZ, the mechanical properties of the molten metal depend on itsstructure and its chemical composition. If it is easy to define a chemical analysis of the molten metal so as to make itcompatible with the tensile properties of the base metal, it is not so simple from theperspective of toughness. Consequently, we will limit our comments here to theissue of impact strength, because this simple and inexpensive test is systematicallyemployed in welding. In a multipass joint, two types of zone can always be distinguished (see Figure4.5): the first has preserved an as-solidified structure while the second has been“reaustentitized” during the execution of successive passes. The microstructuralcomponents of these various zones are in general very different. Except in the caseof a strongly alloyed weld, the reaustenitized areas have a ferritic structure with asmall proportion of pearlite because the percentage of carbon in welding products isalways very low. The toughness of this ferritic structure with equiaxial grains depends, as alwaysin metallurgy, on the fineness of the grains. It is thus a function of the thermalwelding cycle, which dictates the time spent in the austenitic state and the coolingspeed and so the transformation temperature of the austenite. It also depends on thepresence of elements such as titanium, niobium, vanadium, aluminum or boron,which limit grain enlargement at the reaustenitization phase. At all events, thisreheated structure is generally not at the origin of problems of impact strength inwelded joints. On the other hand, the as-solidified zones can have very different structures fromone joint to another and, therefore, considerable variations in terms of their impactstrength characteristics, as illustrated in Figure 4.6. The proportion of the as-solidified and reheated zones depends on the processand the welding conditions. In the case of TIG multipass welds or when using smalldiameter coated electrodes, a narrow bead width effectively ensures that the wholeof the molten metal has a reheated structure. On the other hand, in submerged arcwelds, the as-solidified zones never represent less than 50% of the molten metal andcan even reach 90% in the case of double sided bypass welds.
140 Metallurgy and Mechanics of Welding b a c Figure 4.5. Submerged arc welding: a) macrographic aspect; b) microstructure of the as-solidified zones; c) microstructure of the reheated zones The proportion but especially the position of these two types of structure at thenotch bottom of the impact test specimens will affect the result. Indeed, the fractureenergy measured during this test is the sum of energy necessary to initiate a crack atthe notch bottom and the energy necessary for it to progress and lead to the creationof two surfaces. The crack will be initiated under the pendulum impact as soon asthe critical initiation stress which is specific to each microstructure is reached in oneor other of them. Thus, the stress which develops at the notch bottom under thependulum impact decreases from its center towards the sides. This is why, in aperfectly homogenous material, the rupture is always initiated in the notch center,while in a heterogenous material, initiation could be offset laterally if themicrostructure located at the notch center has a critical cracking stress higher thanthat of an adjacent structure. Thus, when the most fragile structure is offsetcompared to the notch center, the initiation component of the rupture energymeasured during the impact test is much higher than when this same structure islocated at the center. As for the propagation energy, it can be readily conceived thatit is a function of each microstructures’ size and their intrinsic characteristics.
Molten Metal 141 A % x 1000 B 64 C 67 1510 Mn 1500 370 Si 370 17 S 16 18 P 18 52 Ni 53 65 Cr 67 4 Mo 4 71 Cu 75 4 Ti 8 12 Al 10 1 Nb 1 9 V 11 72 O 75 17 N 17 Nb Figure 4.6. Influence of microstructure on impact strength The principal microconstituents likely to exist in the as-solidified zones arerepresented in Figure 4.7. In the IIS/IIW-999-88 document, the International Institute of Welding proposesa finer analysis and distinguishes more constituents, however, this is not theimportant point. Indeed, all metallurgists know that toughness is improved byrefining the structure.
142 Metallurgy and Mechanics of Welding Under these conditions, it is clear, looking at the micrographies in Figure 4.7,that the as-solidified zones which lead to the best impact strength characteristics willbe primarily made of acicular ferrite. This microconstituent, which never appears in steels, exists in the molten metalonly in the presence of certain inclusions which allow the intragranular germinationof the ferrite at the time of the transformation of austenite [ABS 78, COC 78]. It isknown that the existence of these inclusions depends on the oxygen content of thedeposited metal but, so that there is intragranular ferrite germination, it seemsnecessary that these complex inclusions, which result from oxido-reductionreactions in fused metal and which are trapped during solidification, have locally ontheir surface Ti oxide TiO [STL 93] or a MnTi oxide, MnTi2O4 [BLA 99]. It shouldbe understood then that titanium plays a fundamental role [CHA 83, EVA 97] andbesides it is its variation (0.004 to 0.008%) which explains the difference betweenthe structures and the impact strength values of the welds A and B in Figure 4.6.However, it is not enough to have a minimum of titanium so that it is found in oneor other of the desired forms on the inclusion surface. What is more, it is necessarythat the reaction kinetics which lead to the formation of inclusions allow this result.Thus, in addition to the oxygen content, the nature and the quantity of all of thedeoxidizing elements present in the molten metal will play a part, whether theycome from the wire or the base metal [BUR 88, DEV 83].Figure 4.7. Principal microconstituents of the solidified molten metal in its as-solidified state
Molten Metal 143 The complexity of these phenomena means that even today it is impossible topredict the presence of the germs necessary to the formation of acicular ferrite with asimple reading of a chemical molten metal analysis. Only a metallographicalexamination enables us to definitely determine the presence of this component. These particular inclusions are necessary to achieve a structure rich in acicularferrite and as a result a good toughness in all the welding zones (including the as-solidified zones). However, this condition is not sufficient because the proportion ofacicular ferrite depends on the thermal welding cycle and the chemical compositionof the molten metal which determines its hardenability.Influence of cooling speed In metallurgy, CCT diagrams make it possible to obtain a precise idea of thestructure and hardness of a steel according to the cooling speed after austenitization.These diagrams are specific to each steel and each austenitization condition(austenitic grain size). In welding, such diagrams do not exist and will undoubtedly never exist becausethe variations in cooling speed in the field of austenite transformation ( 800/500or 700/300) are always accompanied by a variation in the conditions ofaustenitization, but there is no correlation between these two factors: the increase inthe welding energy, the pre-heating temperature, thickness of the parts to beassembled or the implementation of different welding processes do not have similarconsequences on the upper (austenitic field) and lower parts (field of transformation)of the thermal cycle [BON 80]. In any event, if the necessary inclusions are present, it has been clearly shown[ANT 81] that an increase in the cooling speed leads, initially at least, to an increasein the proportion of acicular ferrite and is accompanied by an improvement intoughness (see Figure 4.8). Secondly, additional hardened structures (lower bainiteand/or martensite) can be found if the hardenability of the molten metal is high.Influence of alloying elements The addition of alloying elements to a steel increases its hardenability bydelaying transformations which proceed by germination and growth, and loweringthe temperature at which martensitic transformation (Ms) begins. If the CCTdiagram is considered, the principal effect of this additions is to shift the curves ofthe diagram towards the right.
144 Metallurgy and Mechanics of Welding Figure 4.8. Influence of the thermal cycle on the structure and the temperature transition – analysis of the molten metal: 0.066% C; 0.94% Mn; 0.62% Si; from [BON 80]
Molten Metal 145 It is much the same for molten metal, except that the slowing of transformationsby the addition of alloying elements seems to favor the “traditional” transformationsmore than acicular ferrite formation. That is easily explained when we consider that,for a field in which austenite is transformed into acicular ferrite to exist, specificinclusions must be present which play the part of pre-existing germs. Then, theaddition of alloying elements can have an effect on the germination speed ofacicular ferrite but only on its growth. Thus, at a constant cooling speed, the addition of alloying elements causes anevolution in the microstructure similar to that which the increase in cooling speedcauses at a constant chemical composition: initially at least, the proportion ofacicular ferrite increases because the transformations which preceded its formationare considerably slowed down; then, the acicular ferrite grains are refined then,finally, these are gradually replaced by an increasing proportion of martensite and/orlower bainite. Figure 4.9. Influence of alloying elements and cooling rate on the transition temperature of the molten metal However, from the perspective of mechanical properties, the increase in thecooling speed and the addition of alloying elements are not completely equivalent.Indeed, in the same microstructure, the presence of a greater quantity of alloyingelements causes, through a solid solution effect, an increase in rupture strength,yield strength and hardness but also a reduction in impact strength values.
146 Metallurgy and Mechanics of Welding It is then possible to summarize the effect of the cooling speed and chemicalcomposition on the impact strength characteristics in the following way (see Figure 4.9): – when the content of an alloying element is low (low hardenability), we obtain avery coarse as-solidified structure primarily made up of proeutectoid ferrite and alamellar component. Toughness is then badly effected whatever the cooling speed(high transition temperature); – when the alloying content (Mn, Mo, etc.) is increased and if favorableinclusions are present, the acicular ferrite proportion increases, its grains becomeincreasingly fine and toughness improves considerably; – if the content of alloying elements is increased further beyond T1 for ( t 8/5)1or T2 for ( t 8/5)2, a deterioration in the values of impact strength is observedbecause the negative effect of hardening through the solid solution effect related tothe increase in the alloying elements becomes higher than the positive effectresulting from the increase in the quantity and fineness of the acicular ferrite; – comparison of the two curves in Figure 4.9 shows conclusively that an increasein the cooling rate ( t 8/5)1 compared to ( t 8/5)2 always improves the impactstrength. In the absence of inclusions essential to the formation of acicular ferrite, granularbainite is first seen to appear then lower bainite. These structural variations are alsoaccompanied by a certain improvement in impact strength values but they remainsignificantly lower than those obtained in the presence of acicular ferrite.Influence of oxygen content In ferritic steel welds, a minimum oxygen content is necessary so that thetransformation of austenite into acicular ferrite can exist. This minimum contentdepends on the other deoxidizers present and increases particularly with thealuminum content. It is about 250 ppm when the aluminum content is lower than0.015%; it can reach 350 to 400 ppm for an aluminum content of about 0.035 to0.040%. It is because this minimum is not reached that poor impact strengths are obtainedat low temperature in ferritic steel welding carried out by means of high energydensity processes such as plasma, electron beam and laser. The oxygen content also gives a certain indication of the inclusion rate and thisrate has a direct incidence on the ductile rupture energy: all things being equalotherwise, an increase in the inclusion rate generates a reduction in the ductilerupture energy (see Figure 4.10).
Molten Metal 147 There thus exists an optimum oxygen parameter for ferritic steel welds when therequired tensile characteristics are accessible to an acicular ferrite structure (<650 or700 MPa) because the best tensile/toughness compromise will be obtained. Beyondthis, structures of lower bainite or martensite will have to be resorted to and amaximum reduction in oxygen content sought so as to minimize the inclusion rate.Obviously this is also the case for austenitic stainless steel welds or, more generally,of face centered cubic materials which do not present a ductile/brittle transition. Figure 4.10. Influence of oxygen content on the Charpy-V transition curveInfluence of nitrogen, niobium and vanadium In ferritic steels, nitrogen can be associated with three metallurgical phenomena: – solid solution effect: the nitrogen atoms in an interstitial position in the cubiccentered iron lattice generate large distortions of the crystal lattice that cause anincrease in the tensile and hardness characteristics, associated with a reduction intoughness. It is to these free nitrogen atoms that the most harmful effect is generallyattributed; – precipitation hardening: this hardening results from a coherent precipitation ofnitrides or carbo-nitrides of elements with a strong affinity for nitrogen (in particularniobium and vanadium). This precipitation primarily occurs in the temperature range400-650°C; – ageing: this stems from the diffusion of nitrogen atoms in the interstitial solidsolution towards the crystalline defects that strongly limits the possibilities ofdislocation displacements. An increase in the elasticity limit is then observed, while impact strength drops.This phenomenon really appears only at low temperatures (ambient/250°C). In the welding of these steels, the increase in nitrogen content is observed tohave a negative effect on impact strength in all the zones of multipass weldings, thatis to say not only in the last pass, which has an as-solidified structure rich in acicularferrite, but also in the reaustenitized zones which have an equiaxed ferritic structure
148 Metallurgy and Mechanics of Weldingwith fine grains and the zones with an as-solidified structure but reheated to a valuelower than Ac1 during the execution of subsequent passes [BON 86]. In these lastzones, the increase in transition temperature with the nitrogen content is moremarked when the welding contains a small quantity of niobium and, more still whenit contains vanadium. Niobium and vanadium are very seldom added voluntarily in welding productsbut they are necessary for TMCP (Thermal-Mechanical Controlled Processing) steelmanufacturing, and are also found in certain quenched-tempered steels. Via adilution effect, some will be found in molten metal and particularly in the rootpasses, where they will cause a reduction in impact strength values, which areincreasingly significant the higher the nitrogen content. This embrittlement will beeven more marked if the assembly has to undergo a post-welding relief treatment,because it will allow niobium carbo-nitrides and vanadium nitrides to precipitatemore completely.The titanium/boron effect This effect results from the presence of a very small quantity of boron (typically20 to 60 ppm) that considerably delays the appearance of proeutectoid ferrite in theaustenitic grain boundaries during the cooling of the weld bead. Thus, the austenitetransformation can occur primarily by intragranular acicular ferrite germination onthe inclusions, provided that these have the necessary characteristics and are thuspresent on titanium oxide surface zones. When the whole chemical analysis of themolten metal is well balanced in terms of manganese, and possibly nickel, so that itshardenability is optimal for the thermal cycle undergone by the weld, theproeutectoid ferrite network is reduced to a fine edging, the remainder of austenitebeing transformed into acicular ferrite. What is more, if it is possible to resort to anaddition of molybdenum, which is the case when a yield strength higher than 550 or600 Mpa is sought, a synergic boron-molybdenum effect is thus obtained whichmakes it possible to remove the proeutectoid ferrite network completely and toobtain a structure only made up of acicular ferrite whose toughness properties areremarkable. Lastly, it should be noted that the action of titanium and boron is notlimited to the increase in the proportion of acicular ferrite, in the zones with a roughsolidification structure, it also causes a refinement of the ferrite grains in thereaustenitized zones (see Figure 4.11). Our recourse to the titanium-boron effect thus makes it possible to achieve anotable improvement of impact strength values in all the weld zones and a betterhomogeneity of the properties in these various zones. However, these positiveresults are obtained only if the nitrogen content is low and perfectly controlled. Thisis why this effect was originally implemented in the filler products for themanufacture of large tubes by bypass multielectrode sub-merged arc welding. It wasthen used in filled rutile wire and gave this product a privileged position as it
Molten Metal 149conformed to the strictest metallurgical specifications. On the other hand, it is notused in coated electrodes because this process does not allow a sufficient control ofthe nitrogen content in the added metal.4.3. Principal welding defects We will not deal with defects of a purely operational origin such as grooves, lackof penetration, sticking, etc. here; we will rather consider only internal defects, thatis to say, hot cracks, cold cracks, reheating cracks and porosities. We will endeavor to clarify the criteria which make it possible to identify thesephenomena and to show the mechanisms of their formation in order to deduce theprecautions we must take to avoid them or the remedies to be applied when theproblems appear.4.3.1. Hot cracking Under this term, we include solidification cracks, liquation cracks and cracksresulting from a lack of ductility at high temperature.Solidification cracks These appear at the end of solidification. They can be internal or emerge on thesurface but they are always localized in interdendritic spaces and thus follow thedirections of solidification. Thus, they are perpendicular to the isotherms at anypoint. As they are formed at high temperature, they are oxidized in contact with theair when they emerge on the surface. Lastly, they are always broad because ofcontractions in the surrounding metal during cooling. The factors that influence hotcracking are partly dependent on the analysis of themolten metal and partly on the welding procedure (see Table 4.4).
150 Metallurgy and Mechanics of Welding Figure 4.11. a) Rutile filled wire without Ti-B effect; b) same formula with addition of boron. Impact test notches positioned in the pass axis (zb) and in the mold axis (zr)
Molten Metal 151 Figure 4.12. Localization of solidification cracks A long solidification period and the presence of constituents with a low meltingpoint mean that the solid and liquid phases will coexist over a vast temperaturerange. During cooling in this field, the liquid is transformed into a solid whilecontracting (volume variation in solidification) while the solid already formedcontracts according to its own dilation coefficient. It can be understood that thelonger the solidification time, the greater the risks of insufficient material at the endof solidification and of a crack appearing in the zones which solidify last, i.e. in theinterdendritic spaces. Factors related to material Factors related to the operational process and the welding process Lengthy solidification Certain weld bead shapes (concave surface, width/depth ratio <0.7) Constituents with a low melting point High speed of welding Base metal with high elastic limit Rigorous clamping Table 4.4. Factors leading to cracking on solidification The influence of the base metal’s yield strength and the clamping of the parts tobe assembled are of a different nature. When the molten zone cools, it contracts sothat stresses will develop if the shrinkage cannot freely take place. These shrinkagestresses will apply to the molten metal in the course of cooling, forcing it to distort,which it will be able to endure or not as the case may be. The greater the internal orexternal clamping thus limiting the deformations of the assembly, the greater thesestresses will be. Although often underestimated, the shape of the weld beads and the weldingspeed have a major influence. The zone which solidifies last concentrates theimpurities because of their rejection in the liquid phase during solidification. Thismakes it chemically more sensitive to the risk of cracking and, when the weld has aconcave surface, this zone is also smaller in its cross-section. Thus, shrinkagestresses are more likely to generate cracking than when the surface is convex (seeFigure 4.13). In the same way, when a bead penetrates deeply (low
152 Metallurgy and Mechanics of Weldingwidth/penetration ratio), its edges are parallel so that the final stage of solidificationaffects its entire height (central column); on the other hand, when the form istriangular, solidification finishes on the bead surface, which reduces the risks ofcracking. Lastly, a reduction in the welding speed, and thus the solidification speed,makes it easier for the remaining liquid to fill the gaps created between theinterdendritic spaces by the reduction in volume related to the liquid to solid phase;thus, the risk of cracks appearing are reduced. Figure 4.13. Influence of the shape of weld beads on solidification cracking These considerations are general and thus apply to all types of materials, but tostate that a lengthy solidification period or the presence of constituents with a lowmelting point worsens the risk of cracking is not in practice of any great use for thewelding engineer who must use materials of whose characteristics he is oftenunaware. It is more in his interest to take account of these risks by using thematerial’s chemical analysis. In the case of mild and low alloyed steels, Bailey [BAI 78] deduced from afactorial experiment the parameter UCS (Units of Crack Susceptibility) whichcharacterizes susceptibility to the formation of cracks at solidification in submergedarc welding analyzing the molten metal: UCS = 230C* + 190S + 75P + 45 Nb – 12.3Si – 5.4Mn - 1with C* = 0.08 if C < 0.08% and C* = C if C > 0.08%. He indicated its validity for the following values: C<0.23%; S 0.010-0.050%; P0.010-0.045%; Si 0.15-0.65%; Mn 0.45-1.6%; Nb<0.07%; Ni <1%; Cr <0.5%; Mo<0.4%; V <0.07%; Cu <0.3%; Ti <0.02%; Al <0.03%; B <0.002%; Pb <0.01%; Co<0.03%. Later [BAI 94], he specified that an increase in chromium, molybdenum orvanadium beyond these values reduces the risk of cracking at solidification, while anincrease in nickel and boron have a negative effect. However, he also stated that the
Molten Metal 153harmful influence of boron was demonstrated only for values higher than 0.01%. Inthis same document, the author considered that the risk of cracking is negligiblewhen the UCS parameter is lower than 10 and very large when it is higher than 30,value 20 corresponding to the threshold of appearance of cracks during theexecution of fillet welds in the first publication. From this formula, it is seen that carbon does not have an effect up to 0.08% butproves to be the most harmful element beyond this value, i.e. from the momentwhen solidification involves the peritectic reaction. That is broadly explained by thefact that the solubility of sulfur and phosphorus are much lower in austenite than inferrite, so that the appearance of the peritectic reaction results in an increase in thesegregation of these elements, thereby promoting the formation of interdendriticfilms with a low melting point and thus the risk of cracking. The element coefficients which play a part in this UCS parameter are relative tosubmerged arc welds. They cannot be generally applied to other processes, inparticular because other factors which have an influence on cracking (beadgeometry, welding speed) differ enormously from one welding process to another.Nevertheless, the chemical elements with negative or positive effects remain thesame. Faced with a problem of solidification cracking in a C-Mn or low alloyedsteel weld, it will always be beneficial to reduce the content of elements C, S, P andNb and to an increase in Mn and S in the molten metal. A wise choice of the fillerproduct can contribute to increase Mn and Si but will not have an effect on theharmful elements because these elements do not vary significantly in weldingproducts. In practice, if their concentration is at an unacceptable level in the moltenmetal, this is because they come from the dilution of the base metal. A procedurewill then have to be implemented which makes it possible to minimize dilution andwill, in extreme cases, involve preliminary buttering of the faces to be joined. In the case of austenitic stainless steels, the risk of solidification cracking isclosely related to the phases involved at this time. Indeed, depending on theirchemical composition, austenitic stainless steel welds can solidify completely inaustenite or primary austenite then ferrite, or in primary ferrite then austenite or,finally, completely in ferrite. However, we have already seen that the solubility of impurities such as sulfurand phosphorus was much greater in ferrite than in austenite and that the segregationof these elements could lead to interdendritic film formation at a low melting point.If the results of the many studies relating to the cracking sensitivity of austeniticstainless steels are classified according to the mode of solidification [KOT 93], anincreasing resistance is observed passing from the purely austenitic mode to theprimary austenite mode, then to the completely ferritic mode and finally to theprimary ferrite mode. The large resistance of the primary ferrite mode compared to
154 Metallurgy and Mechanics of Weldingthe completely ferritic mode probably resulting from the fact that the mixedsolidification ferrite + austenite generates a greater length of interfaces and thusminimizes the segregations. Many diagrams exist for predicting the structure of the deposited metal addedaccording to the content of alpha gene elements (chromium equivalent) and gammagene elements (nickel equivalent), the first and best known of them being thatestablished by Schaeffler more than 50 years ago [SCH 49]. However, the majorityof these diagrams indicate the structure of the as welded metal after cooling to roomtemperature and this structure can be very different from that which existed at thetime of solidification because, during cooling, the ferrite generally regresses intoaustenite. Suutala [SUU 83] proposed a diagram to forecast the solidification mode,in which he distinguishes the fields of solidification in primary austenite andprimary ferrite. However, in our opinion, the most informative and best adapteddiagram to modern day steels is WRC 92 (see Figure 4.14) because it marks out thezones corresponding to the four solidification modes and also gives, expressed interms of Ferrite Number, the ferrite content after cooling. From this diagram it is thus possible to evaluate the cracking sensitivity of aweld according to the position of the point being analyzed in the fields A, AF, FA orF; this analysis can be the result of a measurement or an evaluation starting from theanalysis of the base metal, the deposited metal and the estimated dilution rate. Therisk can also be evaluated by measuring the ferrite number of a standard weldrepresentative of the proposed joints with an apparatus such as the feritscope MP30since it can be seen in this diagram that a ferrite number higher than 4 correspondsin the majority of cases to welds solidifying in the FA field (most resistant) or F. Ifthe representative point is in a zone at risk (A or AF, or FN <4), it will be found tobe very beneficial, unless the specifications prohibit it, to modify the choice of fillerproduct or the welding procedure (dilution rate) so as to fall inside the fields FA orF. Lastly, for the cases where that proves to be impossible, it will be absolutelyessential to pay attention to the shape of the bead, to minimize clamping and to use alow welding speed as we indicated before.
Molten Metal 155 Figure 4.14. WRC 92 diagram; from [KOT 92]Liquation cracks Liquation cracks occur mainly in the base metal’s HAZ, in the vicinity of thebond zone. They can also occur in the molten metal during thermal reactivation by alater pass, but in this case are generally prolonged in the form of solidificationcracks in the pass currently being made. They are localized in the part of the HAZbrought up to temperatures that conform to the material’s solidification interval, aperiod which will be longer, the greater the content of the material’smicrosegregations of elements which support the formation of constituents at lowmelting point. Under the shrinkage effect associated with cooling, these partialfusion zones will be all the more likely to experience cracks the deeper they extendinside the HAZ. It is this type of mechanism which is frequently encountered duringthe welding of molded products; it is very close to the formation mechanism ofsolidification cracks in the molten metal. Another cause of the appearance of liquation cracks can be the formation of aeutectic around a phase of the dissolution process in the matrix. This can occur when a thermodynamic phase, stable at room temperature, isunstable at high temperature and its return into solution could not be complete or itschemical homogenity reached because of the speed of the thermal welding cycles inregard to the kinetics of dissolution and diffusion. In this case, a liquid phase will
156 Metallurgy and Mechanics of Weldingappear inside the HAZ and will penetrate the surrounding grain boundaries, entailingtheir liquation and their cracking upon cooling because of shrinkage. The sensitivity of any material to liquation cracking can be evaluated by meansof hot tensile tests conducted via a simulation of a thermal welding cycle during theheating phase and the cooling phase (see Figure 4.15). This test makes it possible todetermine the difference between the temperature at which the reduction in therupture area becomes zero after heating and the temperature at which a certaincapacity for deformation is restored on cooling. The greater the difference, the moresusceptible the material is. Figure 4.15. Hot ductility of the Cabot 214 alloy containing (a) 2 ppm of boron, or (b) 30 ppm; from [CIE 93] This sensitivity to liquation cracking by is thus an intrinsic characteristic of thematerial; it depends on all of the chemical elements present, their distribution andthe microstructure, i.e. that the welding process has little influence on the resultunless using a filler product whose melting point is significantly lower than that ofthe base metal (braze welding).Cracks due to lack of hot ductility (ductility dip cracking) During cooling from the liquid state, many industrial alloys enjoy a temperaturerange in which the liability for deformation is notably lower than for thetemperatures either side. The cooling curve in Figure 4.15a makes it possible topredict such behavior. This decline in ductility, which is more marked the lower the deformation speed,is in the vicinity of the alloy’s recrystallization temperature. It can be at the origin ofintergranular cracks both in the HAZ as well as in the molten metal, due toshrinkage caused by the weld cooling [HEM 69] but this type of cracking is seldom
Molten Metal 157evoked in the case of ferritic steels. In these steels, however, certain authors [LIM96] consider that these intergranular cracks can be prolonged, after completecooling, by transgranular cracks induced by hydrogen, and would be at the origin ofherringbone cracks (see following section). On this subject, the bibliography is more descriptive than explanatory;nevertheless, it seems that there still, sulfur accentuates the phenomenon.4.3.2. Cold cracking These cracks appear at low temperatures (lower than 200°C). Thus, they are fineand do not have an oxidized surface. They do not have a particular orientationcompared to the microstructure. They generally develop in the HAZ but cansometimes occur in the molten metal when it has a very high elastic limit. Theyderive from the stress field, which explains why they occur in the concentrationzones which constitute the surface defects (poor wetting, grooves) or discontinuitiesrelated to the assembly design (partial penetration for example). Figure 4.16. Example of cold cracking These cracks require the combination of three factors to occur: – a not very ductile structure (martensite), – stresses, – hydrogen. The respective influence of these three factors is perfectly highlighted by meansof implant tests. To carry out these tests, cylinders of the material underconsideration are taken. A notch of well defined geometry is machined close to oneof the ends. The bar is placed in a support plate (see Figure 4.17) then a weld bead is
158 Metallurgy and Mechanics of Weldingmade so that the notch of the bar is located in the HAZ of the weld bead. Duringcooling, a load is applied to the other end of the bar and is maintained for severaldays. The specimen is then cut open in order to determine whether cracks havedeveloped at the notch extremity. The test is repeated by applying various loads in order to evaluate the minimalcracking load of the structure in the notch bottom. It is also repeated by modifyingthe welding conditions, which makes it possible to highlight the influence of t800/500 and to plot the cracking curve as it appears in Figure 4.16. In parallel thehardness curve under the bead is plotted according to the same t 800/500parameter, the hardening evolution in fact representing the structural evolution. Figure 4.17. Implant test We thus see in Figure 4.17 that for low t 800/500 parameters which areassociated with a martensitic structure (peak of the hardness curve), the crackingstress is very low but, as soon as the structure is no longer 100% martensitic, thecracking stress increases significantly. The steel considered in this example being oftype E36, it can moreover be seen that in this figure there will be no risk of crackingif t 800/500 is higher than 7 or 8 seconds, since then the coarse grain zone is ableto support a stress higher than the elastic limit of the base metal without fissuring,which cannot occur because that would generate the deformation of the base metaland its stress relaxation. All steels have a behavior similar to that in Figure 4.17 where the relationbetween cracking stress and structure is clearly seen. The tests corresponding to this figure were carried out using a welding productwhose diffusible hydrogen content was of 5.5 ml per 100 g of metal deposited. The
Molten Metal 159same tests can be reproduced with other hydrogen contents in order to evaluate theinfluence of this third factor. In Figure 4.18 we see that when diffusible hydrogen content increases, crackingstress significantly decreases whatever the t 800/500 considered. Thus, hydrogenseems a fundamental determinant of cold cracking. However, even when hydrogenis in a reduced quantity, a low stress is enough to cause cracking if the structure iscompletely martensitic. Thus, wherever possible, it will be necessary to choosewelding conditions (welding energy, pre-heating) which avoid the formation of a100% martensitic structure in the HAZ. Figure 4.18. Influence of diffusible hydrogen content on the cracking curve; from [COL 77] However, this is not possible with all steels. Indeed, some, like martensiticstainless steels for example, have a hardenability such that to avoid the martensitictransformation, cooling should last several days. To weld such steels it is imperativeto ensure that hydrogen has been expelled before letting the assembly cool in thetemperature range, otherwise cracking may appear (under 200°C). This is the aim ofpost-heating. The crack curves in the preceding figures relate to the HAZ but the influence ofhydrogen, the stress and the structure which these figures illustrate turns out to beidentical when tests are carried out by taking extracts from the deposited metal[DEB 92]. As we indicated previously, cold cracking can occur in molten metal when steelsof high elasticity limits are welded. Generally, it is in this case transverse across the
160 Metallurgy and Mechanics of Weldingbead but can also be longitudinal when a discontinuity exists under the bead root(partial penetration) or take the appearance of a herringbone crack (microscopiccracks angled at 45° to the welding direction) in welds with intermediate tensilecharacteristics [MOT 82]. This transfer of cold cracking localization away from theHAZ towards the molten metal is increasingly likely the higher the elastic limit ofthe deposited metal, given that welds are made with steels of modern design whosecarbon content is low. Thus, during the welding of these steels, it is no longer theanalysis of the base metal which dictates the pre-heating temperature required toavoid cracking in the HAZ, but the analysis of the molten metal in order to avoidbead cracking. An interesting means of reducing the risk of cold cracking and consequently pre-heating temperature during the welding of these steels consists of using a filler forthe execution of the root passes for “X” or “K” shaped assemblies, the remainder ofthe joint being filled with a filler product akin to the mechanical characteristics ofthe base metal. By doing this, it has been shown that the pre-heating temperature canbe reduced by 50 to 100°C, a reduction of 50°C when compared to the use of asingle product, and this of course without affecting the overall tensile characteristicsof the joint [VUI 94]. In many cases, this amounts to eliminating the need for pre-heating, which, in addition to presenting a direct and immediate economic advantagefor the manufacturer, considerably improves working conditions for welders andgenerally results in a reduced rate of operational defects, and therefore of repairs.Curiously, this practice is still not very widespread today. The actions required to avoid cold cracking are thus derived from all the aboveconsiderations, and are recapitulated in Table 188.8.131.52.3. Reheat cracking Reheat cracking, intergranular in nature, occurs primarily in the coarse grainHAZ and occasionally in the molten metal. It begins during the post welding heattreatment or in service at high temperature [DHO 92]. It relates to low alloyed steelscontaining carbide-forming elements (Cr, Mo, V) but also certain austenitic stainlesssteels such as steel AISI 347, as well as precipitation hardening nickel alloys(Inconel 800H for example).
Molten Metal 161 1) Minimize the quantity of hydrogen introduced into the weld pool – Cleanliness of the joint Moisture, oil, grease, etc. – Choice of welding products Low diffusible hydrogen. – Heating and conservation of the According to supplier recommendations. products (except if cases of airtight stocking) 2) Wherever possible, use a filler product with very low elastic limit and very low hydrogen content for the execution of the first pass and the secondary pass of thick assemblies 3) Control the welding conditions to avoid the formation of a martensitic structure – Welding energy To choose starting from the under bead hardness curves according to t 800/500 – Pre-heating and the IRSID graph for example [COL – Temperature between passes 77] 4) Envisage a post-heating to evacuate hydrogen before cooling (case of steels having a great hardenability), always associate with a pre-heating to avoid cooling lower than the critical temperature before post-heating is effective 5) Minimize the internal or external stresses – Welding procedure – Clamping Table 4.5. Actions to take to avoid cold cracking Such cracking derives from the relieving of strong residual stresses resultingfrom manufacture when the deformations which accompany it are concentrated atthe level of the grain boundaries. This is the case for the coarse grain HAZ ofprecipitation hardened materials because, during welding, the carbides which hardenthese alloys are put back in solution in the zones taken to a very high temperature inthe vicinity of the bond zone and remain during cooling because of the speed of thewelding thermal cycles. During a later reheating, in service or during the post welding heat treatment, thecarbides will precipitate inside the grains on the dislocations created by strainhardening that results from thermal cycles. This will reinforce the matrixconsiderably, so that the creep deformations associated with stress relief will locatethemselves on the level of the grain boundaries which cannot support them. This type of crack thus relates primarily to thick assemblies of materialsdesigned to resist creep, the thickness inducing a high level of residual stresses.However, the risk is not only related to the nominal analysis of material, it is also afunction of the impurity content (S, P, As, Sb) and residuals (Cu, Sn), because theseelements segregate to the level of the grain boundaries and weaken them.
162 Metallurgy and Mechanics of Welding Various methods are used to evaluate susceptibility to reheat cracking [DHO 98,TAM 95], but our preference is to reduce the area measurement during hot tensileisothermal tests of specimens in which, by thermal simulation, the structure of thecoarse grain zone has previously been reproduced. Indeed, it is considered that therisk is very low when no reduction of area value lower than 20% is recordedregardless of the test temperature; on the other hand, it is very high when thestriction becomes lower than 10%. In practice, to minimize risks when a susceptible material must be used, it is ofgreat importance to: – design the joints to reduce clamping as far as possible, – choose a welding product that has the lowest hot tensile characteristicscompatible with the application, – use a low energy welding process in order to limit the pass volume and to thusreduce the dimension of the coarse grain HAZ, – distribute the passes to reaustenitize the coarse grain zones created by thepreceding passes and thus decrease the grain size, – envisage welding sequences to minimize residual stresses, – ensure a good wetting of the finishing passes and the absence of grooves so asto avoid stress concentrations. In addition, the handling of the post-welding heat treatment can have a capitalincidence on reheat cracking since it has been shown in the laboratory andproduction, that the cracking of a CrMoV steel which has a low ductility in theinterval 550-650°C can be avoided by carrying out a stage at a temperature of about450°C then very quickly crossing the field of low ductility in order to reach thetreatment temperature [PIL 86].4.3.4. Porosities We will distinguish four mechanisms likely to engender porosities in moltenmetal: – the instability of the gas capillary for weldings carried out by means of HDEprocesses, – an excessive gas pressure under the bead root, – a dissolved gas content in molten metal higher than the solubility limit in solidmetal at the solidification temperature,
Molten Metal 163 – a chemical reaction within the weld pool giving rise to a gas. The HDE processes involves keyhole work. This implies that the weld pool ismaintained in balance thanks to the gas vapor pressure which is exerted on thecapillary walls created by the volatilization of metal under the influence of a veryhigh density plasma arc, laser beam or electron beam. When the operatingconditions allow us to maintain a perfectly stable state of balance, the liquid walllocated at the back of the capillary can collapse in a more or less periodic way andenclose part of the metal vapors which maintained it, thus forming porosities. Thesehydrodynamic porosities could generally be avoided by modifying the power densitydistribution of the incidental beam (point of focusing, vibration, etc.) and byreducing the welding speed. Figure 4.19. Pre-painted sheet fillet weld – porosity resulting from paint decomposition under the bead When porosities result from excessive gas pressure under the bead root, they takea lengthened form and maintain a connection with the zone at the origin of thisexcessive pressure. The pressure can result from the heating of air imprisoned under the bead; this istypically the case for butt welds with a preparation by joggling when the penetrationis insufficient. It can also derive from a gas release that results from thedecomposition or volatilization of product coating sheets, as is the case during filletwelding of pre-painted sheets (see Figure 4.19) or lap welding with galvanized
164 Metallurgy and Mechanics of Weldingsheets. Lastly, its origin may be a degasification of the faces to be assembled; it is,for example, the nitrogen released from the plasma air cut faces which explainsmany porosities which are formed in the first pass of a butt welded assembly whenthere is no lower edge spacing of the joint (see Figure 4.20). Figure 4.20. Texture test after the first pass of a submerged arc butt welded joint of as-cut sheets cut by the plasma air process The sudden reduction in the solubility of a gaseous element at the time of thepassage from the liquid state to a solid state is the leading cause of porosities in theweld beads because this variation is common to all materials (see Figure 4.21).Indeed, when the dissolved gas concentration in molten metal is higher than thesolubility limit in solid metal at the solidification temperature, there is a rejection ofgas to the solid-liquid interface. This causes the liquid to experience a local increasein the dissolved gas content and, when this becomes higher than the solubility limitin the liquid, a gas bubble is formed. In welding, the weld pool can be contaminated by atmospheric nitrogen andoxygen if protection is not assured, or by hydrogen coming from welding productsthat have absorbed moisture, by water vapor which condenses on the surface of acold sheet, an escape in the coolant circuit of the torch, or the decomposition of oilor grease present at the surface of a badly prepared joint. Oxygen is generally not atthe origin of porosities because it reacts with the majority of materials to formoxides. In ferritic steels and nickel alloys not containing nitride forming elements(Ti, Al, Nb), it is in general the nitrogen which is at the origin of porosities, while itis hydrogen in aluminum alloys but also in austenitic stainless steels, although theyare more resistant than light alloys.
Molten Metal 165 Figure 4.21. Evolution of solubility with temperature: a) hydrogen in various pure metals [LAN 99]; b) nitrogen in pure iron [KOU 87] A chemical reaction giving rise to a gas within the weld pool constitutes the lastcause of porosities which we will deal with here. Formation of carbon monoxidewas at the origin of porosities which were inevitably formed during TIG welding ofrimmed steels unless a filler very rich in deoxidizers was used. However, even if weno longer encounter this kind of steel, the CO release in molten metal can still occurwhen the residual oxygen of steel is present in the form of silicates, because at veryhigh temperature (>1,600°C) they can be reduced by the carbon of the steel. Thisreaction is particularly intense during electron beam welding because thesurrounding vacuum moves thermodynamic balances. It also favors this reduction tothe extent that it becomes impossible to obtain a sound weld, unless the steelcontains residual aluminum (approximately 0.02%), aluminates being more stablethan carbon monoxide at the temperature of the weld pool (see Figure 4.22). Steamformation in the weld pool can also be at the origin of porosities. This will occur inthe presence of hydrogen with materials for which the enthalpy of oxide formation islower in absolute value than that of steam at the temperature of the weld pool. Thisis the case for copper, particularly when it is not deoxidized; it is also the case forpure nickel, Monel metal and even certain nickel-chromium-iron alloys [LAN 99].There is only one remedy: use filler products which contain powerful deoxidizerssuch as titanium and aluminum to avoid this reaction.
166 Metallurgy and Mechanics of Welding Figure 4.22. Surface aspect and X-ray on a section of EB welds of XC 38 (Al = 0.002%):a) without insertion; b) with insertion in the mating plane of an aluminum foil 0.02 mm thick4.4. Bibliography[ABS 78] ABSON, DOLBY R.E., HART P.H.M., “The role of non-metallic inclusions in ferrite nucleations in carbon steel weld metal”, Proceedings of Trends in Steels and Consumables for Welding, The Welding Institute, Paper no. 25, London, 14-16 November. 1978.[ANT 81] ANTUNES M., BONNET C., “Application d’un essai de trempabilité à la recherche des facteurs ayant une influence sur la formation de la ferrite aciculaire”, Journées d’information Métallurgie de la Zone Fondue, Société Française de Métallurgie/Société des Ingénieurs Soudeurs – Section sud-est, Conférence no. 9, Publication de la Soudure Autogène, 1981.[BAI 78] BAILEY N., JONES S.B., “The solidification cracking of ferritic steel during submerged arc welding”, Welding Journal, p. 217s-231s, August 1978.[BAI 94] BAILEY N., Weldability of Ferritic Steels, Abington Publishing, 1994.[BLA 99] BLAIS C., L’ESPÉRANCE G., EVANS G.M., “Characterisation of inclusions found in C–Mn steel welds containing titanium”, Science and Technology of Welding and Joining, vol. 4, no. 3, p. 143-150, 1999.[BON 80] BONNET C., “Relation Structure – Résilience dans les soudures d’aciers doux et faiblement alliés brutes de solidification”, Soudage et Techniques Connexes, p. 3, July- August 1980.[BON 86] BONNET C., GASPARD-ANGELI A., “Influence de la teneur en azote sur la résilience des soudures d’aciers C-Mn”, Soudage et Techniques Connexes, p. 3, May-June 1986.[BUR 88] BURKHARDT J., LAU T., NORTH T.H., L’ESPÉRANCE C., “Effect of aluminum on the Ti-O-B-N balance in submerged arc welding”, Welding Journal, p. 25-30, August 1988.
Molten Metal 167[CHA 83] CHARPENTIER J.P., BONNET C., “Effect of deoxidation residues in wire and of some particular oxides in CS fused fluxes on the microstructure of submerged-arc weld metal”, in Proceedings of the Effects of Residual, Impurity and Micro-alloying Elements on Weldability and Weld Properties, The Welding Institute, Paper no. 8, London, 15-17 November 1983.[CIE 93] CIESLIAK M.J., “Cracking phenomena associated with welding”, ASM Handbook, vol. 6, p. 88-96, 1993.[COC 78] COCHRANE R.C., KIRKWOOD P.R., “The effect of oxygen on weld metal microstructure“, Proceedings of Trends in Steels and Consumables for Welding, The Welding Institute, p. 103, London, 14-16 November 1978.[COL 74] COLLECTIF, Courbes de transformation des aciers de fabrication française, edited by the CPS, 1974.[COL 77] COLLECTIF, Courbes Dureté/Paramètre de refroidissement en conditions de soudage, collection established at the IRSID, 1977.[DEB 92] DEBIEZ S., GAILLARD L., MALTRUD F., Etude de la soudabilité d’un acier de nuance E690 T+R de Sollac avec des produits d’apport à bas et très bas hydrogène, Rapport Institut de Soudure no. 28406, 1992.[DEV 83] DEVILLERS L., KAPLAN D., MARANDET B., RIBES A., RIBOUD P.V., “The effect of low level of some elements on the toughness of submerged-arc welded CMn steel welds”, Proceedings of the Effects of Residual, Impurity and Micro-Alloying Elements on Weldability and Weld Properties, The Welding Institute, London, 15-17 November 1983.[DHO 92] DHOOGE A., VINCKIER A., “La fissuration au réchauffage – revue des études récentes (1984-1990)”, Le Soudage dans le Monde, vol. 30, no. 3-4, p. 45-71, 1992.[DHO 98] DHOOGE A., “Survey on reheat cracking in austenitic stainless steels and Ni base alloys”, Welding in the World, 41, p. 206-219, 1998.[EVA 97] EVANS G.M., BAILEY N., Metallurgy of Basic Weld Metal, Abington Publishing, 1997.[GAR 75] GARLAND J.G., KIRKWOOD P.R., “Towards improved submerged arc weld metal toughness”, Metal Construction, p. 275-283, May 1975, p. 320-330, June 1975.[HEM 69] HEMSWORTH B., BONIZEWSKI T., EATON N.F., “Classification and definition of high temperature welding cracks in alloys”, Metal Construction and British Welding Journal, p. 5-16, February 1969.[KOT 92] KOTECKI D.J., SIEVERT T.A., “WRC-1992 constitution diagram for stainless steel weld metals: a modification of the WRC-1988 diagram”, Welding Journal, p. 171s-178s, May 1992.[KOT 93] KOTECKI D.J., “Welding of stainless steel”, ASM Handbook, vol. 6, p. 677-707, 1993.[KOU 87] KOU S., Welding Metallurgy, John Wiley & Sons Inc., 1987.[LAN 99] LANCASTER J.F., Metallurgy of Welding, Abington Publishing, 1999.
168 Metallurgy and Mechanics of Welding[LIM 96] LIMU H., HANNERZ N.E., “Influence of vanadium and niobium on weld solid state cracking”, Int. J. for the Joining of Materials, vol. 8, no. 4, p. 134-144, 1996.[MOT 82] MOTA J.M.F., APPS R.L., “Chevron cracking – a new form of hydrogen cracking in steel weld metals”, Welding Journal, p. 222, July 1982.[PIL 86] PILARCZYK J., DEBSKI E., “Reheat cracking in low alloy steel weldments and welded structures”, Proceedings of 3rd International Conference Joining of Metals (JOM-3), Helsinki, Finland, December 1986.[SCH 49] SCHAEFFLER A.L., “Constitution diagram for stainless steel weld metal”, Metal Progress, 56, S 680, 1949.[STL 93] ST LAURENT S., Etude de l’influence du Bore, de Titane et de l’Azote sur les propriétés de la zone fondue de dépôts soudés d’aciers microalliés, Thesis, University of Montreal, Ecole Polytechnique, July 1993.[SUU 83] SUUTALA N., “Effect of solidification conditions on the solidification mode in austenitic stainless steels”, Metall. Trans., 14A, p. 191-197, 1983.[TAM 95] TAMAKI K., SUZUKI J., IMAI I., HORII Y., KUMAGAI T., “Effects of impurities and alloying elements on reheat cracking sensitivity of 720 N/mm2 class high-strength steel”, Welding International, vol. 9, no. 12, p. 960-966, 1995.[VUI 94] VUIK J., VAN WORTEL J.C., VAN SEVENHOVEN C., “Application of very low yield strength consumables in the root pass of weldments to avoid preheating”, Welding in the World, vol. 33, no. 5, p. 362-369, 1994.
Chapter 5 Welding Products5.1. Coated electrodes5.1.1. Constitution of coatings: consequences The classification standards of welding products distinguish several types ofcoated electrodes according to the kind of coating. An electrode coating is always composed of many constituents which providevarious functions: – mineral products which act on fusion characteristics, contribute to theprotection from the surrounding atmosphere of the drops and the weld pool bybreaking up into a gaseous emission under the influence of the arc heat andconstituting a slag whose physico-chemical characteristics have a major influence onthe operational characteristics of the electrode; – metal products which by being combined with metal resulting from the fusionof the electrode core, make it possible to adjust the analysis of the weld metal so asto obtain properties equivalent to those of the steel used in the welded joint; – organic materials added in small quantity in basic coatings as an extrusionagent and which will be destroyed during high temperature heating of theseelectrodes. They are present in much larger quantities in electrodes baked at lowtemperature (cellulose, rutiles, etc.) because the decomposition of these products inthe arc causes a release of hydrogen which confers operational characteristics onthem which prove valuable in many applications;Chapter written by Christian BONNET.
170 Metallurgy and Mechanics of Welding – binders which make it possible to obtain a solid coating which adheres to themetal core. There are in general simple or complex silicates of sodium, potassium orlithium, which in addition to their adherence function act on the arc characteristicsbecause of the low ionization potential of the alkaline elements. In industry, basic and rutile electrodes are the most commonly used. Table 5.1makes it possible to compare on the one hand the constituents and the bakingconditions and, on the other hand, the consequences which result from this both foroperational properties and chemical analysis of the deposited metal. Type of electrode Rutile Basic TiO2, Al2O3, SiO2, CaF2, MgO, Non- components Carbonates, cellulose, etc. Carbonates, etc. Principal metallic Silicates, extrusion additives Silicates, extrusion additives Alloying elements Alloying elements Metallic Deoxidizers Deoxidizers Stoving temperature Low (<160°C) High (350/480°C) Soft fusion, stable arc, Irregular fusion, unstable arc, aggressive, Transfer in fine drops, no or few Transfer in large drops with Operational short-circuits, short-circuits, Difficult restarting, Consequences Easy restarting, Slag with high melting point Slag with low melting point, favoring wetting tendency to undercut O: 600 to 1,000 ppm O: 200 to 500 ppm Ti: 300 to 800 ppm Ti, Nb, V: adjustable to the Analytical Nb: 100 to 300 ppm desired values V: 50 to 250 ppm H2Diff: >15 ml/100 g DM H2Diff: <5 ml/100 g DM Table 5.1. Principal constituents and characteristics of rutile and basic electrodes Thus, it appears that rutile type electrodes present the best properties in use: avery good arc stability, transfer of metal in fine drops which generally results in alow level of spatters and lower fume emission than the basic electrodes, a very goodbead wetting and a very easy restart from cold.
Welding Products 171 However, by its nature, this slag has an influence on the content of residualelements in the deposited metal, elements which are in general not desirable fromthe perspective of optimizing mechanical properties. The oxygen content of the deposited metal can vary according to the nature andthe quantity of the deoxidizing elements present in the coating, nevertheless, itcannot be lowered to the level which can be reached with a basic electrode. Thisresults in a more significant inclusion content and consequently in a lower ductilefracture energy during impact tests. The titanium content of the deposited metal cannot be adjusted, as we wouldwish, in order to optimize the mechanical properties. Indeed, the slag being mainlycomposed of rutile elements (titanium oxide TiO2), some titanium is inevitablytransferred to the deposited metal in variable quantities according to the oxido-reduction reactions and the metal-slag exchanges which occur in the arc and at theinterface with the weld pool. These reactions depend on all the chemical elementspresent, which must be balanced according to the various mechanical characteristicsthat the weld must meet (tensile strength, yield strength) and depending on the typeof steel that we have to weld. The niobium and vanadium content of the deposited metal cannot be loweredbeyond a certain point because these elements exist as impurities in the naturalrutiles used in the manufacture of welding products. The use of synthetic rutiles,which are therefore very pure, is possible but not common because its cost issignificantly higher than that of the natural rutiles. The diffusible hydrogen content of welds created with rutile electrodes is alwaysvery high. This results from the presence of organic materials added to facilitateextrusion and to improve the arc’s characteristics. However, it is also a result of lowbaking temperatures which makes it possible to eliminate only a small proportion ofthe water incorporated with the silicate and it does not break up the extrusion agents. Thus, rutile electrodes are valued for their user-friendliness and the creation of aweld bead, whereas basic electrodes are essential when the joints to be made mustsatisfy severe metallurgical quality standards. A basic electrode must satisfy the required mechanical properties of the steelswhich it is intended to weld (tensile, impact strength, CTOD, creep, etc.). Manyanalytical combinations make it possible to obtain the tensile characteristics soughtin the deposited metal, but the solutions that satisfy both the tensile and toughnesscharacteristics are much more limited. This is increasingly true the higher the tensileproperties. In addition, the chemical balance retained for an electrode must be themost robust possible, i.e. it must satisfy the various requirements in spite of the
172 Metallurgy and Mechanics of Weldingvariations inherent in any industrial production, and that, in a broad field of weldingconditions (thermal cycles). Lastly, a basic electrode must be designed so that thediffusible hydrogen content in the deposited metal is as low as possible in order toavoid any risk of cold cracking, while minimizing or even precluding pre-heatingand post-heating.5.1.2. Basic electrodes and diffusible hydrogen The determination of the diffusible hydrogen content of welding products isproblematic because, due to its small size, the hydrogen atom diffuses easily andescapes from steel even at room temperature, so that it is impossible to know theexact quantity of hydrogen introduced during welding. Faced with this difficulty butalso the need to classify welding products according to their cold crackingsusceptibility, the determination of the diffusible hydrogen content is the subject ofstrict guidelines which very precisely describe the methodology to be used. Thismethodology must be respected scrupulously if extreme variations in results (asmuch as double) are not to be recorded (ISO 3690 or AWS 4.3-1993). Figure 5.1. Diffusible hydrogen/coating humidity ratio for electrodes of type AWS 7018 The diffusible hydrogen content is generally expressed in milliliters per 100grams of deposited metal (ml/100 g DM). It is naturally a function of the moisturecontained in the welding product, but Figure 5.1 clearly shows that there is nogeneral relation between these two measurements and we see in Figure 5.2 that evenwhile being limited to a particular electrode coating, two different relations exist
Welding Products 173according to whether the variation of moisture results from a modification of thebaking conditions or from moisture pick-up. Figure 5.2. Diffusible hydrogen/coating humidity ratio for an electrode type AWS 7018 In fact, the complexity of the relations connecting diffusible hydrogen and thecoating humidity derives from the fact that water exists in various forms: the waterknown as free which corresponds to the first water state taken up during an exposureto a damp atmosphere, and the water called water of crystallization, which ischemically bound to the various electrode constituents. If the temperature of thecoating is raised, free water escapes as soon as it exceeds 100°C, while water ofcrystallization is released only at much higher temperatures which depend on thetype of bond, and therefore the material from it is derived. Thus it can be seen thatfor the same quantity of water in the electrode coating, the higher the extractiontemperature of this water, the more it will be released near the arc in the course ofwelding and the greater the transfer of hydrogen in the weld pool. Thus, when theelectrode baking temperature is lowered during the manufacture of a basic electrode,a decreasing quantity of water of crystallization is eliminated from the coatingmaterial. This small variation of residual water from the baking results in an increasein the diffusible hydrogen content, much greater than a similar variation of watercontent in the coating when it results from moisture pick-up (see Figure 5.2). As acorollary, it is clear that to impose a maximum moisture content in the purchasespecifications of electrodes (or flux for submerged arc welding) with the aim ofobviating the risk of cold cracking has no practical logic, since no universal relationconnecting moisture to diffusible hydrogen exists. On the other hand, using thehumidity measurement, which is much simpler and more rapid than themeasurement of diffusible hydrogen, to verify the manufacturing consistency of agiven electrode at the end of the baking process is a practice that is viable andaccepted. This is acceptable because, for each electrode, a single relation existsbetween the residual baking humidity and diffusible hydrogen.
174 Metallurgy and Mechanics of Welding Today, the majority of welding product manufacturers have a range of basicelectrodes with very low levels of diffusible hydrogen. The best of these guaranteesa level lower than 3 ml/100 g of deposited metal with rods from a newly openedpackage. Such a result can be achieved only by a rigorous selection of raw materials,a high baking temperature and airtight packaging, so as to avoid moisture pick-upduring product storage [LED 92]. In general, these electrodes are also characterizedby a low moisture pick-up when they are exposed to a humid atmosphere. Figure 5.3. Origins of diffusible hydrogen in the molten metal However, the diffusible hydrogen content of the deposited metal is not only afunction of the hydrogen brought in one form or another by the welding product. Inthe case of coated electrodes, the gas flow resulting from the decomposition of thecoating’s constituents is not sufficient to prevent an exchange with the surroundingatmosphere (see Figure 5.3). Thus, the partial hydrogen pressure at the arc level and,consequently, diffusible hydrogen in the deposited metal increase in concert with theabsolute humidity content of the surrounding atmosphere (see Figure 5.4).
Welding Products 175 Figure 5.4. Influence of atmospheric water content on diffusible hydrogen in the deposited metal (SAF data) Dickehut and Ruge proposed a diagram which makes it possible to know thediffusible hydrogen content under any temperature and pressure conditions,provided that we know the result under any single condition. This graph is notuniversal because atmospheric exchanges are necessarily dependent on theprotection given to the electrode (crater depth, volume of released gas, etc.).Nevertheless, the experiment shows that as a first approximation it encompasses thebehavior of the majority of low hydrogen electrodes of type AWS 7018 currentlymarketed.5.2. Fluxes for submerged arc welding5.2.1. Fused fluxes and granular fluxes: advantages and disadvantages Fluxes for submerged arc welding can be produced by fusion or granulation. Fused fluxes are manufactured from coarse raw materials which are mixedbefore being introduced into an electric furnace. They are then brought up to atemperature of about 1,600°C which makes it possible to obtain a chemicallyhomogenous liquid product. This product is then cast on a plate, strongly cooled inorder to confer a glassy structure after solidification and cooling to roomtemperature, thus preserving a perfect chemical homogenity.
176 Metallurgy and Mechanics of Welding This glass is then crushed and sieved so as to obtain the desired granulometricdistribution. In an alternative manufacturing process, the liquid product is atomizedin a water jet instead of being cast on a plate, which obviates the crushing operation. The manufacture of granular fluxes begins with a dry mixture, formed from rawmaterials which in this case have a very fine granulometry (in general lower than300 microns). After homogenization of the dry mixture, mixing is carried out byadding a simple or mixed silicate of sodium, potassium or lithium. Granulation, i.e.the agglomeration of small particles taken from various raw materials, can then takeplace thanks to the silicate binder. This is followed by a pre-drying stage often usinga fluidized bed, then by baking at a temperature of about 500°C if the manufacturedflux contains carbonates or at higher temperature (800°C approximately) even if itdoes not contain any. Fused fluxes and granular fluxes each have their advantages and disadvantages. Each grain of a fused flux is chemically identical to the others, unlike those of agranulated flux whose particles are not chemically homogenous. Thus, it is possibleto manufacture fused fluxes in which a particular element must be present in verysmall quantity, without risking segregation formulae (boron for example). This isparticularly critical for a granular flux. The manufacture of fused fluxes does not require the use of binder. This bringstwo advantages and one disadvantage compared to granular fluxes: – the moisture pick-up of fused fluxes is practically negligible, since water isonly adsorbed on the grain surface. That of a granular flux is on the contrary muchgreater because the binder reacts with atmospheric humidity [GAS 86]; – the fused flux grains are more solid than those of granular fluxes which makesthem more suitable for recycling; – however, the binders used in the manufacture of granular fluxes generallycreate better arc stability than fused fluxes. Fused fluxes, unlike granular fluxes, cannot contain either ferro-alloys ordeoxidizers because these would be oxidized during production in the liquid state.This enables the slag to be reground after welding and reused, mixed with new flux – apractice that can be economically beneficial for certain large industries whose fluxconsumption is high (manufacture of tubes for example) [GAS 86]. On the otherhand, it precludes analytic adjustments and control of the oxygen content of thedeposited metal something which can be achieved with a granular flux by theaddition of deoxidizing elements.
Welding Products 177 Today, granular fluxes are most commonly used in Europe and the USA,whereas fused fluxes are still very popular in Japan and Russia.5.2.2. Roles of flux: metallurgical aspects Submerged arc welding involves the use of a solid or cored wire and a flux, thearc striking into the flux from the end of the wire to the parts to be assembled. Theflux must perform two fundamental functions: it must provide good arc stability andit must protect the weld pool and the metal drops from atmospheric nitrogen andoxygen contamination during their transfer in the arc. Flux also has an importanteffect on the shape of the weld bead (wetting and penetration). This is because italters the power distribution in the arc as well as the physical characteristics of theslag, which result from its fusion and the oxido-reduction reactions occurring duringwelding. This is why, depending on its formulation, a flux can be more or less welladapted to fillet welding, high speed welding or multielectrode welding. Yet, from astrictly metallurgical perspective, the fundamental characteristics of a flux derivesfrom the fact it governs the oxygen and diffusible hydrogen contents of thedeposited metal for a given wire. All contemporary manufacturers of welding products still use the empiricalformula initially put forward by Tuliani to classify submerged arc welding fluxes[TUL 69]. This formula makes it possible to calculate a basicity index bydistinguishing the flux constituents according to their basic character; acid,amphoteric or neutral: 1 [CaO] [MgO] [BaO] [SrO] [Li2O] [Na2O] [K2O] [CaF2] 2 ([FeO] [MnO])BI 2 1 [SiO2] ([Al2O3] [TiO2] [ZrO2]) 2with [AxBy] = percentage by weight of flux constituent AxBy. Tuliani, and others after him, showed that the oxygen content of the depositedmetal decreases when the basicity index increases up to 1.5, then stabilizes around280 to 300 ppm (see Figure 5.5). The net result is that it is pointless to resort to aflux with a significantly higher basicity index when seeking to optimize thecharacteristics of the deposited metal.
178 Metallurgy and Mechanics of Welding Figure 5.5. Relation between the oxygen content of the deposited metal and the basicity of the flux; from [EAG 78] Figure 5.6. Relation between the transition temperature at 70 J and the oxygen content of submerged arc welds; from [TAY 75] What is more, if the temperature change corresponding to a certain value ofrupture energy (70 J in Figure 5.6) measured during impact tests on a great numberof welds according to their oxygen contents, it appears that above 400 to 450 ppm ofoxygen this temperature is always high. Conversely, at lower values a very greatdisparity in the results appears. This confirms the fact that oxygen content, animperfect indicator of the inclusion rate, governs the ductile energy of rupture,which, for high rates, comes very close to the value selected here to characterize thetransition. On the other hand, the very great scattering observed in Figure 5.6 foroxygen contents lower than 400-450 ppm shows that this factor is not determiningbecause it is in fact the microstructure which governs the ductile/fragile transition.
Welding Products 179 The second property of a flux, fundamental on the metallurgical level, lies in thehydrogen content of the deposited metal which it controls. With regard to granularfluxes, what was stated previously for coated electrodes applies: – there is no universal relation between flux humidity and diffusible hydrogen; – for a given flux, two different relations exist between humidity and hydrogendepending on whether the moisture variation results from a variation in residualhumidity after baking or from moisture pick-up; – to achieve low hydrogen levels requires a selection of raw materials containinglittle water of crystallization and releasing this water at the lowest possibletemperature; – the use of mixed binders i.e. sodium, potassium, lithium makes it possible tominimize moisture pick-up; – a rise in flux baking temperature makes it possible to lower the diffusiblehydrogen content of the deposited metal. However, we should not lose sight of the fact that a flux must satisfyrequirements for operational weldability which often prove incompatible with thesearch for a very low hydrogen level. To preclude this difficulty, certain basic fluxesare not baked at very high temperature, they then contain carbonates which whilebreaking up in the vicinity of the arc make it possible to lower the partial hydrogenpressure in the gas cavity and thus reduce the transfer of hydrogen into the moltenmetal. In the case of fused fluxes, the factors which influence the diffusible hydrogencontent are fewer than with granular fluxes but even for a given flux formula, it isnot possible to make the least correlation with the moisture content. This is owing tothe fact that humidity measurements are conventionally taken at 950 or 1,000°C,whereas the preparation of fused fluxes involves taking the flux in its liquid state upto 1,500 or 1,600°C. The moisture measurement, such as it is practiced, cannot thusreveal water content still present in the flux because it is released only at a higherhigher temperature than the manufacturing temperature of fused fluxes. In fact, foreach flux formulation, a strict correlation between its manufacturing temperature andthe content of diffusible hydrogen in the deposited metal is observed (see Figure5.7). A low diffusible hydrogen content is thus not necessarily associated with fusedfluxes; conversely, the exposure of the flux to a humid atmosphere is of littleconsequence, which minimizes the precautions to be taken before its use (storageconditions or heating conditions, etc.).
180 Metallurgy and Mechanics of Welding Figure 5.7. Influence of manufacturing temperature on the diffusible hydrogen content of the metal deposited by two calcium-silicate fused fluxes Figure 5.8. Manganese transfer of granular fluxes AS 231 and AS 589 and fused flux AS 72 (SAF data) A final characteristic to take into account for fused as well as granular fluxesrelates to the transfer of alloy elements in the arc. Indeed, the flux determines the arcatmosphere and thus the chemical exchanges which occur there: the analysis of thedeposited metal is never the analysis of the wire used. Generally, we observe anenrichment in silicon while the manganese content can be above or below that of thewire depending on the flux used (see Figure 5.8). This does not constitute a qualitystandard but these chemical transfer characteristics, given by the supplier, must betaken into account before choosing the wire appropriate for the flux, or dictated bythe properties sought for the weld.
Welding Products 1815.3. Welding gases5.3.1. Welding processes under a gas flux with an infusible electrode TIG (tungsten inert gas) and plasma processes both use a tungsten electrode as acathode. Since tungsten is a very oxidable material and, what is more, tungstenoxide sublimates at low temperature, the shielding gas for TIG and theplasmagenous gas for plasma welding can contain neither oxygen nor CO2. Inaddition, the nitrogen content must be maintained below 2% so as not to adverselyaffect the electrode’s lifespan, even when from a metallurgical perspective it isadvantageous to have more (in the case of welding of duplex stainless steels forexample). Thus, leaving aside the rare and extremely expensive gases such as neon, xenonand krypton, the only gases usable in the mixtures associated with these processesare argon, helium, hydrogen and nitrogen, within the limit indicated before. Argon and helium are neutral gases and can thus be used whatever materials areto be welded, but their respective physical characteristics confer on them specificeffects when welding: – argon has a much lower ionization potential than helium (15.7 and 24.5 eVrespectively) and a much higher electric conductivity (see Figure 5.9). The result isthat it is much easier to start an arc and to stabilize it under argon than under heliumbut also that an arc of given length is, for the same current, more powerful underhelium than under argon (higher voltage); – the thermal conductivity of helium is much greater than that of argon. Thus,with the same current, an arc under helium is more opened out than under argon, andleads to a lower heat gradient at the level of the parts to be assembled, promotingbead wetting. Hydrogen is a diatomic gas at room temperature. When the temperature rises, itpasses initially into an atomic state then to an ionized state, which explains the twothermal conductivity peaks of Figure 5.9, whereas the other gases show only theionization peak. This characteristic has very important consequences for arcwelding: – the hydrogen molecule of the shielding gas absorbs energy by disintegratingaround the periphery of the arc column, which lowers the temperature locally andcauses arc constriction; – the atomic hydrogen present in the arc will recombine while releasing someenergy in the “cool” zones, i.e. at the level of the weld pool, etc.
182 Metallurgy and Mechanics of Welding Figure 5.9. Electric and thermal conductivities of various gases depending on the temperature; from [BOU 83] The arc constriction increases the power density and consequently thepenetration, as the recombination of the hydrogen atoms at the site of the weld poolthus improves the transfer of energy and thus the efficiency of the welding process(see Figure 5.10). As a corollary, for a given electric output and thickness, thecombination of these two effects makes it possible to significantly increase thewelding speeds in the TIG or plasma process by using an argon-hydrogen mixturerather than pure argon or argon-helium. Figure 5.10. Influence of the shielding gas on penetration in TIG welding (316L steel: I = 200 A; distance of electrode to part = 2 mm; welding speed 20 cm/min
Welding Products 183 Thus, the basic gas in TIG or plasma welding is argon, but each time that it ispossible, i.e. in the absence of adverse metallurgical effects, it will be beneficial tofavor the use of argon-hydrogen mixtures. This is because they allow an increase inwelding speed or pass thickness which, in both cases, leads to a significantimprovement in productivity. The use of the ternary mixture Ar-He-H2 can furtherraise welding speed, with helium aiding the bead wetting. Metallurgical incompatibility can result from the formation of porosities in theweld bead with alloys presenting an important variation in the solubility of hydrogenon solidification like aluminum alloys for example. It can also derive from the riskof cold cracking with ferritic steels when they are sufficiently “hardenable” todevelop a non-ductile structure in the HAZ or the molten metal. This last risk musthowever be carefully calculated because the diffusible hydrogen content carried intothe molten metal of course depends on the hydrogen content of the gas mixture used,but remains lower than 5 ml/100 g for a hydrogen content of 3% in argon. On theother hand we can, without disadvantage, use mixtures containing up to 5% ofhydrogen to weld austenitic stainless steels or nickel alloys. When a filler wire is used in TIG or plasma welding, it is introduced in front ofthe arc, just above the liquid bath. It is then molten at the periphery of the arc andthe drops are incorporated one by one in the weld pool without being exposed to thevery high temperatures reached in the center of the arc column. Consequently, thereare few analytical differences between the deposited metal and the filler wire, theonly notable variation relating to the loss of nitrogen during the welding of duplexand superduplex steels. The use of a welding gas containing nitrogen makes itpossible to adjust the content in the deposited metal and to thus improve thecorrosion resistance of the weld bead (see Figure 5.11). Figure 5.11. Nitrogen content of the deposited metal as a function of the nitrogen content of the shielding gas (TIG welding); superduplex wire; nitrogen in the wire: 0.25%
184 Metallurgy and Mechanics of Welding5.3.2. Welding processes under a gas flux with a fusible electrode The gas mixtures used in welding with fusible wire (GMAW) have an influenceon arc stability, the mode of metal transfer from the wire to the weld pool and thebead shape. They also determine the chemical exchanges in the arc and consequentlythe analysis of the deposited metal with a given wire.Operational aspects Arc stability is dependent on the more or less easy extraction of electrons fromthe cathode in order to maintain the arc. However, in MIG/MAG welding, it isactually the parts to be assembled which form the cathode. This is why, each time itis metallurgically acceptable, oxidizing gas mixtures are used, so as to form a fineoxide coating just in front of the arc which aids thermo-electronic emission [JON 95]. The metal transfer can take various forms depending on the parameters used: – with low welding currents, i.e. for low wire feed speeds, the metal transferfrom the wire to the weld pool is performed by short-circuit (short arc mode). Thearc periods are interrupted with periods during which the drop which was formed atthe end of the wire comes into contact with the weld pool. During this phase, the arcdies out and the current greatly increases which, via electromagnetic forces, initiallycauses a striction of the molten metal at the upper part of the drop, then itsdetachment. The arc can then be restored and the process started again; – with high currents (high wire feed speeds), the metal transfer takes place byaxial pulverization (spray arc). The end of the wire takes the shape of a cone fromthe point of which fine droplets are ejected in the wire axis, which are thentransfered towards the weld pool. The higher the current, the finer the droplets andthe greater their speed; – with intermediate currents, the transfer is known as globular. The drops whichare formed at the end of the wire grow bigger until reaching a diameter significantlyhigher than that of the wire and are detached in an erratic way before the short-circuit occurs. This mode, which is relatively unstable, is the origin of muchspattering. The welding current is thus a determining factor of the mode of transfer.Nevertheless, for a current compatible with transfer by short-circuit or by axialpulverization, it is possible to obtain a globular transfer by adjusting the voltage(very high voltage with low currents or very low voltage with high currents).
Welding Products 185 Generally, the various transfer fields can be represented in a diagram U = f (I), asin Figure 5.12. Figure 5.12. Modes of metal transfer according to MIG/MAG welding parameters In this figure, the points to be noted are the following: – the current Icc max, which corresponds to the maximum at which a transfer byshort-circuit is possible; – the right segment CC’ which delimits the maximum voltage value permittingthis type of transfer; in practice, welders regulate the voltage to a value slightlylower than this maximum (see shaded zone); – the current Is min., which corresponds to the minimum at which transfer byaxial pulverization can be achieved; – the segment SS’ indicates the minimum voltage at which a transfer by axialpulverization is observed, welders generally working with a slightly higher value; – the precise limits of these transfer fields in the diagram U = f (I) arecharacteristic of a given wire/gas combination. They change with the nature of theshielding gas but also with the wire diameter used: any addition of CO2 and/oroxygen in the argon increases the size of the globular field by decreasing Icc and byincreasing Is (see Figure 5.13) so that it is no longer possible to obtain a metaltransfer by axial pulverization as soon as the CO2 content exceeds 50% in the argon. In addition, an increase in wire diameter causes an increase in current Is, Iccremaining practically unchanged (see Figure 5.14).
186 Metallurgy and Mechanics of Welding Figure 5.13. Influence of O2 and CO2 content in argon on the size of the globular field in MAG welding (wire ER 70S3; 1 mm; distance of contact tube to part, 15 mm)Figure 5.14. Influence of wire diameter on the transfer fields in MAG welding (wire ER 70S3; gas: Ar + 3% CO2+ 1% O2; distance contact tube and contact/part, 15 mm) In addition to these three basic fields, a mode exists at very high currents whenwelds are made with a large gap from the contact tube to the part (>25 mm), wherethe transfer is rotary (rotating jet transfer or rotating spray) [LES 58, USC 93].Beyond a certain value of welding current, the cone which is formed at the end of
Welding Products 187the wire electrode becomes sufficiently long and malleable to curve in on itself androtate under the electromagnetic forces. The curve is more pronounced the higherthe current is and can even reach 90°, so that the molten metal drops which areejected according to the direction of the cone end then give rise to many spatters.This is undoubtedly the reason why this type of transfer has long been regarded asundesirable; nevertheless, as long as the curve remains slight, it can lead to animprovement in bead wetting and compactness because it is strongly dependent onthe shape of the penetration. The shape of the penetration is directly related to the mode of metal transfer. Inshort-circuit or globular mode, a lenticular penetration is observed which isexplained simply from the laws of heat propagation from the surface. On the otherhand, when the transfer is carried out by axial pulverization, the penetrationbecomes pointed. This is because the drops which are propelled at high speed in thewire axis cause a depression of the liquid bath at their impact point and impart amovement to it, which transfers heat towards the bead bottom. In this part of thebead, shaped like a glove finger, the solidification speed is much higher than in theremainder of the bead and when this is very deep, i.e. that at high welding currents,we often observe a lack of compactnesses such as blisters and shrinkage cavities areobserved (see Figure 5.15). On the other hand, the rotating transfer mode generallyleads to sound beads in spite of the very high currents employed, because the impactof the drops in the weld pool changes place permanently, so that round or even flatpenetration is found, which does not imply high solidification speeds.Figure 5.15. Morphology and compactness of beads created at high currents according to the mode of metal transfer: a) transfer by axial pulverization; b) rotating transfer The various fields which we have just described correspond to natural evolutionsin the metal transfer modes according to the current density in the wire electrode, thearc length (voltage) and its atmosphere; provided a simple voltage generator is usedfor welding. This causes some problems for the welder because these naturaltransfer modes are closely related to the energy employed which, in practice, cannot
188 Metallurgy and Mechanics of Weldingbe selected independently of the welding position and the type of joint envisaged.Thus, a current corresponding to the axial pulverization mode cannot be employedto weld in vertical or overhead positions because the weld pool would be too bulkyand would collapse. Thus, we must weld in the globular mode and accept the erratictransfer and the associated spatters, unless we reduce productivity considerably bylowering the current and welding in the short arc mode. To mitigate thesedisadvantages, and to a certain extent to dissociate the metal transfer mode from thecurrent and the welding voltage, certain generators employ electronics whichconstantly control the current in a very fast and precise way, so that the transfer ofthe drops can be regulated and controlled even for average values of the weldingcurrent and voltage which would naturally incline us to the globular mode. This iscalled the pulsed mode. For each average current and thus wire feed speed, thismode is characterized by a base current and time value, a peak current and timevalue as well as the ascending and descending slopes. The peak current must behigher than the minimum current allowing axial pulverization (Is in Figure 5.12), theother parameters being programmed so that only one metal drop transfers from thewire towards the weld pool in each cycle. This leads to a perfectly stable mode, freefrom spatters – provided of course that programming the various pulsed modeparameters is well adapted to the wire/gas combination. Recall that each wire/gascombination has “natural” transfer characteristics which are intrinsic to it. Generally, the same generators which are equipped with fast control electronicsare also able to preserve the short-circuit transfer mode for average current valueshigher than Icc in Figure 5.12. This is particularly advantageous when we want toweld at high speed, because it is possible to utilize a linear energy adapted to thetravel speed while preserving a very short arc, which is thus less likely to stall thanthe “natural” or pulsed arc corresponding to the same average current.Chemical aspects The analysis of a deposited metal is never identical to the analysis of a wireelectrode in welding under a gas flow with a fusible wire, because during theirtransfer in the arc, the metal drops on the surface reach boiling point. Thus, the morevolatile elements are vaporized more intensely than the others, which explains whythey are found in great quantities in welding fumes but are less prevalent in thedeposited metal than in the filler wire. Typically this is true of manganese in steels,magnesium in 5000 series alloys or zinc in brasses. In addition to this fractional distillation and independent of the weldingatmosphere, chemical reactions occur, especially at the level of the drops, when theshielding gas has some capacity for oxidation. The greater this oxidation capacity,the greater the analytical variations between the deposited metal and the wire, andthe more oxidable elements (Si, Mn, Al, Ti, etc.) occur as slag on the surface of the
Welding Products 189beads (see Figure 5.16). At the same time, the oxygen content of the deposited metaland the inclusion rate increase. Conventionally, the International Institute of Welding considers that theoxidation power of a shielding gas is equal to the sum of its oxygen content and halfof its CO2 content (Doc. IIS XII-543-77). The two graphs in Figure 5.16 show thatthis approach is very approximate since the losses of manganese and silicon aremuch greater than the IIS suggest with its comparison of argon-oxygen mixtures andargon-CO2 mixtures. In addition, depending on the percentage of carbon in the wireand of CO2 in the shielding gas, there will be a carburizing or decarburizing effect inaddition to its oxidizing effect. Thus, an argon mixture + 18% CO2 will becarburizing if the percentage of carbon in the wire is lower than 0.07% anddecarburizing above that value; for the same reason, we should not have more than1.5% of CO2 in the shielding gas if we hope to preserve the low carboncharacteristic (<0.03%) of an austenitic stainless steel weld (Figure 5.17). Figure 5.16. Chemical transfers according to the CO2 and oxygen content in the shielding gas
190 Metallurgy and Mechanics of WeldingFigure 5.17. Influence of CO2 content in the shielding gas on the percentage of carbon in the deposited metal depending on the transfer mode (ER308LSi wire with C=0.18%)Figure 5.18. Influence of nitrogen content of the shielding gas on the nitrogen content in the deposited metal (MIG welding); superduplex wire (N = 0.24%); two transfer modes Thus, for GMA welding as for welding with a solid flux, the chemicalcharacteristics of welds are not only related to the wire used but to the wire/fluxcombination. However, a difference exists. Whereas, depending on the solid fluxused, the deposit can be more or less rich in alloying elements than the filler wire, it